Recently, Ni-Al layered double hydroxides (LDHs) with hydrotalcite-like structure have shown outstanding performances in electrochemical field with their high specific capacitance, low cost

First of all, I would like to express my love to my dearest mother for her always unconditional love and support, particularly during my education years in France, it is with no doubt because of her high standard expectations for me if today I stand at this glamourous point in my life. My deepest love and appreciation to my late father, thinking about him at this moment of my life refreshes all the sweet memories of a joyful childhood I spend around him, may his soul rest in peace.

I would like to express my highest regards to my thesis supervisor, Dr Hubert Perrot, for his seriousness, kindness and full support during all the steps of this project from beginning to the end. Today, he is one of the pioneers of EQCM and fast electrogravimetric studies in the country and it was indeed a great honor to have him as my mentor. I will be always grateful for all that I have learned from him.

I am thoroughly grateful for the prosperous collaboration we had with Prof Farzaneh Arefi and Dr

Jerome Pulpytel, Plasma field specialists in LISE.

I am really thankful to Dr Christine Mousty (ICCF, Clermont University) for the fruitful collaboration we

had regarding the studies on layered double hydroxide (LDHs) materials.

I am indeed grateful to Dr Particia Beaunier for her high quality work and for all that I've learned from her in the field of surface classical characterization techniques (SAED, TEM, HR-TEM). I am thankful to: Dr Francois Huet (LISE) director, Mrs Francoise Pillier (LISE) SEM-FEG Microscopy, Mr Cyril Bazin (LISE) and Mr Benoit Baptiste (IMPMC lab) X-ray Diffractometry analysis, Dr Houssam Fakhouri (LISE) RF reactive Sputtering, Dr Catherine Debiemme-Chouvy (LISE) XPS analysis, Mrs Sandra Casale (LRS) HR-TEM, Mr Axel Desnoyers de Marbaix (LISE) Mecanicien, Mr Daniel Rose (LISE)

Electrician, Mrs Florence Billon (LISE) Engineer and Mrs Veronique Martin (LISE) documentalist.

During these three years of my PhD project I received the permanent kindness on the behalf of all my friends and colleagues, my kindest regards to Dr Mireille Turmine and Dr Vincent Vivier, my colleague

Freddy Escobar, PhD Students: Pierre, Marie S, Thomas, Azadeh, Larbi.

I am also thankful to Miss Marie Brel, our previous M1 student, with whom I have initiated the work on composite materials.

Lastly, I would like to thank all my other friends for their support, special thanks to my lovely sister Maryam.

IV

Table of Contents

General Introduction

During this thesis project, it was attempted to underline the importance of investigating the ion's exchange phenomena at the metal oxides electrode/electrolyte interface in order to understand and to furtherly improve their promised energetic performances mostly as highly functional electrodes for supercapacitors. Indeed, the key phenomena for all these electrodes functionalities originates in the ion's exchange at the interface of electrode/electrolyte, it is crucial to investigate the role of electrolyte composition, to identify the status of transferred ions and the solvation effect also to investigate their dynamics of transfer at the interface.

Consequently, we have decided to focus on the capabilities of a non-classical methodology socalled, ac-electrogravimetry.

Another subject of crucial matter for our attention was to illustrate the most fundamental reasons of the electrochemical improvements brought by nanostructuration. In fact, the materials structuration with favorable morphologies and unique properties would alter their functionalities and this can effectively be deeply characterized by ac-electrogravimetry.

Different morphologies of TiO2, WO3 and RuO2 metal oxides were prepared as furtherly detailed. As a consequent, during this thesis project, the investigations were performed to see what differences in behavior are brought by procuring porosity within these films. In other words, how mesoporous films with small pore sizes, and large surface area to volume ratios could facilitate the ion intercalation/electroadsorption process involved with our chosen synthesized MOx electrodes. More importantly it was attempted to see how acelectrogravimetry as a non-classical coupled methodology would be served for our study to extract fine dynamics details unreachable with classical tools. To pursue this major goal our results were systematically categorized as following:

 The first chapter provides a general look toward the highlighted aspects and applications Based on these methodologies the scope of this thesis project which underlines the importance of ac-electrogravimetry as our main chosen methodology is presented.

 The second chapter is dedicated to necessary theoretical and experimental basics commonly used during this thesis project. In the first part, the different components of the model used for ac-electrogravimetric fittings are introduced. It is shown how different ac-electrogravimetric transfer functions for an electroactive electrode system with responses to ions transfer are obtained. Another part is focused on the description of various structural and electrochemical characterization techniques applied as diagnostic tools to study the influence of the different electrochemical and physical preparation methods used for fabricating our MOx electrodes with different morphologies.

 The third chapter underlines the results obtained for different morphologies of amorphous non-porous and amorphous porous TiO2 deposited by reactive magnetron RF Sputtering. SEM-FEG accompanied with EDX analysis and HR-TEM were used for the structural studies. Both classical EQCM and then, ac-electrogravimetry were used in LiClO4 and NaClO4 aqueous medium to investigate the impact of a porous morphology and also identify and separate the contribution of the charged and/or uncharged species during the charge compensation process. A comparison is also made to understand the impact of accompanying solvent whether it is organic or aqueous.

 The fourth chapter includes the results obtained for electrochromic mesoporous WO3

prepared by surfactant-assisted electrodeposition. A comparison in behavior is made between the mesoporous electrode with the compact tungsten trioxide electrode fabricated by electrodeposition but in the absent of surfactant molecules. XPS, SEM-FEG, EDX analysis and HR-TEM were used for the primary structural studies. Then, classical EQCM and ac-electrogravimetry were used in LiClO4 aqueous medium to investigate the impact of the nanostructuration, and to identify/separate the contribution of the charged and/or uncharged species during the charge compensation process.

 The last chapter was dedicated to the results obtained for pseudocapacitive hydrous RuOx.nH2O films prepared in both compact and mesoporous morphologies via the same electrochemical route used for WO3 electrode preparation. The structure, the morphology and the composition of these electrodes were analyzed by XRD, XPS, TEM, SAED, HR-TEM and SEM-FEG. Both classical EQCM and acelectrogravimetric techniques were exploited to study the impact of structuration and the ions transfer behavior of the as-prepared compact and mesoporous hydrous RuOx.nH2O films in aqueous H2SO4 and Na2SO4. The second part of this chapter was attributed to the electrogravimetric investigations of CNTs/RuOx•nH2O in order to pursue the ion's kinetics evolution involved with a new 3D composite structure in aqueous H2SO4 electrolyte.

Résumé du Chapitre I

Ce chapitre fournit un état de l'art rapide en ce qui concerne les matériaux potentiellement utiles L'objectif majeur de ce projet de thèse est de mettre en valeur un outil de caractérisation alternatif afin de surmonter les limitations des EQCM classiques pour étudier les mécanismes d'électroadsorption/d'intercalation dans les électrodes associées aux systèmes pseudo-capacitif.

Cette méthode, dite d'électrogravimétrie à courant alternatif ou ac-électrogravimétrie est constituée d'un couplage entre la spectroscopie d'impédance électrochimique (EIS) et une microbalance à quartz rapide (QCM). Cette approche a été développée dans un nombre limité de laboratoires dans le monde.

Chapter I: Bibliography

This Chapter provides an introduction to the highlighted aspects and applications of materials with potential usefulness in energy storage devices, more importantly supercapacitors and/or micro-capacitors. First, the functionality of electrochemical supercapacitors and their main

I. Supercapacitors as Energy Storage Devices:

With the rapid development of the global economy, the depletion of fossil fuels, and increasing environmental pollution, there is an urgent need for efficient, clean, and sustainable sources of energy, as well as new technologies associated with energy conversion and storage. In many application areas, some of the most effective and practical technologies for energy conversion and storage are fuel cells and batteries/electrochemical supercapacitors. In recent years, electrochemical supercapacitors have attracted significant attention, mainly due to their high power density, long lifecycle, and bridging function for the power/energy gap between traditional dielectric capacitors (which have high power output) and batteries (which have high energy storage). The earliest electrochemical supercapacitors patent was filed in 1957.

However, not until the 1990s did electrochemical supercapacitors technology begin to draw some attention, in the field of hybrid electric vehicles. It was found that the main function of electrochemical supercapacitors could be to boost batteries or fuel cells in a hybrid electric vehicle to provide the necessary power for acceleration, with an additional function being to recuperate brake energy [1][2][3][4][5][6][7][8][9][10]. Further developments have led to the recognition that electrochemical supercapacitors can play an important role in complementing batteries or fuel cells in their energy functions by providing back-up power supplies to protect against power disruptions. As a result, the US Department of Energy has designated electrochemical supercapacitors to be as important as batteries for future energy storage systems. Many other governments and enterprises have also invested time and money into exploring, researching, and developing electrochemical supercapacitors technologies [1][2][3][4][5][6][7][8][9][10].

Recent years have yielded major progress in the theoretical and development of electrochemical supercapacitors, as evinced by a large number of research articles and technical reports [4][5][6][7][8][9][10].

At the same time, the disadvantages of electrochemical supercapacitors including low energy density and high production cost have been identified as major challenges for the furtherance of electrochemical supercapacitors technologies. To overcome the obstacle of low energy density, one of the most intensive approaches is the development of new materials for electrodes. Most popular today are carbon particle materials, which have high surface areas for charge storage. But in spite of these large specific surface areas, the charges physically stored on the carbon particles in porous electrode layers are unfortunately limited. Electrochemical Supercapacitors (ES) of this kind, called Electrical Double-Layer Supercapacitors (EDLS), have a limited specific capacitance (measured in Faraday per gram of the electrode material) and a low electrochemical supercapacitors energy density.

Advanced approaches to increase the ES energy density are to hybridize the electrode materials by adding electrochemically active materials to a carbon-particle-based ES electrode layer or to completely replace the carbon materials with another electrochemically active material. ES with electrochemically active materials as electrodes are called pseudo-supercapacitors [4]. It has been demonstrated that faradaic or hybrid double-layer supercapacitors can yield much higher specific capacitance and electrochemical supercapacitors energy density than EDLS.

Regarding advanced electrochemical supercapacitors materials, metal oxides such as ruthenium oxides and manganese oxides are considered the most promising materials for the next generation of electrochemical supercapacitors. Therefore, in this project we pay particular attention to metal oxides and their applications in electrochemical supercapacitors electrodes.

First, however, we provide some introductory background on electrochemical supercapacitors, which we hope will facilitate our review and analysis of the literature. Finally, we will discuss the direction that future research in electrochemical supercapacitors might be expected to take.

I-1. Basic principle of Electrochemical Supercapacitors

An electrochemical supercapacitor is a charge-storage device similar to batteries in design and manufacturing. As shown in Fig. I-1, an ES consists of two electrodes, an electrolyte, and a separator that electrically isolates the two electrodes. The most important component in an electrochemical supercapacitor is the electrode material. In general, the ES's electrodes are fabricated from nanoscale materials that have high surface area and high porosity. It can be seen from Fig. I-1 that charges can be stored and separated at the interface between the conductive solid particles (such as carbon particles or metal oxide particles) and the electrolyte. This interface can be treated as a capacitor with an electrical double-layer capacitance, which can be expressed as the following equation:

𝐶 = 𝐴𝜀 𝑑
where A is the area of the electrode surface, which for a supercapacitor should be the active surface of the electrode porous layer; 𝛆 is the medium (electrolyte) dielectric constant, which will be equal to 1 for a vacuum and larger than 1 for all other materials, including gases; and d is the effective thickness of the electrical double layer. Principles of a single-cell double-layer capacitor and illustration of the potential drop at the electrode/electrolyte interface [11].

As described in the Introduction, two types of ES exist. One is the EDLS, in which the electrode material, such as carbon particles, is not electrochemically active. In other words, there is no electrochemical reaction on the electrode material during the ES charging and discharging processes, and pure physical charge accumulation occurs at the electrode/electrolyte interface.

The other type is the faradaic supercapacitors, in which the electrode material is electrochemically active, e.g. metal oxides, which can directly store charges during the charging and discharging processes.

Two types of Electrochemical Supercapacitors

I. 1.1. Electrostatic supercapacitors

The capacitance of the electrode/interface in an electrostatic or EDLS is associated with an electrode-potential-dependent accumulation of electrostatic charge at the solid/electrolyte interface. As shown in Fig. I-1, this electrical double-layer capacitance comes from electrode material where an excess or a deficit of electric charges can be accumulated on the electrode side as electrolyte ions must counterbalance them on the electrolyte side in order to meet electroneutrality.

During the process of charge, the electrons travel from the negative electrode to the positive electrode through an external load. Within the electrolyte, cations move towards the negative electrode while anions move towards the positive electrode. During discharge, the reverse processes take place. In this type of supercapacitors, no charge transfer across the electrode/electrolyte interface is observed and no net ion exchanges occur between the electrode and the electrolyte.

I .1.2 Faradaic supercapacitors

Faradaic supercapacitors or pseudocapacitors are different from electrostatic or EDLS. When a potential is applied to a faradaic supercapacitor, fast and reversible faradaic reactions (redox reactions) take place on the electrode materials and involve the passage of charge across the interface, similar to the charging and discharging processes that occur in batteries, resulting in faradaic current passing through the supercapacitor cell. Materials undergoing such redox reactions include conducting polymers and several metal oxides, including RuO2, MnO2, or Co3O4. Three types of faradaic processes can occur at faradaic supercapacitors electrodes: direct electrochemical reactions it is a little beat confused as in EDLC it is electro adsorption (for example, adsorption of hydrogen on the surface of platinum or gold), redox reactions of transition metal oxides (e.g. RuO2), and reversible electrochemical doping-dedoping in conducting polymer based electrodes. It has been demonstrated that these faradaic electrochemical processes not only extend the working voltage but also increase the specific capacitance of the supercapacitors. Since the electrochemical processes occur both on the surface and in the bulk near the surface of the solid electrode, a faradaic supercapacitor exhibits far larger capacitance values and energy density than an EDLS. As reported by Conway et al. [11] the capacitance of a faradaic supercapacitors can be 10-100 times higher than the electrostatic capacitance of an EDLS. However, a faradaic supercapacitor usually suffers from relatively lower power density than an EDLS because faradaic processes are normally slower than nonfaradaic processes. Moreover, because redox reactions occur, faradaic supercapacitors often lack stability during cycling, similarly to batteries. It is worth mentioning that hybrid faradaic supercapacitors with an asymmetrical electrode configuration (e.g. one electrode consists of electrostatic carbon material while the other consists of faradaic capacitance

II. State of the Art of Different Types of Electrochemical Capacitors (ECs):

The most promising materials for electrochemical supercapacitors should utilize both the fast and reversible faradaic pseudocapacitance coming from the redox transitions of the interfacial electroactive species and the indefinitely reversible capacitance of electric double-layer formed at the electrolyte-electrode interface. Based on this point of view, the electrochemical supercapacitors can be considered as a hybrid device exhibiting transitional behavior between batteries and capacitors. Potential candidates of electrodes should be consisted of electroactive materials with very high surface areas, which prosecute the fast reversible redox transitions in the potential window of charge and discharge.

ECs are intermediate systems between dielectric capacitors and batteries. While batteries able to store higher energy density than supercapacitors, they deliver less power; as compared to dielectric capacitors, supercapacitors can store higher energy density with less delivered power.

These particular properties make them suitable for numerous applications such as power electronics, spatial or military field; they can also be used in hybrid electric vehicle in order to help the stop and go function, to provide peak power for improved acceleration, for energy recovery.

Three main classes of supercapacitors are described in the literature: metal oxide [12][13][14][15][16][17][18][19][20][21][22],

electronically conducting polymer [23][24][25][26][27][28][29][30] and Carbon/Carbon supercapacitors [31,[32][33][34][35][36][37]. Recently, hybrid supercapacitors have been developed where an activated carbon electrode is associated with a faradic electrode [38][39][40][41][42][43][44][45][46][47][START_REF] Bi | Highly dispersed RuO2 nanoparticles on carbon nanotubes: facile synthesis and enhanced supercapacitance performance[END_REF][START_REF] Su | RuO2/activated carbon composites as a positive electrode in an alkaline electrochemical capacitor[END_REF][START_REF] Wang | Hydrous ruthenium oxide nanoparticles anchored to graphene and carbon nanotube hybrid foam for supercapacitors[END_REF][START_REF] Leng | Hydrothermal synthesis and pseudo capacitance behavior of a highly homogeneous dispersed graphene sheets/ruthenium oxide nanocomposite[END_REF][START_REF] Zhou | Amorphous RuO2 coated on carbon spheres as excellent electrode materials for supercapacitors[END_REF][START_REF] Cormier | Temperature-dependent structure and electrochemical behavior of RuO2/carbon nanocomposites[END_REF].

II-1. EC based on Carbon materials:

Carbon/Carbon supercapacitors have been largely investigated because of their low-cost, high cycling-life and high capacitance. Small (few farads) up to large-size (5000 F) devices are commercially available (Maxwell, Epcos, Panasonic, etc.). Highly-porous carbons are used as electrode material due to their high surface area, good electronic conductivity and high electrochemical stability; the most frequently used is activated carbon (1500-2000 m 2 g -1 ).

Charge storage is performed through the reversible electro adsorption of the ions at the active material/electrolyte interface; no faradaic reactions occur during the charge-discharge of the supercapacitor [START_REF] Portet | High power density electrodes for carbon supercapacitor applications[END_REF].

Carbon materials, such as activated carbons (ACs) and carbon nanotubes (CNTs) (Fig 2D, two-dimensional; 3D, three-dimensional [10].

The most recent advances in supercapacitor materials include the development of nanoporous carbons with the pore size tuned to fit the size of ions of the electrolyte with Ångström accuracy.

In a recent review by P. Simon and co-workers [START_REF] Daffos | Recent advances in understanding the capacitive storage in microporous carbons[END_REF] it was attempted to achieve an improved understanding of charge storage and ion desolvation in sub-nanometer pores. It has also stressed the requirement of matching the active materials with specific electrolytes and the need to use a cathode and anode with different pore sizes. The very large number of possible active materials and electrolytes requires better theoretical guidance for the design of more powerful and long-lasting EDLCs (Fig. I-4). J Tang et al. [START_REF] Tang | Three-Dimensional Nitrogen-Doped Hierarchical Porous Carbon as an Electrode for High-Performance Supercapacitors[END_REF] synthesized of nitrogen-doped hierarchical porous carbons and by this way a three-dimensional interconnected framework (NHPC-3D) was developed (Fig. I-5). This device showed a high capacitance retention of 75,7% at a higher current density of 20 Ag -1 in aqueous electrolyte. This value is due to a sufficient surface area for charge accommodation, reversible pseudocapacitance, and a minimized ion-transport resistance, as a result of the advantageous interconnected hierarchical porous texture.

II-2. Pseudocapacitive oxide materials

In energy sources, there is a need, particularly with transportation and grid storage applications, of a large amounts of energy delivered quickly, within seconds or minutes. Although carbon based electrochemical capacitors possess the required power density, their relatively low energy density limits their usefulness for these applications.

II. 2. 1. WO 3

Tungsten oxides are great electrochemically active materials for energy storage. They have intriguingly fast and reversible surface redox reactions, which is associated with the similar W-O bond lengths in tungsten oxides with different oxidation states. Furthermore, the intrinsic high densities of tungsten oxides show potential applications in the fabrication of compact devices with excellent power performance. Theoretically, tungsten oxides are formed by corner and edge sharing of the WO6 octahedra. By ordered stacking of WO6 octahedra, a considerable number of interstitial sites can be formed. Such interstitial sites are effective accommodations for guest ions, rendering the absorption and desorption of ions at the surface, as well as insertion and deinsertion into the inner parts [START_REF] Zhu | Proton-insertion-enhanced pseudocapacitance based on the assembly structure of tungsten oxide[END_REF]. In a recent paper by M. Zhu et al. [START_REF] Zhu | Proton-insertion-enhanced pseudocapacitance based on the assembly structure of tungsten oxide[END_REF], it is reported that proton insertion, a faradaic mechanism, may effectively enhance the global capacitance of metal oxides with low surface area but Recently, J. Xu et al. [START_REF] Xu | Tungsten oxide nanofibers self-assembled mesoscopic microspheres as high-performance electrodes for supercapacitor[END_REF] reported on the fabrication of WO3 mesoscopic microspheres composed of nanofibers and prepared via a hydrothermal process (Fig. I-7). Then, an asymmetric supercapacitor was constructed using these as-prepared WO3 mesoscopic microspheres as positive electrode and an activated carbon as negative electrode. The favorable electrochemical performances are attributed to the mesoscopic structure of the WO3 which consist of a self-assembled interconnected WO3 nanofibers framework. Thus, films have open porous characteristics and abundant active sites accessible to charge storage leading to high specific capacitance of 797 F g -1 at a current density of 0,5 A g -1 . The specific capacitance reported by author is much higher than that of tungsten oxide materials. Nano-WO3.H2O/MnO2 was synthesized on Ti/RuO2+TiO2 substrate via anodic electrodeposition by C. Yuan et al. [START_REF] Yuan | Anodic deposition and capacitive property of nano-WO3•H2O/MnO2 composite as supercapacitor electrode material[END_REF]. The advantageous aspects of this new nanostructure is firstly related to good electron conduction of the nano-WO3-H2O due to MnO2. In their study, tungsten oxide had a conductivity of 1,76 S cm -1 which is several orders of magnitude higher than that of MnO2 (10 -5 -10 -6 S cm -1 ). Secondly, thin layer of MnO2 on each nanosheet enables fast faradic reaction and provides a short ion diffusion path and therefore improved capacitive performance, finally, the porous structure can create channels for effective transport of electrolyte and consequently increase electrochemical active sites. The high rate performance is mainly due to the coexistence of high ionic and electronic conductivity in the hierarchical h-WO3•nH2O crystal structure. Besides the high mass-, area-, and volumetric-specific capacitances and extraordinarily fast charge/discharge kinetics, the unique hierarchical nanostructure with proton-conducting channels also endows the h-WO3•nH2O with outstanding cycling stability.

II. 2. 2. TiO 2

Using TiO2 anatase nanosheets interfaced with lithium ion-containing electrolytes as an example, J Kang et al. [START_REF] Kang | First-principles theory of electrochemical capacitance of nanostructured materials: Dipole-assisted subsurface intercalation of lithium in pseudocapacitive TiO2 anatase nanosheets[END_REF] revealed a microscopic mechanism for lithium intercalation in this system. They have demonstrated that a TiO2 nanosheet is a hybrid between supercapacitor and battery, possessing characteristics of both depending on the electrode potential. At positive electrode potential above 2.2 V versus Li/Li + , the system behaves as a capacitor with the formation of electric double layers at the surface. As the electrode potential decreases below the threshold, lithium intercalation into the interior takes place. Their findings provide a coherent picture of how a transition from pure capacitors to batteries or pseudocapacitors occurs in these nanostructured materials.

In another work by T. Brezesinski et al. [START_REF] Brezesinski | Templated nanocrystalbased porous TiO2 films for next-generation electrochemical capacitors[END_REF], the considerable enhancement of the electrochemical properties of self-organized TiO2 results are shown when the films are both made from nanocrystals and mesoporous structures. Such materials show high levels of capacitive charge storage and high insertion capacities. When nanocrystal-based films are formed without mesoscale porosity, a high fraction of the total stored charge is again capacitive, but the total capacity is low, likely because most of the film is not accessible to the electrolyte/solvent. By contrast, when mesoscale porosity is created in a material with "dense" walls (rather than porous walls derived from the aggregation of nanocrystals), insertion capacities comparable to templated nanocrystal materials can be achieved, but the capacitance is much lower. These results underscore the importance of pseudocapacitive behavior which is developed in high surface area mesoporous oxide films. Moreover, the data suggest that both a mesoporous morphology and the use of nanocrystals as the basic building blocks are very promising for the rational development of metal oxide pseudo/supercapacitors. Through this combination, it may become possible to attain greater power densities while maintaining energy density in the next-generation of electrochemical capacitors that utilize this bimodal nanoporous architecture.

X. Sun et al. [START_REF] Sun | Pseudocapacitance of amorphous TiO2 thin films anchored to graphene and carbon nanotubes using atomic layer deposition[END_REF] fabricated pseudo supercapacitors by depositing amorphous TiO2 thin films onto the surface of both graphene and CNT samples by atomic layer deposition (ALD). An ultrathin Al2O3 adhesion layer was employed to obtain conformal and amorphous TiO2 films.

The electrochemical characteristics of TiO2 films in 1 M KOH electrolyte were then determined using a variety of techniques including cyclic voltammetry, galvanostatic charge/discharge curves, and electrochemical impedance spectroscopy. The relatively low electrical conductivity and ionic diffusivity of TiO2 did not limit these measurements because the TiO2 films were ultrathin. The pseudocapacitance of the TiO2 films greatly exceeded the electric double layer capacitance of the uncoated graphene and CNT samples. The measurements determined that the specific capacitances of the TiO2-coated graphene and CNT samples were 97,5 and 135 F g -1 , respectively, after 50 TiO2 cycles at 1 A g -1 . An asymmetric cell was also developed based on TiO2 ALD coated CNT samples as the positive electrode and uncoated CNT samples as the negative electrode. This energy storage device could be reversibly operated over a wide voltage range of 0-1,5 V in aqueous electrolyte. A high energy density of 4,47 W•h kg -1 was achieved on the basis of the total weight of both electrodes. This energy density was ∼4 times higher than the symmetric CNT cell. The TiO2 ALD-coated G and CNT electrodes and the asymmetric cell based on the TiO2 ALD coated electrode also exhibited excellent stability over >1000

cycles. The results of this study demonstrate that metal oxide on high surface area conducting substrates can be used to fabricate high energy storage supercapacitors.

II. 2. 3. MnO 2

The pseudocapacitive behavior of MnO2 was first investigated in 1999 by Lee and Goodenough [START_REF] Zhu | Oxidationetching preparation of MnO2 tubular nanostructures for high-performance supercapacitors[END_REF][START_REF] Brousse | To be or not to be pseudocapacitive?[END_REF][START_REF] Zhang | Microwave-assisted reflux rapid synthesis of MnO2 nanostructures and their application in supercapacitors[END_REF][START_REF] Hu | Facile chemical synthesis of nanoporous layered δ-MnO2 thin film for high-performance flexible electrochemical capacitors[END_REF] as they studied the properties of amorphous MnO2.nH2O in a KCl aqueous electrolyte.

The presence of a rectangular voltammogram and the storage of approximately 200 F g -1 (240 C g -1 , 4 min) indicated that rapid faradaic reactions were responsible for charge storage in this material.

Q Qu et al. [START_REF] Qu | Electrochemical Performance of MnO2 Nanorods in Neutral Aqueous Electrolytes as a Cathode for Asymmetric Supercapacitors[END_REF] investigated the electrochemical behavior of MnO2 nanorods prepared from a precipitation reaction in 0,5 mol L -1 Li2SO4, Na2SO4, and K2SO4 aqueous electrolytes (Fig. I-11). The MnO2 nanorods show the superior rate behavior in the K2SO4 electrolyte due to the smallest hydrated radius of K + , highest ionic conductivity, and smallest equivalent series resistance. Moreover, the initial cycles could be an effective way to activate the MnO2 electrode and make the electrolyte solution soak into the material surface completely. The assembled asymmetric AC/K2SO4/MnO2 nanorods supercapacitor shows an excellent cycling behavior between 0 and 1,8 V and also exhibits a large energy density of 17 Wh kg -1 at a power density of 2 kW kg -1 . of the Ru 4+ atoms participated in the redox reaction), it demonstrated the unique electrochemical features of pseudocapacitive processes. This study also demonstrated the need for a porous and hydrous oxide as the bulk, single-crystal material did not exhibit a rectangular CV. Subsequent studies improved the capacitance to over 700 F g -1 by identifying the importance of structural water (specifically, RuO2 nH2O where x=0.5) and a porous, nanoscale architecture [27]. RuO2 0,5H2O exhibits four unique features that enable rapid faradaic reactions with high capacitance:

(1) the redox behavior of the Ru 4+ cation that allows for faradaic energy storage; (2) the metallic conductivity of RuO2 that allows for rapid electron transport; (3) the presence of structural water that enables rapid proton transport within the so-called "inner surface"; and (4) a large "outer" surface area that decreases diffusion distances. Unfortunately, the high cost of ruthenium In a galvanostatic experiment, the shape is sloping so that a capacitance value, dQ/dE, may be assigned at each point, and the voltage hysteresis is small. Here, Q is the capacity and E is the potential window. (c) In an AC impedance experiment, the Nyquist representation will contain a vertical line with a phase angle of 90° or less. A semi-circle at high frequencies, associated with charge-transfer resistance, may also be present [27].

Both amorphous and microcrystalline ruthenium oxides have been employed as electrode materials for the EC supercapacitors although ruthenium is a noble metal. The kinetics of electron transfer and/or the diffusion of protons within the electroactive materials determined the reversibility of redox transitions. An integration relating the electrochemical characteristics and textural properties to their preparation methods are very important in searching and optimizing the suitable materials for the application of EC supercapacitors [START_REF] Hu | Design and tailoring of the nanotubular arrayed architecture of hydrous RuO2 for next generation supercapacitors[END_REF][START_REF] Hu | Effects of preparation variables on the deposition rate and physicochemical properties of hydrous ruthenium oxide for electrochemical capacitors[END_REF][START_REF] Hu | Cyclic voltammetric deposition of hydrous ruthenium oxide for electrochemical supercapacitors: effects of the chloride precursor transformation[END_REF]. Even though RuO2 has a great advantage in terms of attractive high specific capacitance, it is somewhat expensive for commercial electrochemical capacitors. However, if one would be able to develop a thin film process for preparing RuO2 electrode, this would reduce significantly the cost of these electrodes.

Hu et al. [START_REF] Hu | Cyclic voltammetric deposition of hydrous ruthenium oxide for electrochemical supercapacitors: effects of the chloride precursor transformation[END_REF] produced nanotubular hydrous RuO2 electrodes using the anodized aluminium oxide (AAO) membrane template and showed a specific capacitance of 1300 Fg -1 . Zheng et al.

[71] synthesized hydrous RuO2 films through a sol-gel process and showed specific capacitance depending on hydrate species contents and surface area. A maximum specific capacitance of 720 Fg -1 was obtained for RuO2•0,5H2O with a surface area of 68,6 m 2 g -1 . Suh et al. [START_REF] Suh | Synthesis of high-surface-area ruthenium oxide aerogels by non-alkoxide sol-gel route[END_REF] produced high surface area RuO2 aerogels of 350 m 2 g -1 with the high hydrate contents of RuO20.5H2O by carbon dioxide supercritical drying method and showed a specific capacitance of 595 Fg -1 . Subramanian et al. [START_REF] Subramanian | Mesoporous anhydrous RuO2 as a supercapacitor electrode material[END_REF] prepared the mesoporous anhydrous crystalline RuO2 by using nonionic surfactant template and achieved a specific capacitance of 58 Fg -1 . In RuO2 as a pseudocapacitor, in which both electrons and cations have to be transported, facile transport paths for both types of carriers should exist. Anhydrous RuO2 has the rutile structure and is composed of RuO6 octahedra in the three-dimensional structure, the ordering of RuO6 octahedra is able to promote electron transport, but not cation transport. However, hydrous RuO2 may comprise the chains of disordered RuO6 octahedra and exhibit the three-dimensional disorder, which is able to promote cation transport, but less electron transport. Therefore, pseudocapacitance should be optimized and increased when the hydrated contents and ordered RuO6 octahedra in amorphous RuO2 are balanced. The control of the hydrated contents of (RuO2•xH2O) in the porous nanoarchitectures of RuO2 is an important parameter to obtain a high specific capacitance.

In a recent study in this regard, H-S Nam et al. [START_REF] Nam | Electrochemical capacitance of nanoporous hydrous RuO2 templated by anionic surfactant[END_REF] proposed a new process for preparing nanoporous and hydrous RuO2 using sodium dodecyl sulfate (SDS) at a low temperature below

II-3. Conducting Polymers:

Generally, ECs performance is considered in specific capacitance which either can be estimated from the cyclic-voltammogram or from the discharge measurement. Each class of materials has its unique advantages and disadvantages. Some of the transition-metal oxides suffer from poor electrical conductivity and high cost. On the other hand, conducting polymers are highly conducting, can follow easy synthesis process, are associated to fast rate of redox transfer and present low cost, etc. But their poor cycle life and low mechanical stability are major barriers for practical applications. Therefore, many studies have recently been addressed to increase their electrochemical performances [24][25][26][27]31].

Various research groups are trying to investigate a hybrid nanostructure containing RuO2 and conducting polymers such as polyaniline, polypyrrole etc., for ECs application. Employing template-free anodic deposition of cone-shaped nanostructure of polypyrrole with ultrathin layer of RuO2, a specific capacitance of 302 Fg -1 has been reported. Polyaniline/nafion/hydrous RuO2 ternary composite electrode has demonstrated a 475 Fg -1 specific capacitance at 100 mV s -1 [24][25][26][27]31].

In recent years, polypyrrole (PPy), an important conducting polymer, has been successfully employed as redox electrode material. The specific capacitance of PPy has been measured to be 180-250 Fg -1 . In spite of its high charge storage capacitance, PPy and other conducting polymers lack in long-term stability [24][25][26][27][28][29][30][31].

In a report from F. Tran-Van's group, the capacity of chemically synthesized PPy, as well as its stability during cycling was optimized. In their work [28,29] polymerization of pyrrole is performed in a colloidal solution of Fe2O3 and in the presence of PTS anions. In this conditions, improvements are reached in terms of the charge storage capacity of the material. This is attributed to a morphological modification of the composite. Nanoparticles role as a support to the polymerization process of pyrrole and eventually this leads to a more porous structure with a higher specific surface area. By this way, it increases the accessibility of the conducting polymer sites during the electrochemical process. As a consequence, the kinetics of charge transfer is altered amplified in this nanocomposite structure. The insertion-extraction of anions during the charge-discharge process was reported to be easier and it may allow higher rates of charge-discharge and higher power density to be obtained. S. F. Shaikh et al. [25] reported on the superior electrochemical supercapacitive performance of hybrid structure over organic and inorganic structures (Fig. decreases. This is attributed to the diffusion limitation in the WO3 dense film. Due to the distribution of WO3 in the PANI network, WO3/PANI composite displays only a minor decrease in the specific capacitance, with the mass of film increasing from 2,4 to 8,1 mg. This implies that the pseudocapacitive reaction takes place not only at the surface but also in the bulk of the film.

Fig. I-14.

The specific capacitance of PANI, WO3 and the composite WP as a function of the film mass measured through constant current charge-discharge at 1 Ag -1 in 1M H2SO4 [START_REF] Zhu | Oxidationetching preparation of MnO2 tubular nanostructures for high-performance supercapacitors[END_REF].

In a reported work by J. Zang et al. [24] a well-aligned cone-shaped nanostructure of PPy was successfully grown on Au substrate by using a simple, one-step, cost-effective, template-free, and anodic deposition method. Furthermore, the 3D, arrayed, nanotubular architecture coated with an ultrathin layer of RuO2 was tailored to construct a supercapacitor. The unique structure and design not only reduces the diffusion resistance of electrolytes in the electrode material but also enhances its electrochemical activity. The specific capacitance and conductivity of RuO2/PPy by the modification with an ultrathin layer of RuO2 was significantly improved in comparison to that of the bare PPy, which was verified by CVs and EIS for the two electrodes.

The good stability of the RuO2/PPy electrode is very promising for applications in microsupercapacitor devices.

II-4. Carbon-MO x Composites:

Owing to their high conductivity, permeability (resulting in high power density) and chemical inertness (long cycle lifetime), single wall carbon nanotube (SWCNT) thin films are promising candidates for active supercapacitor electrode materials [START_REF] Tang | Three-Dimensional Nitrogen-Doped Hierarchical Porous Carbon as an Electrode for High-Performance Supercapacitors[END_REF][START_REF] Taberna | Activated carbon-carbon nanotube composite porous film for supercapacitor applications[END_REF]. In nanocomposite form, metal oxides and conducting polymers could improve electrochemical and mechanical properties of the supercapacitors. Therefore, recent researches has been focused on the exploration of potentiel pseudocapacitive metal oxides have been investigated [44][45][46][47][START_REF] Bi | Highly dispersed RuO2 nanoparticles on carbon nanotubes: facile synthesis and enhanced supercapacitance performance[END_REF][START_REF] Su | RuO2/activated carbon composites as a positive electrode in an alkaline electrochemical capacitor[END_REF][START_REF] Wang | Hydrous ruthenium oxide nanoparticles anchored to graphene and carbon nanotube hybrid foam for supercapacitors[END_REF][START_REF] Leng | Hydrothermal synthesis and pseudo capacitance behavior of a highly homogeneous dispersed graphene sheets/ruthenium oxide nanocomposite[END_REF][START_REF] Zhou | Amorphous RuO2 coated on carbon spheres as excellent electrode materials for supercapacitors[END_REF][START_REF] Cormier | Temperature-dependent structure and electrochemical behavior of RuO2/carbon nanocomposites[END_REF][START_REF] Peng | High-performance aqueous asymmetric supercapacitor based on carbon nanofibers network and tungsten trioxide nanorod bundles electrodes[END_REF][START_REF] Ma | Hydrothermal preparation and supercapacitive performance of flower-like WO3•H2O/reduced graphene oxide composite[END_REF][START_REF] Wang | Dispersing WO3 in carbon aerogel makes an outstanding supercapacitor electrode material[END_REF].

R. Yuksel et al. [START_REF] Yuksel | Ternary nanocomposite SWNT/WO3/PANI thin film electrodes for supercapacitors[END_REF] have recently reported on the fabrication of ternary nanocomposite SWCNT/WO3/PANI thin films as supercapacitor electrodes. High electrical conductivity of SWCNT thin films allowed the possibility of the fabrication of supercapacitors without a separate charge collector and enhanced the properties solely arised by the WO3 and PANI components in a synergistic manner. These fabricated ternary nanocomposite supercapacitor electrodes were found to have a specific capacity of 28.5 mF/cm 2 at a current density of 0.13 mA/cm 2 therefore they could be promising electrode active materials for electrochemical energy storage systems if an air-stable conducting polymer can be integrated into the structure.

In a study by A Eftekhari et al. [38,39], manganese oxide films were galvanostatically deposited in the presence of a small amount of carbon nanotube (CNT). The resulting film cannot be considered as a CNT based nanocomposite, as no CNT is detected by electron microscopy.

However, the manganese oxide electrodeposited delivers an excellent pseudo-capacitive behavior to be used as a superior supercapacitor. The samples showed a specific capacitance of 280 F g -1 . As it seems that the capacitance of this electrode is related to the chemisorption of the alkali cation, an extremely high specific capacitance of 434 F g -1 was achieved in a saturated medium of Li electrolyte. This high specific capacitance can be attributed to the presence of carbon nanotubes results in the formation of nanostructured films which provide a better ion accessibility. Although the exact mechanism for this phenomenon is still vague, the presence of carbon nanotubes (probably as a solid charge carrier) close to the electrode surface is apparently responsible for a different pathway for the electrodeposition process.

Graphene has also been considered as a promising candidate for a supercapacitor electrode material due to its attractive characteristics such as large surface area, good flexibility, excellent electrical conductivity and wide potential windows.

III. Strategies Toward New Ways of Materials Design for High Performance ECs

III. 1. Elaboration Methods and Process

S. Music et al. [START_REF] Musić | Influence of synthesis procedure on the formation of RuO2[END_REF][START_REF] Musić | Synthesis and characterization of nanocrystalline RuO2 powders[END_REF] presented a new route in the synthesis of RuO2 powder. This synthesis is based on the addition of strong organic alkali, tetramethylammonium hydroxide, into an alcoholic solution of RuNO(NO3)3 and thermal treatment of amorphous ruthenium hydrous oxide, previously precipitated at 90 °C. They have also investigated conditions for the precipitation of amorphous ruthenium hydrous oxide in water medium at high pH. Similarly reported by U. M. Patil et al. [START_REF] Patil | Chemically synthesized hydrous RuO2 thin films for supercapacitor application[END_REF], the amorphous hydrous RuO2 thin films have been successfully synthesized at low temperature on glass and stainless steel substrates using chemical bath deposition (CBD) method which is single step, simple, easy, and efficient. SEM images reveal that porous and spherical grained morphology of their synthesized films. The equivalent series resistance, ESR, power corresponding to heat production due to internal resistance and higher loss factor of hydrous RuO2 thin film, restricts maximum specific capacitance up to the 73 F g -1 . The specific power, specific energy and coulombic efficiency (%) of the prepared electrode is found to be 0,151 kW kg -1 , 3,57 Wh kg -1 and 94%, respectively.

G-H Jeong et al. [19] reported on the synthesis of porous ZrO2-SiO2 sheets with well-defined ultrasmall WO3 nanoparticles for energy storage performance. To overcome relatively low surface areas in binary composites, they have synthesized a new ternary oxide system of porous ZrO2-SiO2 sheets with ultrasmall WO3 NPs as shown in figure I-16. Therefore, in their system, ultrasmall WO3 NPs are synthesized on porous ZrO2-SiO2 sheets by an impregnation process. The advantageous aspect of their work is the utilization of WO3 NPs as a real active material for capacitance generation which was greatly enhanced by distributing WO3 NPs on the framework wall. The synthesized electrode with about 13 nm thickness and about 10 nm pores, has a maximum capacitance value of 313 F g -1 at a current density of 1 A g -1 and a minimum value of 160 F g -1 at a current density of 30 A g -1 .

In a report from T.P. Gujar et al. [START_REF] Gujar | Spray deposited amorphous RuO2 for an effective use in electrochemical supercapacitor[END_REF] network like amorphous RuO2 electrodes were synthesized successfully by spray pyrolysis method. The specific capacitance of RuO2 electrode decreased with an increase of scan rate and a maximum capacitance 551 F g -1 was observed at 5 mV s -1 . According to their work the spray pyrolysis method is useful for preparation of large area RuO2 electrodes with amorphous structure for supercapacitive applications at the expense of small amount of initial ingredients.

Y-Y Liang et al. [START_REF] Liang | Solid state synthesis of hydrous ruthenium oxide for supercapacitors[END_REF] have successfully developed a novel solid state synthetic route for the preparation of mesoporous hydrous ruthenium oxide. The efforts in this work have been focused on exploring the relationships among the annealing conditions, structural changes and the electrochemical performances. Combined with the existing results, it was found that the specific capacitance of RuO2•xH2O is strongly dependent on the corresponding crystalline structure.

Based on their results the high value of specific capacitance can be obtained only from the amorphous phase, once the crystalline phase was formed, the specific capacitance dropped rapidly. For example, a maximum capacitance of 655 F g -1 was obtained by annealing at 150 • C, higher temperatures (exceeding 175 • C) presumably contributed amorphous phase of RuO2•xH2O into crystalline one and the corresponding specific capacitance dropped rapidly from 547 F g -1 at 175 • C to 87 F g -1 at 400 • C.

There are also many examples of MOx preparation in the literature based on sol-gel route [START_REF] Sassoye | Block-Copolymer-Templated Synthesis of Electroactive RuO2-Based Mesoporous Thin Films[END_REF][START_REF] Sassoye | A sustainable aqueous route to highly stable suspensions of monodispersed nano ruthenia[END_REF][START_REF] Liu | A sol-gel process for fabrication of NiO/NiCo2O4/Co3O4 composite with improved electrochemical behavior for electrochemical capacitors[END_REF]. In a work by J.P. Zheng et al. [START_REF] Zheng | Hydrous ruthenium oxide as an electrode material for electrochemical capacitors[END_REF] a specific capacitance of 768 F g -1 has been obtained from an amorphous hydrous ruthenium oxide prepared by sol-gel method. MWCNTs coated with RuO2 have been fabricated on a noble stainless steel substrate by M. Kahram et al. [START_REF] Kahram | Synthesis and electrochemical characterization of sol-gel-derived RuO2/carbon nanotube composites[END_REF].

Structure and composition analyses by their group was based on the effects of film preparation parameters such as pH, the concentration of the sol and the heat treatment temperature.

The electrodeposition of various metal oxides is also a strategy of growing interest [START_REF] Hu | Design and tailoring of the nanotubular arrayed architecture of hydrous RuO2 for next generation supercapacitors[END_REF][START_REF] Hu | Effects of preparation variables on the deposition rate and physicochemical properties of hydrous ruthenium oxide for electrochemical capacitors[END_REF][START_REF] Hu | Cyclic voltammetric deposition of hydrous ruthenium oxide for electrochemical supercapacitors: effects of the chloride precursor transformation[END_REF]

III-2. Materials Nanostructuration for Development of Flexible Device Architectures:

For the improvement of the performance of metal oxide based electrodes, main attention has been attributed to their nanostructuration with various morphologies due to the unique properties and functionalities that can be effectively exploited in electrochemical energy storage devices [START_REF] Wang | A review of electrode materials for electrochemical supercapacitors[END_REF]. The new nanostructures, with small sizes, and large surface area to volume ratios, are expected to facilitate the ion transfer process which is the key phenomena in all energy storage devices including electrodes for supercapacitors. These improvements are attributed to (i) a facilitated transfer and short diffusion length for ions transport, (ii) a high electrode/electrolyte contact area, and (iii) a better stress/strain management of the material during ion intercalation/extraction. As a consequent of these advantages various synthesis methods some of them mentioned in the previous section could provide tremendous possibilities in order to have favorable new nanoarchitechtures for ideal electrode materials. The following part brings few examples of these efforts in order to procure materials with large surface areas. 18). Therefore, high specific capacitance of 740 F g -1 for the as-deposited RuO2.xH2O NTs is obtained. The great performance is reasonably attributed to the novel nanotubular arrayed structure of RuO2.xH2O, which not only reduces the diffusion distance of protons but also increases the facility of ion transportation during the rapid charge/discharge reactions. In addition, the metallic conductivity of annealed, crystalline RuO2.xH2O NTs provides the "superhighways" for electron motion.

Brzezinski et al. [START_REF] Brezesinski | Templated nanocrystalbased porous TiO2 films for next-generation electrochemical capacitors[END_REF] showed that considerable enhancement of the electrochemical properties of self-organized TiO2 results when the films are both made from nanocrystals and mesoporous.

Such materials show high levels of capacitive charge storage and high insertion capacities.

When nanocrystal-based films are formed without mesoscale porosity, a high fraction of the total stored charge is again capacitive, but the total capacity is low, likely because most of the film is not accessible to the electrolyte/solvent. By contrast, when mesoscale porosity is created in a material with "dense" walls (rather than porous walls derived from the aggregation of nanocrystals), insertion capacities comparable to templated nanocrystal materials can be achieved. These results underscore the importance of pseudocapacitive behavior developed with high surface area of mesoporous oxide films. Moreover, the data suggest that both a mesoporous morphology and the use of nanocrystals as the basic building blocks are very promising for the development of metal oxide pseudo/supercapacitors. Through this combination, it may become possible to attain greater power densities while maintaining energy density in next-generation electrochemical capacitors that use this bimodal nanoporous architecture [START_REF] Sun | Pseudocapacitance of amorphous TiO2 thin films anchored to graphene and carbon nanotubes using atomic layer deposition[END_REF].

In another work by R B Rakhi et al. [17], they have demonstrated that the rate performance of mesoporous Co3O4 nanosheet arrays grown directly over carbon cloth collectors can be improved by the uniform dispersion of hydrous RuO2 nanoparticles. The Co3O4/RuO2 nanostructured electrode morphology was tuned by controlling the electrodeposition time to achieve a balance between good electrode conductivity and efficient electrolyte access to the RuO2 nanoparticles, hence optimizing performance. A high specific capacitance value (905 F g -1 at 1 A g -1 ), high rate performance of 78% at the current density ranging from 1 to 40 A g -1 , and excellent cycling stability (96% after 5000 charge discharge cycles) were achieved using symmetric two-electrode configuration. Mesoporous cobalt oxide (Co3O4) nanosheet electrode arrays are directly grown over flexible carbon paper substrates using an economical and scalable two-step process for supercapacitor applications. The interconnected nanosheet arrays form a three-dimensional network with great supercapacitor performance in standard two electrode configuration. Dramatic improvement in the rate capacity of the Co3O4 nanosheets is achieved by electrodeposition of nanocrystalline, hydrous RuO2 nanoparticles dispersed on the Co3O4 nanosheets. As a result, an excellent specific capacitance of 905 F g -1 at 1 A g -1 is obtained, and a nearly constant rate performance of 78% is achieved at current density ranging from 1 to 40 A g -1 .

K-H Kim et al. [START_REF] Kim | Electrodeposition of mesoporous ruthenium oxide using an aqueous mixture of CTAB and SDS as a templating agent[END_REF] have performed an electrodeposition method for the synthesis of mesoporous RuO2 electrodes with very uniform pore sizes. They synthesized successfully these films using a mixture of SDS (sodium dodecyl sulfate) and CTAB (cetyl trimethyl ammonium bromide) as a templating agent. When SDS was used as a templating agent, collapse of porous structure, resulting in the formation of disordered porous structure, was observed after removal of this surfactant. The addition of small amount of CTAB significantly improved the stability of the porous structure. Electrochemical behaviors of synthesized RuO2 electrodes were investigated. Compared with non-porous RuO2 electrodes, mesoporous RuO2 electrode showed much higher specific capacitance and current density during charge-discharge processes.

Furthermore, mesoporous RuO2 showed higher supercapacitor performance which is attributed to the high surface area and facilitated charge transport of mesoporous structure.

IV. Diagnostics Tools for MO x based Electrodes for Energy Storage

IV-1. Surface and Structural Analysis: SEM, TEM, XRD, XPS, FT-IR: (i) SEM images:

Scanning Electron Microscope (SEM) has widely used for morphological analysis of various MOx materials. This diagnostic tool was employed by L Li et al. [42] As a result of this observation, the composite exhibit superior electrochemical performance with high specific capacitance, good cycling stability and rate capability. It is believed that the unique hierarchical WO3•H2O microstructures and the synergistic effect originated from the intimate combination of WO3•H2O with reduced graphene oxide are responsible for the enhanced electrochemical properties including large surface area for the electrolyte access and therefore promoting ions or electrons rapid transport [START_REF] Ma | Hydrothermal preparation and supercapacitive performance of flower-like WO3•H2O/reduced graphene oxide composite[END_REF].

(ii) TEM images M. Sasidharan et al. [20] have demonstrated a simple method for fabrication of WO3 hollow nanospheres of size ~ 42 nm using polymeric micelles with core-shell-corona architecture as a soft template under mild conditions. From Transmission Electron Microscopy (TEM) observation of hollow nanospheres with a void space diameter of 2 nm with thin shell domain of size 10 nm is evident (see figure I-21). As a result, the retention capacity of this nanostructured material when used as anode was very high compared to dense tungsten trioxide.

The author has observed that improved electrochemical behavior is attributed to nanosize effect coupled with hollow void space of WO3 hollow particles that facilitates fast lithium transfer kinetics. is employed in order to follow up the effect of annealing temperature on the structuration and in order to target the crystallographic evolution of the film as given in figure I-22 [START_REF] Muñoz-Rojas | Effect of particle size and cell parameter mismatch on the lithium insertion/deinsertion processes into RuO2[END_REF]. The RuO2 film crystallinity was then analyzed using X-ray diffraction for films with different deposited weights (Fig. I-24). The peak intensities of titanium substrate were reduced with increasing thickness (weight cm -2 ) of RuO2 film. However, the peaks corresponding to RuO2

were observed for all film thickness, indicating that the as-deposited film is not the amorphous form of RuO2, contradicting to the observations made by Zhitomirsky et al. [START_REF] Zhitomirsky | Ruthenium oxide deposits prepared by cathodic electrosynthesis[END_REF], and Hu et al. [START_REF] Hu | Effects of preparation variables on the deposition rate and physicochemical properties of hydrous ruthenium oxide for electrochemical capacitors[END_REF][START_REF] Hu | Cyclic voltammetric deposition of hydrous ruthenium oxide for electrochemical supercapacitors: effects of the chloride precursor transformation[END_REF]. According to the illustrated results the broadening of RuO2 peaks suggests that the deposited RuO2 consists of grains of nanometer size. The intensities of RuO2 peaks were increased with increasing film thickness (g cm -2 ). The peak at 40.1 • (d-value =2.05 Å) could not be well resolved, as it can be attributed to the both, deposition of metallic ruthenium or ruthenium oxide. Therefore, it is concluded that in their study, RuO2 and Ru have been codeposited [START_REF] Park | Performance of supercapacitor with electrodeposited ruthenium oxide film electrodes-effect of film thickness[END_REF][START_REF] Park | Cathodic electrodeposition of RuO2 thin films from Ru(III)Cl3 solution[END_REF].

(iv) FTIR methods

The Fourier Transform Infra-Red spectroscopy (FT-IR) was used by UM Patil et al. [START_REF] Patil | Chemically synthesized hydrous RuO2 thin films for supercapacitor application[END_REF] in order to verify the formation of chemically prepared RuO2 powders.

IV-2. Electrochemical Tools: (i) Cyclic voltammetry

The examples of using cyclic voltammetry in order to study the electrochemical behavior of pseudocapacitive materials are numerous. In order to improve the capacitive performance of WO3, in a recent paper by Y-H Wang et al. [START_REF] Wang | Dispersing WO3 in carbon aerogel makes an outstanding supercapacitor electrode material[END_REF] this metal oxide was introduced to carbon aerogels, in a form of well-dispersed single crystalline nanoparticles with a simple immersioncalcination process. The carbon aerogels serve as the conducting, mesoporous template to host the dispersion of WO3. Therefore, the capacitive performance of WO3 was greatly improved over that of the plain WO3 electrode through the dispersion design achieved with the carbon aerogels template. As chosen in figure I-26 specific capacitance as high as 700 F g -1 were obtained at the scan rate of 25 mV s -1 in 0.5 M H2SO4 over a potential window of -0.3 to 0.5 V (vs. Ag/AgCl). 2) asymmetric (RuO 2 -WO 3 ) capacitors. The total weight of all active materials (including cathode and anode) for both symmetric and asymmetric capacitors is equal to ca. 4mg cm -2 [START_REF] Chang | Microwave-assisted hydrothermal synthesis of crystalline WO3-WO3•0.5H2O mixtures for pseudocapacitors of the asymmetric type[END_REF]. From these examples and also other available studies not presented here it could be concluded that EIS could bring information in terms of resistance of transfer and capacitance determined through an equivalent circuit approach. Nevertheless, it would describe globally the elements involved in this electrochemical system from a general point of view. However, this methodology lonely doesn't give that much of kinetics information necessary to understand the key reactions involved with ions and charge compensation at the interface of electrode/ electrolyte.

(ii) EIS technique

(iii) Quartz Crystal Microbalance

Another methodology which could target ions intercalation/electroadsorption is quartz crystal microbalance (QCM).There have been various studies using quartz crystal microbalance as an in situ gravimetric probe to study the insertion and/or electroadsorption of ions in metal oxides or carbon based electrodes [START_REF] Tsai | Electrochemical quartz crystal microbalance (EQCM) study of ion dynamics in nanoporous carbons[END_REF][START_REF] Fernandes | Nanogravimetric studies of tungsten oxide thin films obtained by the polymeric precursor method[END_REF][START_REF] Vondrák | Insertion of cations into WO3 investigated by QCM techniques[END_REF][START_REF] Arias | New Insights into Pseudocapacitive Charge-Storage Mechanisms in Li-Birnessite Type MnO2 Monitored by Fast Quartz Crystal Microbalance Methods[END_REF].

Electrochemical quartz crystal microbalance (EQCM) and cyclic voltammetry (CV) measurements (Fig. I-30) were used by P Simon et al. [START_REF] Tsai | Electrochemical quartz crystal microbalance (EQCM) study of ion dynamics in nanoporous carbons[END_REF] to characterize ion electroadsorption involved with carbide-derived carbon (CDC) with two different average pore sizes, from neat and solvated EMI-TFSI electrolytes. Their EQCM study showed some key differences existing between EMI + and TFSI -ions during transport and electroadsorption into carbon nanopores. The equivalent weight values, higher than that of Li + (7 g mol -1 ) were simply attributed to the acetonitrile molecules, accompanying the Li + ions.

A similar study by Vondrak et al. [START_REF] Vondrák | Insertion of cations into WO3 investigated by QCM techniques[END_REF] investigated the electrochemical insertion of H + , Li + , Na + ions into thin layers of WO3 by EQCM in propylene carbonate. EQCM data of their work also detected molar mass values higher than that would correspond to the cation present in the electrolyte. Therefore, it was suggested that ions do not enter the space lattice alone but may be accompanied by propylene carbonate solvent molecules without any other pertinent explanation.

Despite useful information given by EQCM when it comes to describe the ion intercalation/electroadsorption mechanisms involved with charge storage in capacitive materials, there are also some limitations. EQCM gives a global response corresponding in fact to several possible pathways such that ions, ions with solvation shells and even indirectly free solvent molecules can be associated to the electrochemical process. Additionally, ions may lose a part of their solvation to access to the sites in smaller nanopores. These possible pathways, and kinetic or dynamic aspects of the ion intercalation/electroadsorption processes have never been characterized in the previous mentioned EQCM studies due to the limitations of the classical technique.

An alternative characterization tool was proposed to overcome the limitations of the classical EQCM to study the ion intercalation/electro adsorption mechanisms in pseudocapacitive electrodes. This method, so-called ac-electrogravimetry consists of an in situ coupling of electrochemical impedance spectroscopy (EIS) and a fast quartz crystal microbalance (QCM).

Although QCM exists more or less routinely in laboratories these days, this coupling has been developed in a limited number of laboratories worldwide. The ac-electrogravimetry simultaneously measures the electrochemical impedance, ()

E I   
, and the mass/potential transfer functions, ()

m E   
during a sinusoidal potential perturbation with a small amplitude applied to the modified electrode. The mass/potential transfer functions allow the change in mass due to a unit charge passing through the electrode/film/electrolyte interfaces to be determined. It provides the access to the relevant information on (i) the kinetics of species transferred at the solid/ solution interfaces, and their transport in the bulk of the materials, (ii) the nature of these species as well as their relative concentration within the material. This coupling dominates over the limitations of QCM technique and has the ability to deconvolute the global mass changes provided by QCM measurements. Specifically, it detects the contribution of the charged or uncharged species and to identify anionic, cationic, and the free solvent contributions during various redox processes, and recently has been applied to study pseudo-capacitive charge storage mechanisms in Li-birnessite type MnO2 electrodes [START_REF] Arias | New Insights into Pseudocapacitive Charge-Storage Mechanisms in Li-Birnessite Type MnO2 Monitored by Fast Quartz Crystal Microbalance Methods[END_REF].

V. The Scope and Principle Objectives of Thesis Project:

In the first section of this chapter the importance of investigating materials, with an emphasize on those which can be used for fabricating pseudocapacitive films for energy storage devices, was discussed. Furtherly several examples of capacitive metal oxides and various possibilities for their elaboration were categorized. Then, different structural and electrochemical diagnostic tools were employed in order to characterize them and therefore, to improve their performances.

Since the key phenomena in all these examples of capacitive materials is the ion's exchange at the interface of electrode/electrolyte, it was clearly seen that none of mentioned diagnostic methods lonely provide information on the exact identification of the intercalated ionic species, their dynamics of transfer at the interfaces, as well as the role of electrolyte composition and the effect of ions solvation on the various phenomena. The status of transferred ions is not a quite solved problem and the characterization of their transfer dynamics is not straightforward using conventional characterization tools. Therefore, the challenge is to find an eligible technique offering mechanistic solutions in a single body. This technique should allow the study of ion intercalation/electroadsorption phenomena in situ and in contact with an electrolyte.

Consequently, it was concluded to focus on the special capability of ac-electrogravimetry as a powerful coupled electrochemical methodology in order to exploit information and to study the ion intercalation/extraction behavior of WO3, RuO2 and TiO2 metal oxides. Special attention is given to the poorly understood aspects, such as the nature of the ions involved in the charge compensation, solvation and the role of the electrolytes and the dynamic information of ions transfer at the electrode/electrolyte interfaces.

Another equally important discussion was the improvement of the performance of metal oxide based electrodes which is with no doubt attributed to their structure. Nanostructuration could procure materials with favorable morphologies, unique properties and functionalities that can effectively be exploited in electrochemical devices. As a consequent, the main objective of this thesis project is to provide an answer to the following questions:

 Do mesoporous films, with small pore sizes, and large surface area to volume ratios, facilitate the ion intercalation/electro adsorption process involved with each chosen synthesized MOx?  What differences in behavior are mainly brought by procuring porosity within the film?

 How ac-electrogravimetry as the main non-classical methodology served in this project could be advantageous for our study?

 Is this technique able to extract subtleties unreachable with classical tools?  In which way the obtained information could be helpful for the future design and optimization of electrode materials for energy storage systems?

Résumé du Chapitre II

Ce chapitre est consacré aux différentes techniques de mesures/caractérisation utilisées au cours de ce projet de thèse ainsi qu'aux bases théoriques associées et aux méthodes d'élaboration des différents matériaux examinés dans ce travail.

La première partie est consacrée à la description des différentes techniques de caractérisation structurale (diffractométrie de rayons X, spectrométrie de photoélectrons induits par rayons X, microscopie électronique à transmission (haute résolution), microscopie électronique à balayage) et électrogravimétriques (électrogravimétrie cyclique, acelectrogravimetrie). L'ensemble de ces outils sera utilisé pour étudier l'influence des différentes méthodes de préparation électrochimiques et physiques utilisés pour la fabrication des électrodes de type MOx avec différentes morphologies sur la réponse électrochimique de ces différents films.

La fabrication des films de TiO2 amorphes a été faite selon trois types de morphologie, compacte, poreuse et très poreuse (résultats présentés dans le chapitre III) grâce à un dispositif de pulvérisation réactive de type magnétron au sein de notre laboratoire. Ceci a été possible en contrôlant un paramètre important qui est la pression d'argon et d'oxygène dans la chambre de pulvérisation pendant le dépôt. Cela permet de déposer des couches denses mais également poreuses qui présentent des porosités différentes. La question fondamentale qui doit être posée lors de la pulvérisation réactive est comment le gaz réactif qui se combine avec la cible métallique va modifier sa nature chimique. Ainsi les propriétés de surface de la cible métallique sont modifiées en fonctions des conditions de fonctionnement du réacteur de pulvérisation magnétron. Le taux de pulvérisation pour le nouveau matériau formé sur la cible, est en général nettement inférieur par rapport à celui du matériau cible métallique en particulier si ce composé est un semi-conducteur comme TiO2 ou un isolant. L'objectif du champ magnétique est d'augmenter l'efficacité du phénomène d'ionisation du gaz noble employé en piégeant les électrons dans le plasma. En effet, cela permet de confiner le plasma au voisinage de la surface de la cible. Une source RF est plus efficace qu'une source de courant continu dans le cas de la pulvérisation cathodique réactive d'un matériau semi-conducteur en raison de l'accumulation de charges isolantes sur les surfaces dans ce dernier cas. Avant d'effectuer les analyses électrogravimétriques, la structure de ces films a été étudiée par MEB et MET à haute résolution.

La synthèse de films minces de WO3 denses et mésoporeux (résultats présentés dans le chapitre IV) a été réalisée par voie électrochimique sans ou avec la présence de molécules de tensioactifs. Pour cette voie de préparation, les molécules tensioactives, du dodécylsulfate de sodium (SDS), ont été ajoutées à la solution de dépôt électrolytique en tant qu'agents structurants. L'incorporation de ces molécules dans les films électrogénérés résulte de l'autoassemblage contrôlé d'agrégats de tensioactifs inorganiques aux interfaces solide-liquide. Lors

Chapter II: Theory and Experimental I: Introduction

This chapter is dedicated to necessary theoretical and experimental basics used in this thesis project. The first part is attributed to the description of various structural and electrochemical characterization techniques applied as diagnostic tools to study the different electrochemical and physical preparation methods used for fabricating the MOx electrodes with different morphologies. In the second part, the different components of the model used for acelectrogravimetric fittings/simulations will be introduced; it will be shown how the different ac-electrogravimetric transfer functions for an electroactive film can help in a pertinent way to ion transfer investigations.

II: Experimental

II-1: Electrochemical and (Electro)gravimetric Characterization Techniques

II-1.1: Quartz Crystal Microbalance (QCM)

Principle of piezoelectricity:

The word piezoelectricity comes from the Greek and it means "electricity by pressure" (piezo means pressure in Greek); it was proposed by Hankel in 1881, a year after the discovery of this phenomenon by Jacques and Pierre Curie. The piezoelectric effect is the property of certain materials to polarize under the action of a mechanical force, and vice versa to be altered if an electric field is applied. Both effects are inseparable. The first is called direct piezoelectric effect, the second inverse piezoelectric effect. More generally, the direct effect can be utilized in the production of sensors (pressure sensor, microbalance) while the reverse effect can be used (piezo injectors in automotive, nano-manipulator, etc).

According to the definition of piezoelectricity, the quartz crystal is capable of converting a mechanical stress into an electrical signal. It can be used to make a transducer. In fact, the piezoelectric transducer is an entity capable of converting an interaction to the modified electrode / liquid interface in an easily measurable electrical signal. Piezoelectric transducers, more commonly called quartz microbalance, are increasingly used in electrochemistry for the study of interfaces [1][2][3][4][5][6]. Among the piezoelectric components existing in nature, quartz is the one most commonly used. Quartz is a crystal of silica (SiO2) available in nature which is synthesized in industry. This crystal has a great hardness and it is chemically inert. Only hydrofluoric acid might attack the crystal. Under ambient temperature and normal pressure, quartz solubility is almost zero in basic solution [7].

The AT-cut oriented 35° 12' relative to the axis Z, is the one we use thereafter [8]. It is the mode of the microbalance the most commonly used. The crystal is shaped like a thin disc (Figure II-1), with a 14 mm diameter. The thickness of the quartz determines the resonant frequency. On each side of the disk, a gold electrode was deposited by vacuum evaporation. Each electrode is in the form of a key hole with a central disk of 5 mm diameter. Practically, a chromium underlayer is sandwiched between the crystal and the gold, this is due to the poor adhesion of the gold on the crystal. In general, the gold electrode has a thickness of 200 nm and the sub-layer of chromium is about ten times finer. The piezoelectric effect can only take place within the area defined by the two gold electrodes opposite from each other, so-called active surface area.

II-1.1.1: Principle of QCM

According to the definition of piezoelectricity, the quartz crystal is capable of converting a mechanical stress or a mass load into an electrical signal. Indeed, this piezoelectric transducer is an entity capable of converting an interaction at the modified electrode / liquid interface to an easily measurable electrical signal. Piezoelectric transducers, more commonly called quartz microbalance, are increasingly used in electrochemistry for the study of interfaces. The quartz crystal microbalance is a high precision instrument able to measure the mass changes at the surface of one of the quartz faces by measuring the change in frequency associated with the quartz resonator. The quartz crystal microbalance is made of a quartz crystal inserted in an electronic circuit which provides a stable signal over time. This set-up is called an oscillator and any perturbation applied to the quartz surface varies the oscillation frequency, with a measured quantity.

In 1959 Sauerbrey was the first to establish a simple equation relating mass variations to microbalance frequency [9]. When a rigid material, purely elastic, and thin, is deposited on the surface of one of the quartz faces, the relationship between the mass of material ∆m and the translation of the microbalance frequency of quartz, Δfm, is linear and can be expressed as:

2 0 2 S m th f f k m m Sn             (1)
Where m f  is the microbalance frequency variation (Hz), S is the surface of metal electrodes positioned on the quartz (cm²), ρ is the quartz density (2,648 g cm -3 ), μ is the quartz shear modulus (2,947 10 +11 g. s -2 . cm -1 ), n is the harmonic number, f0 is the frequency of the microbalance in the air and kth S is the theoretical sensitivity of the microbalance.

With a microbalance operating at 9 MHz, kth S is theoretically equal to 16,7×10 +7 Hz. g -1 .cm +2 ;

for a microbalance frequency change of 1 Hz variation, a mass variation of 1 ng for 0,2 cm² of active surface is estimated theoretically. The calibration of the microbalance by copper galvanostatic deposition on the electrode gives a value of the sensitivity of the microbalance around 16,3 10 +7 Hz. g -1 . cm +2 for an imposed current of 0,5 mA, which is in good agreement with theory. Sauerbrey Equation (eq. 1) shows that an increase in mass at the electrode causes a decrease in the microbalance frequency. The sensitivity of the microbalance follows a constant value in the gravimetric regime or in other words, of the Sauerbrey equation is valid for a fine thickness of a purely rigid material deposited on the surface of the quartz. When electrochemical studies are performed in solution, the validity of the Sauerbrey equation is limited by the viscosity, the density of the solution and also by the viscoelasticity of the deposited film. To limit this effect, electrogenerated films with a sub-micron thickness could be considered as acoustically thin enough layers: the equation of Sauerbrey will be valid and the microbalance will operate in gravimetric regime.

II-1.1.2: Experimental Set-up

The quartz crystal and its electrodes constitute a piezoelectric resonator: the surface modifications (mass, mechanical stress, etc.) are transformed into measurable electrical signals.

The quartz resonator, coupled with appropriate electronic to form an oscillator, experience its resonant frequency shift as a result of these surface modifications.

The experimental set-up used usually for our experiments is a microbalance fully fabricated at

II-1.2: Cyclic Electrogravimetry (EQCM) II-1.2.1: Principle

Cyclic voltammetry is a classic electrochemical characterization method. This technique is used in a first approach to study the electrochemical reactions mechanisms because of its simplicity and rapidity. Cyclic voltammetry also allows to electrogenerate electroactive films on the surface of the working electrodes and in a second step, to determine the field of activity of these deposited films in a given electrolyte. The measurements are made with a classical threeelectrode assembly. The principle is to impose two successive scans of potential in the opposite direction, the term cyclic, between the working electrode and a reference electrode and monitoring the change in current across the working electrode. By using the gold electrode of the microbalance as a working electrode, it is possible to follow concurrently the variation of the microbalance frequency, fm, as a function of potential, and thus, to evaluate the mass variations within an electroactive film. As a matter of fact, the changes in the potential applied through the film, by the charge compensation process, lead to insertion/expulsion of charged or non-charged species at the interface of film/solution. These species movements procure changes in the mass of the film on the crystal's surface also in the microbalance frequency, fm.

The experimental montage includes: a reference electrode either saturated calomel electrode (SCE) or saturated Ag/AgCl, a platinum counter electrode with a dimension of 2cm × 4cm, a gold working electrode deposited on the quartz resonators, with 0,5 cm diameter with an electrochemical active surface of 0,27 cm 2 and an effective surface area of 0,2 cm 2 (for mass).

This electrochemical three-electrode cell is connected to a potentiostat specially modified to be compatible with our microbalance as our working electrode is grounded. The potentiostat is equipped with an additional acquisition data card (analog / digital or A / D) to measure, in parallel with the current, the microbalance frequency variation consecutive to voltage sweep.

The assembly is controlled by a BioLogic software. Between 9 MHz oscillator and the potentiostat A/D input, a frequency meter (Yokogawa, TC110) is also intercalated. The latter operates for the conversion of microbalance frequency variations, fm, using a 15-bits frequency/voltage converter: each change in fm is converted to a voltage between 0 and 10 V, which is then received by the potentiostat. Thus, it is possible to measure both the current changes, i, and microbalance frequency variations, fm , over potential scans (Figure II-3).

II-1.3: Electrochemical Impedance Spectroscopy (EIS)

in the case of complex electrochemical reactions consisting of a series of elementary steps of different kinetics. But to better understand the different mechanisms of an electrochemical system, it is interesting to characterize each of these reactions. If the conventional techniques make it difficult to distinguish these basic steps of each other, the electrochemical impedance can provide the necessary information in this regard [10][11][12].

II-1.3.1: Principle

The basic principle of the electrochemical impedance is to apply on an electrochemical system a stationary potential accompanied with a sinusoidal perturbation of a small amplitude at a given frequency of modulation. The electrochemical system can be considered under stationary condition and this low level perturbation should help to separate the different reactions with different kinetics [12]. Most electrochemical systems have generally a non-linear currentvoltage characteristic curve. However, working only on a small portion of this curve, it could be considered having a linear relationship between the different variables measured (Figure II-4). As a result, by applying to the system a sinusoidal perturbation of small amplitude V around a stationary potential Vs, the current response will also be sinusoidal, with a small amplitude I around a stationary value Is. By definition for a linear system, there is a linear relationship between V and I. Then, we can measure the

) ( I V  
transfer function, called electrochemical impedance, where ω = 2πf

is the pulsation.

The electrochemical impedance, Z (ω), is a complex number that can be represented either in

polar    , Z
or in cartesian coordinates (Re Z, Im Z):

  Z j Z j Z Z Im Re exp      (2)
The relationship between these quantities are:

Firstly,     2 2 2 Im Re Z Z Z   and Z Z Re Im arctan   (3)
Then,

 cos Re Z Z  and  sin Im Z Z  (4)
Where | Z | is the modulus, the ratio between the amplitudes of V and I; j is the complex number (as j² = -1); φ is the phase, the representative phase difference between V and I; Re Z and Im Z are the real and imaginary parts of Z (ω).

  d t s C j R R Z      1 1 (5)
      1   Z Y
can be similarly analyzed and used.

II-1.3.2: Experimental Set-Up

The experimental setup is shown in figure II-6. It consists of:

 A SOTELEM-PGSTAT100 potentiostat that works in potentiostatic mode, and imposes the stationary potential Vs,  A frequency generator that delivers the sinusoidal perturbation of small amplitude, V.

 A three-electrode cell

II-1.4: Ac-electrogravimetry ; Fast Electrogravimetric Method

II-1.4.1: Principle

The ac-electrogravimetry is similar to the electrochemical impedance technique. In fact, a E sinusoidal perturbation signal of low amplitude, applied to the electrochemical system, may cause changes in the mass of the film, m, deposited on the microbalance allowing the measurement of a transfer function called mass/potential or electrogravimetric transfer function,

) ( E m  
. By using the gold electrode of the quartz crystal microbalance as a working electrode, we can simultaneously perform two distinct types of measures: The electrochemical

impedance ) ( I E  
, and the electrogravimetric transfer function,

) ( E m   .
The measurements are made with the same three-electrode cell described above in an aqueous medium. When a sinusoidal perturbation, E, of small amplitude is applied to the electroactive film deposited on the gold quartz microbalance electrode, a certain number of charged species in the solution will participate in the charge compensation process within the material. This insertion or expulsion of species in/from the film is detected by the microbalance frequency variations, fm. Moreover, due the high sensitivity of the microbalance, it measures mass changes, m, in the scale range of nanograms and with a very fast response time, less than a millisecond. The corresponding mass variation, m, is then estimated through the Sauerbrey's equation (Eq. ( 1)).

The modulation frequency of the perturbation signal provides additional information: it allows to separate the kinetics of different species involved in the charge compensation of electroactive film. The measurements are controlled by a computer via the FRACOM software, which was also developed at LISE laboratory. For these measurements, it is necessary to use a multichannel analyzer (Solartron 1254) in order to determine, in parallel, the two main experimental transfer functions: the electrochemical impedance,

     I E
, and an the

) ( V V f  
transfer function, which allows to calculate the electrogravimetric transfer function

) ( E m  
. Indeed, it is not possible to measure directly the electrogravimetric TF,

) ( E m  
. So, a lab-made frequency / voltage converter was used for transforming the signal of the microbalance fm in a measurable voltage signal, Vf, which can then be received by the analyzer 1254. Then, it is possible to extrapolate m from this signal, Vf, for a configuration and a given type of measurement. This was achieved by calibrating the system before measurements.

III-1.4.2. Experimental Method

The experimental setup (

II-1.4.3. Calibration and System Corrections

The purpose of the calibration is to measure the parasitic transfer function of the electronic part which distorts electrogravimetric transfer function. In reality, the calibration will give us a characterization of the electronic set-up used and then, it will be used to digitally correct the experimental files

) ( V V f   to obtain ) ( E m  
for each frequency modulation.

The relation between electrogravimetric transfer function

) ( E m  
and various correction terms is described below:

            E V V V V f f m E m f f m m            (6)
Where,

m f m  
is the sensitivity of the microbalance obtained by calibration and it appears in the Sauerbrey equation (eq. 1). For a 9 MHz quartz [13], the experimental sensitivity value is 16.3

10 +7 Hz g -1 cm +2 .    f m V f  
is the inverse of the sensitivity of the frequency-voltage converter and it might be estimated by the equation:

         f m f m V e e f V f        (7)
Where

      e f e f s m      / /
is the sensitivity of the synthesizer that simulates the microbalance considering

s m f f    .    f V e   /
is the inverse of the transfer function of the frequency / voltage converting device and it is obtained by calibration.

    V V f  
is the measurement obtained directly with FRA-1254 analyzer and FRACOM software.

    E V  
is the term that allows the IR drop correction to be done. Using the electrolyte resistance, Re, the expression can be taken:

     1 /         I E R E V e .
It is observed that the voltage perturbation during a calibration is denoted ∆e = ∆|e.|sin (ωt). It should also be noted that the converter sensitivity is given by the value of

s f f V   .

II-1.4.4. Transfer Function of the Frequency/Voltage Converter:

This transfer function is determined by replacing the microbalance by a frequency synthesizer, Agilent 33205A. The rest of the montage is identical to what was previously explained with the exception of the electrochemical part which disappears. The signal e  , from the FRA 1254 generator, will allow to modulate the frequency of the synthesizer, Agilent 33205A, to be done and also to simulate the response of a microbalance on which sinusoidal mass variations are observed.

An example of calibration curve obtained is presented in the form of a Bode diagram in figure II-9. It is noted that for frequencies of modulation, f, less than 1 Hz, the phase shift is negligible and the modulus has a constant value in relation to the sensitivity of the converter used. This means that up to this frequency, a simple proportional correction can be performed on experimental measurements. Below 1 Hz, a frequency to frequency correction should be performed digitally in order to eliminate the electronic contribution to modulus and to phase of

the ) ( V V f   measurement.

II-1.4.5. Calibration of the Synthesizer:

It is then to determine the e f s   transfer function of the Agilent 33250A synthesizer which was used to simulate a microbalance during the calibration process previously mentioned. To determine the transfer function of this synthesizer it should simply apply, via the FRA 1254 generator, a fixed sinusoidal perturbation of frequency f, which with a certain amplitude e.

The Agilent synthesizer 33250A is adjusted to a 9.0 MHz carrier frequency equivalent to the frequency of microbalance used. Three levels of depth linked to the frequency carrier (FM mode) were tested. Three configurations of the Agilent 33250A, 10 Hz, 100 Hz and 300 Hz, were selected. For the rest of the study, the work is performed with the FM setting = 100 Hz. So, to correct the measurements, the following table should be considered (Table II-1) to use the equations 2 and 6.

m f m   (g. cm². Hz -1 ) 0         e V f e f s   (Hz V -1 )

II-2: Preparation of MO x based Thin Films Electrodes

II-2.1: Elaboration of Compact, Porous and Highly Porous TiO 2 by RF Reactive Magnetron Sputtering

The deposition of compact, porous and highly porous TiO2, was realized by reactive RF magnetron reactive sputtering at LISE laboratory. Optimal deposition conditions were chosen based on previous reports by H. Fakhouri et al. [14][15][16]. According to their reports, the basic issue that must be faced during reactive sputtering is that the reactive gas combines with the target material to form a new compound, in this way it will change the surface properties of the target [14]. Ideally, this reaction takes place on the surface of the substrate, but in reality it occurs not only at the substrate but also in the reactor volume, on chamber walls and even on the target surface. It is the reaction on the target surface that leads to the classic problem in reactive sputtering called "poisoning" phenomena. The sputtering rate for the compound material, which forms on the target, is usually significantly less than the rate for the metallic target material especially if this compound is a semiconductor (TiO2) or an insulator. The major components of the system are presented in fig. II-12. The objective of the magnetic field is to increase the ionization efficiency by trapping the electrons in the plasma. This allows plasma to be confined at the vicinity of the target surface. An RF source is more efficient than DC source in the case of the reactive sputtering of a semiconductor or insulating material because of charge accumulation on such surfaces in the case of the latter.

The thin films are deposited in a 13.56 MHz RF magnetron sputtering deposition chamber (SPT 120, Plasmionique, Canada), using a balanced magnetron cathode (MAGNION-B). The pumping system includes a turbo molecular pump (300 s -1 , Varian TV301 Navigator) and a mechanical pump (ULVAC) for backing the turbo. The SPT 120 magnetron sputtering reactor has two quartz windows used as vacuum viewports for optical spectra acquisition. To prevent any contamination on the windows, the viewports are mounted about 10 cm away from the reactor walls using special flanges with additional aluminum foils inside the reactor.

The background pressure for all depositions was about 5×10 -6 Torr (6.7×10 -4 Pa), while the total working pressure was adjusted between 2 to 20 mTorr (0.3 to 3 Pa). All films were deposited using a metallic Ti target (99.95% purity, 2-inch diameter, NEYCO). Prior to each deposition, the target was pre-sputtered in argon atmosphere for 10 minutes to remove any contaminations or "poisoned film" from the Ti surface. Then, the target was sputtered in a reactive gas atmosphere containing Ar + O2 for TiO2 films deposition. The typical RF power delivered by the generator was 200 W, corresponding to a typical DC bias ranging from -140 V to -160 V, depending on the target surface conditions (clean target or poisoned target).

Pure TiO2 thin films of different morphologies were prepared by this methodology with the following details. A metallic Ti target of high purity (99.95%), was sputtered in a reactive gas atmosphere containing Ar and O2 for the deposition of pure TiO2 films. For that, the deposition pressure was controlled by the Ar flow rate in the deposition chamber, fabricating films at p = 3, 6, and 14 mTorr with corresponding Ar flow rates of 30, 60, and 140 sccm (standard cubic centimeter) respectively. The O2 gas flow rate was fixed at 1.9 -2.1 mtorr for all the samples.

The fixed experimental conditions chosen were situated in the intermediate region between two stable sputtering modes, reactive and metallic. The substrate holder was maintained at low temperature below 100°C. The distance between the substrate holder and the target was fixed at 10 cm. The films were deposited on gold-patterned quartz substrates of 9 MHz. Before deposition, the substrates were ultrasonically cleaned with acetone, ethanol and then, deionized water for 20 min each.

II-2.2: Electrochemical Elaboration of Amorphous Compact and Amorphous Mesoporous WO 3

The electrodeposition solutions for the synthesis of dense and mesoporous WO3 thin films were prepared as described elsewhere [17,18]. Briefly, 0.9 g W powder (99.99%, Aldrich Chem, USA) was dissolved in 30 ml of 30% H2O2 (analytical reagent, Sigma-Aldrich Germany) which takes about 4 hours for complete dissolution. A small portion of Pt black was then added to remove the excess of H2O2. This removal process can be accelerated by heating the solution up to 70 °C to obtain a pale-yellow solution of HxWO3. The solution was diluted to 50 mM with a 50:50 water and isopropanol mixture. For the mesoporous thin film synthesis, the solution also contained 0.05 M sodium dodecyl sulfate (SDS) (ACS reagent, 99.0% Sigma-Aldrich, Japan).

Gold-patterned quartz substrates of 9 MHz (RAKON, France) were used as working electrodes.

A platinum grid and an Ag/AgCl (3M KCl saturated with AgCl) served as counter electrode and reference electrode, respectively. The electrochemical WO3 synthesis was performed by potentiostatic electrodeposition at -0.5 V vs Ag/AgCl. During electrodeposition, a salt-bridge junction equipped with a porous glass frit on the end was used to prevent the reference electrode to be contaminated by the media and vice versa. The electrodeposition was performed by using a potentiostat (Autolab PGSTAT100) and the deposition process was monitored by quartz crystal microbalance measurements. Film area is 0.25 cm 2 (gold electrode on the quartz resonator) and the film thickness was controlled by the electrodeposition time, typically for 15, 20 or 30 minutes. The SDS surfactant in the WO3 thin films was extracted from the inorganic matrix by washing with ethanol/double distilled water mixture before the electrogravimetric studies.

For the electrochemical synthesis of the mesoporous WO3 thin film, surfactant molecules

II-2.3: Electrochemical Elaboration of Compact and Mesoporous RuO x .nH 2 O

In our approach, the following reactions are considered to generate base on the electrode surface:

O2 +2H2O+ 4e -↔ 4OH - (8) 2H2O + 2e -↔ H2 + 2OH - (9)
These reactions consume H2O, generate OH -and high pH values at the cathode are observed.

In cathodic deposition, metal ions or complexes are hydrolyzed by electrogenerated base to form oxide, hydroxide or peroxide deposits on cathodic substrates. Hydroxide and peroxide deposits can be converted in to corresponding oxides by thermal treatment.

Electrodeposition can appear as an appropriate method for the deposition of RuO2 films. The mechanism of RuO2 deposition is not fully understood [20][21][22][23][24]. Hydrated ruthenium chloride, the salt used in this application, is a heterogeneous ionic material with an average ruthenium oxidation state between 3 and 4, close to 4. For this reason, the mechanism of formation of RuO2 from RuCl3•nH2O precursor is rather complex. The ruthenium species are most likely to precipitate as hydrated ruthenic oxide (RuO2•nH2O) or ruthenic hydroxide Ru(OH)4. This process consumes the electrochemically generated OH -ions. As the deposition process progresses, an insulating layer forms, which in turn prevents OH -generation, and therefore, further deposition is stopped. However, ruthenium oxide exhibits metallic conductivity so deposition of high thickness of ruthenium oxide is possible. It has been reported elsewhere [20][21][22][23][24] that the initial pH of the deposition bath strongly influences the RuO2 deposition process.

This effect was considered to be due to the chemical conversion of the dissolved RuCl3 Gold-patterned quartz substrates of 9 MHz (RAKON, France) were used as working electrodes.

A platinum grid and an Ag/AgCl (3M KCl saturated with AgCl) served as counter electrode and reference electrode, respectively. The electrochemical RuCl3.xH2O synthesis was performed by potentiostatic electrodeposition at -0.6 V vs Ag/AgCl. The electrodeposition was performed using a potentiostat (BioLogic SP-200) and the deposition process was monitored by quartz crystal microbalance measurements. The film area is 0.2 cm 2 (gold electrode on the quartz resonator) and the film thickness was controlled by the electrodeposition time, typically for 15, 20 or 30 minutes. The CTAB surfactant in the as-prepared mesoporous thin films was extracted from the inorganic matrix after deposition by washing with ethanol/water mixture and heating the sample up to 150°C for 1h maximum, before the different studies.

II-2.4: Elaboration of CNTs/RuO x .nH 2 O Films

CNT deposition: The carbon nanotube CNT film deposition includes a direct deposition of a CNT suspension droplets on the gold-covered quartz substrates. To do so, the CNT solution should be prepared before procedure is as follows [26]:

First, 32 mg of CNT (90 %, Sigma-Aldrich, Belgium) (single wall) are mixed with 2 mg of acetylene black (99.9%, Alfa Aesar, USA) (which is added to improve the electrical conductivity of the composite electrode), 4 mg of polyvinylidene fluorine which is the polymeric binder (PVDF-HFP, Solvay, Belgium), and 10 mL of N-methyl-2-pyrrolidone (99.5%, Sigma Aldrich, Germany). Then, the resulting suspension is placed in an ultrasonic bath. The homogenisation of this suspension takes quite a time (at least two days) and when the solution is ready, a very fine micropipette is used to cover the substrate with 4 μL of this suspension. A mask is used in order to drop the suspension properly only on the gold surface.

The prepared samples are then kept for 12 hours in a silica gel desiccator and finally heated in a tubular ceramic furnace at 130°C for ~ 30-45 minutes [26]. In a second step, the metal oxide deposition is performed as previously explained by varying the deposition time (between 5 to 15 minutes).

II-3: Structural and Morphological Investigation Methods: II-3.1: Scanning Electron Microscopy (SEM) and Energy Dispersive X-rays (EDX)

A scanning electron microscope (SEM) [27][28][29] is a type of electron microscope that produces images of a sample by scanning it with a focused beam of electrons. The electrons interact with atoms in the sample, producing various signals that contain information about the sample's surface topography and composition. The electron beam is generally scanned in a raster scan pattern, and the beam's position is combined with the detected signal to produce an image.

Specimens can be observed in high vacuum, in low vacuum, in wet conditions (in environmental SEM), and at a wide range of cryogenic or elevated temperatures. The most common SEM mode is detection of secondary electrons emitted by atoms excited by the electron beam. The number of secondary electrons that can be detected depends, among other things, on the angle at which beam meets surface. By scanning the sample and collecting the secondary electrons that are emitted, using a special detector, an image displaying the topography of the surface is created.

The figure II-15 shows SEM compartments. Before speed up with an electric field, the electrons are extracted from a heat filament or from a tip with a very high voltage. An anode broken with a small gap produces the speed up field of the electrons canon. These particles are then lead by magnetic coils. Two levels of coils allow homogenising the energy beam which will scan the sample. The microscopy used for our studies performs at high resolution (between 0.4 and 20

nanometres) provides high quality images of the surface also from cross-section view in order to estimate the film thickness. If needed to assure more conductivity a carbon touch could be sputtered for amelioration. The film morphology and the thickness were investigated by field emission gun scanning electron microscopy (FEG-SEM) (Zeiss, Supra 55). The elemental analysis was performed with an energy dispersive x-ray (EDX) detector associated to the FEG-SEM equipment.

II-3.2: Transmission Electron Microscopy (TEM)

Transmission electron microscopy (TEM) [27,30] is a microscopy technique in which a beam of electrons is transmitted through an ultra-thin film, interacting with the specimen as it passes through it. An image is formed from the interaction of the electrons transmitted through the specimen; the image is magnified and focused on an imaging device, such as a fluorescent screen, on a layer of photographic film, or to be detected by a sensor such as a CCD camera (fig II -16). This enables the instrument's user to examine fine detail-even as small as a single column of atoms, which is thousands of times smaller than the smallest resolvable object in a light microscope.

At smaller magnifications TEM image contrast is due to absorption of electrons in the material, to the thickness and composition of the material. At higher magnifications complex wave interactions modulate the intensity of the image, requiring expert analysis of observed images.

Alternate modes of use allow for the TEM to observe modulations in chemical identity, crystal orientation, electronic structure and sample induced electron phase shift as well as the regular absorption based imaging.

II-3.3: High-Resolution Transmission Electron Microscopy (HR-TEM)

High-resolution transmission electron microscopy (HRTEM) [27,30] is an imaging mode of the transmission electron microscope (TEM) that allows direct imaging of the atomic structure of the sample to be done. HRTEM is a powerful tool to study properties of materials on the atomic scale. HRTEM is often also used to refer to high resolution scanning TEM. For disambiguation, the technique is also often referred to as phase contrast TEM. At present, the highest point resolution realized in phase contrast with the new generation of TEM is around 0.5 ångströms (0.050 nm). At these small scales, individual atoms of a crystal and its defects can be resolved. For 3-dimensional crystals, it may be necessary to combine several views, taken from different angles, into a 3D map. This technique is called electron tomography.

The microscope uses an electron beam at a high voltage, issued by the electron gun. The, electromagnetic lenses focus the electrons on the sample. The electron beam produces different types of radiation by coming through the atoms of the sample. Finally, only the transmitted electrons are analyzed by the detector which converts the signal in a contrasted image.

The sample could be analysed either in directly in powder form or scratched from the surface:

 Powder: the powder is dismissed in ethanol, then, a drop of the solution is laid on the sample holder (which is a 3 mm copper grid).

 Electrodeposited films on a substrate: The deposit is scraped off the gold foil by a razor and collected by ethanol droplets. The solution is then pumped into a micropipette and deposited on the Cu grid.

The proper sample is then positioned in the microscope chamber and then, analysed by observing every tile of the grid (about 100), focusing on each nano-agglomerate. Images are taken at various magnifications, prior to image acquisition, an elemental analysis could assure the nature of metal oxide. For HR-TEM studies of the electrochemically prepared WO3 and RuOx.nH2O by surfactant assisted electrodeposition, the thin films were deposited on gold substrates (gold foil, 0.05 mm thickness, 99.95% purity (Goodfellow)) followed by thermal treatment at different temperatures. The samples were scraped off from the gold substrates and ultrasonically dispersed in ethanol. For TiO2 films, the samples were directly deposited on the copper grids. Our analyses were performed using a JEOL JEM 2010 UHR with a LaB6 filament microscope operating at 200 kV equipped with a CCD camera (GATAN). The chemical analyses were obtained by selected Energy-Dispersive X-Ray Spectroscopy (EDX) associated to a microanalyser (PGI_IMIX PC) mounted in the microscope.

II-3.4: Selected Area Electron Diffraction (SAED)

Selected area (electron) diffraction (abbreviated as SAD or SAED) [31], is a crystallographic experimental technique that can be performed inside a transmission electron microscope (TEM). In a TEM, a thin crystalline specimen is subjected to a parallel beam of high-energy electrons. As TEM specimens are typically ~100 nm thick, and the electrons typically have an energy of 100-400 KeV, the electrons pass easily through the sample. In this case, electrons are treated as wave-like, rather than particle-like. Because the wavelength of high-energy electrons is a few thousands of nanometer and the spacing between atoms in a solid is about a hundred times larger, the atoms act as a diffraction grating to the electrons, which are diffracted.

That is, some fraction of them will be scattered to particular angles, determined by the crystal structure of the sample, while others continue to pass through the sample without deflection.

As a result, the image on the screen of the TEM will be a series of spots, the selected area diffraction pattern, and each spot corresponding to a satisfied diffraction condition of the sample's crystal structure. If the sample is tilted, the same crystal will stay under illumination, but different diffraction conditions will be activated, and different diffraction spots will appear or disappear.

SAD is referred to as "selected" because the user can easily choose from which part of the specimen to obtain the diffraction pattern. Located below the sample holder on the TEM column is a selected area aperture, which can be inserted into the beam path. This is a thin strip of metal that will block the beam. It contains several different sized holes, and can be moved by the user. The effect is to block all of the electron beam except for the small fraction passing through one of the holes; by moving the aperture hole to the section of the sample the user wishes to examine. This particular area is selected by the aperture, and only this section will contribute to the SAED on the screen. This is important, for example, in polycrystalline specimens. If more than one crystal contributes to the SAED, it can be difficult or impossible to analyze. As such, it is useful to select a single crystal for analysis at a time. It may also be useful to select two crystals at a time, in order to examine the crystallographic orientation between them. As a diffraction technique, SAED can be used to identify crystal structures and examine crystal defects. It is similar to X-ray diffraction, but samples as small as several hundred nanometers in size can be examined, whereas X-ray diffraction typically can only examined samples areas with several centimeters in size. In our studies, the crystallinity of the synthesized as-prepared hydrated ruthenium oxide, as well the structural evolution of heated samples (at 150°C and 450°C) was investigated by SAED during TEM analyzes. This operation has been conducting in a JEOL JEM 100CX UHR microscope equipped with a CCD camera Keenview.

II-3.5: X-ray Diffraction (XRD)

XRD [31][32][33] is a tool used for identifying the atomic and molecular structure of a crystal, in which the crystalline atoms cause a beam of incident X-rays to diffract into many specific directions (the elements of X-ray are shown in figure . By measuring the angles and intensities of these diffracted beams, a crystallographer can produce a three-dimensional picture of the density of electrons within the crystal. From this electron density, the mean positions of the atoms in the crystal can be determined, as well as their chemical bonds, their disorder and various other information. In a single-crystal X-ray diffraction measurement, a crystal is mounted on a goniometer. The goniometer is used to position the crystal at selected orientations. The crystal is illuminated with a finely focused monochromatic beam of X-rays, producing a diffraction pattern of regularly spaced spots known as reflections (see Fig. . The two-dimensional images taken at different orientations are converted into a three-dimensional model of the density of electrons within the crystal using the mathematical method of Fourier transforms, combined with chemical data known for the sample. Poor resolution (fuzziness) or even errors may result if the crystals are too small, or not uniform enough in their internal makeup.

X-ray crystallography is related to several other methods for determining atomic structures.

Similar diffraction patterns can be produced by scattering electrons or neutrons, which are likewise interpreted by Fourier transformation. If single crystals of sufficient size cannot be obtained, various other X-ray methods can be applied to obtain less detailed information; such methods include fiber diffraction, powder diffraction and (if the sample is not crystallized) small-angle X-ray scattering (SAXS). If the material under investigation is only available in the form of nanocrystalline powders or suffers from poor crystallinity, the methods of electron crystallography can be applied for determining the atomic structure.

The diffractometer used for the XRD results (of RuOx.nH2O) was a Panalytical Xpert Pro MPD equipped with a copper anode. A Bragg Brentano configuration with a Göbel mirror was used to parallelize the beam and measure the sample at grazing incidence (omega = 3°). The Soller slits of 0.04° sides incident. The measured angular range was 25 to 95° in 2 theta with a step of 0.067° and a total acquisition time of 1h.

II-3.6: X-ray Photoelecron Spectroscopy (XPS)

X-ray photoelectron spectroscopy (XPS) [27,34] is a surface-sensitive quantitative spectroscopic technique that measures the elemental composition the chemical state and electronic state of the elements that exist within a material. XPS spectra are obtained by irradiating a material with a beam of X-rays while simultaneously measuring the kinetic energy and number of electrons that escape from the top 0 to 10 nm of the material analyzed (as shown in figure II-18). XPS requires high vacuum (P ~ 10-8 millibar) or ultra-high vacuum (UHV; P < 10-9 millibar) conditions. XPS can be used to analyze the surface chemistry of a material in its as-received state, or after some treatment. These treatments may include: fracturing, cutting or scraping in air or UHV to expose the bulk chemistry, ion beam etching to clean off some or all of the surface contamination or to intentionally expose deeper layers of the sample in depth profiling XPS, exposure to heat to study the changes due to heating, exposure to reactive gases or solutions, exposure to ion beam implant, exposure to ultraviolet light. In principle XPS detects all elements. In practice, using typical laboratory-scale X-ray sources, XPS detects all elements with an atomic number (Z) of 3 (lithium) and above. It cannot easily detect hydrogen (Z = 1) or helium (Z = 2). Detection limits for most of the elements (on a modern instrument) are in the parts per thousand range. Detection limits of parts per million (ppm) are possible, but require special conditions: concentration at top surface or very long collection time (overnight). Because the energy of an X-ray with particular wavelength is known (for Al Kα X-rays, Ephoton = 1486.7 eV), and because the emitted electrons' kinetic energies are measured, the electron binding energy of each of the emitted electrons can be determined by using an equation that is based on the work of Ernest Rutherford (1914):

Ebinding = Ephoton -(Ekinetic + ϕ) ( 10
)
where Ebinding is the binding energy (BE) of the electron, Ephoton is the energy of the X-ray photons being used, Ekinetic is the kinetic energy of the electron as measured by the instrument and ϕ is the work function dependent on both the spectrometer and the material. This equation is essentially a conservation of energy equation. The work function term ϕ is an adjustable instrumental correction factor that accounts for the few eV of kinetic energy given up by the photoelectron as it becomes absorbed by the instrument's detector. It is a constant that rarely needs to be adjusted in practice.

III: Theory of ac-electrogravimetry

III-1. A Three Species Model with a Cation, an Anion and a Free Solvent Contribution

The ac-electrogravimetric methodology and theoretical background were precisely discussed by Gabrielli et al. [35][36][37][38][39][40]. Briefly, ac-electrogravimetry consists of coupling electrochemical impedance spectroscopy (EIS) with a fast quartz crystal microbalance (QCM) used in ac-mode.

It allows the response in current, ()

E I   
, electrochemical transfer function, and in mass,

() m E   
, mass-potential transfer function to be simultaneously obtained owing to a sinusoidal potential perturbation with a small amplitude (ΔE). The combination of such transfer functions provides the possibility of a fair separation of different electrochemical processes, which involves concomitantly mass and charge changes.

III-2. Electrochemical reactions and kinetics

The transfer of two cations (c1 and c2), and an anion (a) in the electroactive films incorporating three different sites, P1, P2 , and P3 during the redox reaction of the host material P  where a single electronic transfer takes place in three independent sites can be expressed as:

c1 c1 k k P1 e c1 P1c1     (11) c2 `c2 k k P2 e c2 P2c2      ( 12
) 3 3 k k P3 a P3a e         ( 13
)
where P1c1 and P2c2 are the film matrices doped with cations, and P3a is the film matrices doped with anions. The cation and anion transfers at the film solution interface are only taken into account as rate-limiting steps since the ionic transports inside the thin film and in the solution are supposed to be fast enough through thin films or in sufficiently concentrated electrolytes. In case of electroadsorption reactions, a similar approach will be used without any potential dependence of the kinetics rate of transfer (ki and ki ' ).

The net instantaneous molar flux change of each cation, ΔJc1 and ΔJc2 and anion ΔJa can be written as follows taking into account the various concentrations and kinetic rate of transfer:

    ' 1 1 1 1 1min 1 1max 1 1 () c c f f c c c c c c c sol dC J d d k C C k C C C dt       (14)
    ' 2 2 2 2 2min 2 2max 2 2 () c c f f c c c c c c c sol dC J d d k C C k C C C dt       (15)
    ' min max () a a f f a a a a a a asol dC J d d k C C k C C C dt       (16)
By using the Hillman solvation model [41] the same relationship can be used for the solvent flux:

    ' min max () s s f f s s s s s s dC J d d k C C k C C dt       (17)
where (α) df is the film thickness; (β) Ci is the concentration of species i in the film associated to Pi site, Cisol is the concentration of species i in the solution by assuming that the diffusion of the ions in solution does not limit the global kinetics; (χ) the term (Cimax -Ci) is the concentration in free sites for species i at time t, where Cimax is the maximum concentration of the free sites in the film for species i; (δ) the term (Ci -Cimin) is the concentration of species i in the film bulk at time t, where Cimin is the minimum concentration of species i in the film. In case of a redox process, the kinetic constants which appear here depend on the potential under the classical form:

  ' 0 '' o ii b E E ii k k e       (18)   o ii o b E E ii k k e       ( 19
)
where E is the potential, Ei ° is the apparent normal potential, (E-Ei °) is the overvoltage, ki0, k'i0, bi and b'i are constants.

III-3. Dynamic regime and flux of each species

Under the effect of a sinusoidal potential perturbation with low amplitude, ∆E, imposed to the electrode/film/electrolyte system, sinusoidal fluctuations of concentration, ∆C i , and flux, ∆J i , are observed such as:

i i f f i dC J d j d C dt        (20)
The expression of the global insertion/expulsion flux, ∆Ji, which depends on the concentration and potential perturbations, at the film/electrolyte interface is:

() i ii i i i i f i C i E JJ J C E K C d G E CE                  (21)
where 1 j  , ω=2πf is the pulsation, f is the perturbation frequency and Ki and Gi are the partial derivatives of the flux, Ji, with respect to the concentration and the potential respectively,

i i i E J K C          and i i i C J G E      
, where Ji stands for the flux of the species i crossing the film/electrolyte interface. More precisely, Ki is the kinetics rate of transfer and Gi is the inverse of the transfer resistance, Rti, of the species at the film/electrolyte interface (where i is the cation c1, cation c2, anion a, or the free solvent s). Therefore, the characteristic frequency, fi, of the transfer can be estimated through the following equation:

i i f K f d   (22)
The transfer resistance, Rti, can be calculated taking into account the values of Gi:

1 i i Rt FG  (23)
For each transferred species, the ionic transfer resistance, Rti, is a good estimation of the ease of the transfer. Also, under the effect of a sinusoidal potential perturbation with low amplitude, ∆E, imposed to the electrode/film/electrolyte system, sinusoidal fluctuations of concentration, ∆Ci, are observed. In the present case, for electroactive metal oxide thin films, the change of the concentration, ∆Ci, of each species (cation 1 (c1), cation 2 (c2), anion (a), and free solvent (s))

with potential ∆E can be calculated.

  11 1 () cc fc th CG E j d K      (24)   2 2 2 () c c fc th C G E j d K       (25)
  ()

aa fa th CG E j d K      (26)
  ()

s s fs th C G E j d K       (27)

III-4. Charge/ potential transfer function,

  th q E
The charge/potential transfer function,   th q E (𝟂), is calculated for the insertion/expulsion of the two cations, c1 and c2 and an anion, a and by using the Faraday number, F, and the film thickness, df:

  12 c c a f th th th th C C C q Fd E E E E                 (28)
Then, for the two cations, c1 and c2, and an anion it comes using equations 24-27:

  12 12 c c a f f c f c f a th G G G q Fd E j d K j d K j d K                 (29)

III-5. Electrochemical impedance,

  th E I

Then, the Faradaic impedance, () F Z  , relative to the global ionic transfer of the electroactive film for three charged species, cations (c1 and c2) and anion (a) involved in the charge compensation is:

      1 F th F th th E Z q I j E          (30)
And using Eq. ( 29), we can obtain for the Faradaic impedance, ZF :

    12 12 1 ( ) ( ) ( ) F th F th c c a f f c f c f a E Z I G G G j d F j d K j d K j d K                    (31)
Finally, the electrochemical impedance can be estimated incorporating the electrolyte resistance, Rel and the interfacial capacitance, Cdl:

  1 () 1 el th dl F th E R I jC Z        (32)
or with the Ki and Gi parameters related to the two cations and an anion:

12 12 1 () ( ) ( ) ( ) el th c c a dl f f c f c f a E R I G G G j C j d F j d K j d K j d K                     (33)
When the response of the electrochemical system is perturbed at low frequencies with a parasitic electrochemical reaction, characterized by a parasitic impedance (Zpar()) described in equation (34), in parallel with the ionic transfer, the global electrochemical impedance becomes as shown in equation 35.

par par par C j R Z   1 ) (   (34)
 

          1 2 1 2 1 2 c c a s f c c a s th f c f c f a f s G G G G m d m m m m E j d K j d K j d K j d K                         (36)
where mc1, mc2, ma and ms are the atomic weight of involved species.

Partial mass/potential TF are also estimated either by removing the c2 contribution, calculating   .For that, the following equations are used:

In the case of cation c1, anion and solvent, the following equation is defined:

  1 1 1 2 2 ( ) ( ) c as c a s f c c a c s th C C C m d m m m m m E E E E                  (37)
Similarly, in case of cation c2, anion and solvent, it comes:

  2 2 2 1 1 ( ) ( ) c as c a s f c c a c s th C C C m d m m m m m E E E E                     (38)
Endly, for cation c1, cation c2, and solvent, it is written: Chapter III: TiO 2

  12 1 2 1 2 ( ) ( ) c c s c s f c a c a s th C C C m d m m m m m E E E E                     (39

I. Introduction

TiO2 is a versatile material used in numerous important and diverse technological areas [1][2][3].

As an exceptionally stable, inexpensive, nontoxic, and abundant material, TiO2 has garnered significant attention in energy-storage applications, in particular, in lithium-ion batteries and supercapacitor devices [4][5][6][7][8][9]. TiO2 is one of a few transition metal oxide materials that intercalates Li ions at reasonably low voltage (∼1.5 V vs Li/Li + ) with comparable capacities to the dominant graphite anodes. With the success of TiO2 as anode materials for Li-ion batteries, it is also interesting to investigate its utilization for Na-ion batteries.

Nanometric metal oxides for electrochemical energy storage have much shorter diffusion distances required for ion storage and they can overcome low diffusion coefficients. The slow insertion/expelling of ions in bulk metal oxide materials significantly restricts the electrochemical kinetics [10]. Therefore, it is primordial to create the structures in which a better accessibility is provided for the transfer of charged species. Various nanostructures, in the form of nanowires, nanosheets, and nanoparticles, decrease the ion diffusion distance and thus, increase the rate capability even further. A major concern with these materials is that nanostructured forms, which show higher capacity and rate capability than the bulk, exhibit irreversible capacity loss during cycling [10].

In a recent work done by T. Brezesinski et al. [11], a considerable enhancement of the electrochemical properties of self-organized TiO2 was resulted when the films were both made from nanocrystals and mesoporous (called bimodal nanoporous) architecture. Such materials show high levels of capacitive charge storage. Indeed, when nanocrystal-based films were formed without mesoscale porosity the total capacity value was low, likely because most of the film was not accessible to the electrolyte/solvent. Nevertheless, when mesoscale porosity was created in a material with "dense" walls (rather than porous walls derived from the aggregation of nanocrystals), insertion capacities comparable to templated nanocrystal materials can be achieved. This remark underscores the importance of pseudocapacitive behavior that develops in high surface area mesoporous oxide films. High pseudocapacitance behavior in TiO2 was also observed in porous TiO2 films and when the TiO2 particle sizes were below 10 nm. Through this porous structure, it might become possible to attain greater power densities while maintaining high levels of energy density in next-generation electrochemical capacitors that utilize this bimodal nanoporous architecture.

Nanoscale amorphous TiO2 electrode is also a very appealing material to develop Na ion batteries, due to enhanced ion diffusion. The nanostructured materials could propose improved power and energy densities compared with their bulk counterparts due to enhanced kinetics and large surface area. But it has also been shown that increased concentration of interfacial regions in amorphous materials may form percolation pathways to facilitate the ion diffusion [4,12,13]. On the basis of these reasons, H. Xiong et al. [4] have investigated amorphous TiO2 NT electrode as anode materials for Na-ion batteries. X. Sun et al. [14] In this chapter and for the first time this original methodology was used in order to investigate ions intercalation/electroadsorption of two different morphologies related to amorphous porous TiO2 deposited by reactive magnetron RF Sputtering Among possible routine MOx film preparation methods such as hydrothermal pathway [7,8],

or sol-gel [11], the reactive RF sputtering method could serve as an appealing alternative fabrication route. This preparation route allows a low-temperature synthesizing process of various materials with variable morphologies in nano-metric scale to be realized. The high purity deposition conditions are provided under argon atmosphere. This method has been used by H. Fakhouri et al. [20][21] to produce photocatalytic TiO2 electrodes.

Ac-electrogravimetry has the ability to detect the contribution of the charged or uncharged species and to separate the anionic, cationic, and free solvent contributions during the various faradaic or (pseudo)capacitive processes. The amorphous porous TiO2 thin films were studied in two different media, LiClO4 and NaClO4, to understand the charge-storage mechanisms and to identify the species contributions to the charge compensation process. It has been demonstrated herein that the ac-electrogravimetry responses of the porous TiO2 thin films can serve as a gravimetric probe for studying the complex charge-storage mechanisms and extracting subtleties unreachable with classical tools.

II. Structure and Morphology Study of Dense, Porous and Highly porous Thin TiO 2 Films

The In order to estimate the pore morphology of the TiO2 thin films, as now on called 'porous' and 'highly porous', they were investigated by HR-TEM (Fig. III-3b, III-3d), the growth of the intergrain spaces is easily distinguished: pore volumes of ~6-8 nm are estimated. Due to the high operating pressure which is applied for their fabrication a well-developed network of intergrain porosity is created which is quite well dispersed all over the films. During the HR-TEM imagery, SAED (selected area (electron) diffraction) was performed to follow the crystallographic state of the film. Since the atomic plan rings, not shown here, were so faint no distance was measurable, this proved the amorphousness of both analysed films.

III. Electrochemical Study of Dense, Porous and Highly Porous TiO 2 Thin Films

The

III-1. Cyclic voltammetry and EQCM study in LiClO 4

The EQCM results of a dense, porous and highly porous TiO2 film tested at room temperature

III-2. Molecular Mass Estimation

The molecular mass of the species involved in the charge compensation process can be calculated roughly. For that, the function was estimated

/ / m m t F F q Q t        
from the EQCM data. Fig. III-5 depicts the variations as a function of the applied potential for dense, porous and highly porous TiO2 thin films. According to this calculation, the only close estimation was obtained for the highly porous TiO2. In this case, a molecular mass value of ~ 6-7 g mol -1 is measured in 0.5 M LiClO4 aqueous solutions with a scan rate of 10 mV s -1 , which is close to the molecular weight of Li + . On the contrary, the results of the same calculation give

m F q    m F q   
a mass value of ~ 1-2 g mol -1 for dense and ~ 4 g mol -1 for porous TiO2. In these latter cases, the values do not correspond to any of the present species in the electrolyte.

In fact, if there is strictly one species involved, the function should be equivalent to the molecular mass of the species transferred. However, for a complex electrochemical system which is in general the case, these values correspond to an average molecular weight related to the various species. Therefore, at this point, it is arguably observed that at this scan rate (10 mV s -1 ), Li + ions are exclusively involved in the charge compensation process for the highly porous TiO2 films. However, it cannot guarantee neither (i) the absence of any other species involved in the charge compensation process for dense and porous TiO2, nor (ii) the absence of any other species aside from Li + which cannot be detected at this scan rate for highly porous TiO2 electrode (such as heavier ions including , hydrated forms of lithium ions, or free water molecules). Thus, these results show the limitations of the classical EQCM technique: it gives a global response, and does not provide unambiguous information on which of the possible scenarios which can take place. In order to investigate the details which cannot be touched by the classical EQCM method, ac-electrogravimetric studies were performed on the different analogues of TiO2 films.

IV. ac-electrogravimetric studies of TiO 2 Thin Films

To be able to have a resolution at the temporal level to deeply explore the intercalation/electroadsorption mechanism, ac-electrogravimetry (electrochemical impedance spectroscopy (EIS) coupled with fast QCM) was used to characterize our different TiO2 films.

m F q    4 ClO  m F q   
In the case of dense TiO2 films, the response in terms of transfer function was not sufficient to fairly exploit the experimental results. The reason was attributed to a limited electro activity (both in terms of current and mass responses) and probably a very compact morphological structure which may acts as an efficient barrier against facile exchange of charge species. Consequently, the results presented in the following parts include a comparative study between porous and highly porous TiO2.

Ac-electrogravimetry measurements were performed in 0.5 M LiClO4 aqueous solution, 0.5 M NaClO4 aqueous solution and also in 0.5 M LiClO4 prepared by propylene carbonate solution.

Since the most effective electroactive behaviour was observed for the cathodic potentials (see the pronounced electrochemical response and also the mass variation slope in fig. III-4) stationary potential values from -0.7 V to -1 V vs SCE were chosen for this study.

IV-1. ac-electrogravimetric studies of Porous and Highly Porous TiO 2 Thin Films in 0.5M LiClO 4 aqueous solution

The results of the ac-electrogravimetric study of porous and highly porous TiO2 thin films at -0.9 V vs SCE are summarized from figures III-6 to III-8 and the corresponding parameters in Table III- ). At this level, it is impossible to distinguish between the anion and the cation contributions and to determine the nature of the ionic species involved. Nevertheless, the Ki and Gi constants were determined for three ions in each of these films (Table III-1) and were used in the following fittings.

 

m E    q () E    q () E   
  m E      m E      m E   
configurations were tested using theoretical functions (theoretical chapter) to determine the exact contribution of each species. The mass response of both porous and highly porous TiO2 thin films were fitted by considering three species: cation 1 (c1 = Li + .H2O), cation 2 (c2 = Li + ) and the anion (a= ).

The slight contribution of the anion appears at relatively HF, followed by Li + .H2O at MF. Here, (c2 = Li + )). Since the bulk hydration numbers for Li + ions is high, n ~ 7-8 [22], the cation 1 (c1 = Li + .H2O n =1) detected in our study can be considered as partially dehydrated.

f i (Hz) Cap i (mF cm -2 ) K i (s cm -1 ) G i (mol s -1 cm -² V -1 ) (Ω cm²) (mol cm -3 V -1 )
Porous TiO 2 c 1 (cation 1) :

Li + .
  q E      E I      m E      m E   
estimating the molar weight, mi (Table III-1). The Gi parameters permit to calculate the transfer resistance, Rti, for each species (theoretical chapter). The kinetic constants, Ki, obtained from ac-electrogravimetry at -0.9V vs SCE reveal the transfer rates of species at the electrode/electrolyte interfaces. For porous and highly porous TiO2 thin films, similarly: (i) species contribute at high frequencies (the fastest species), (ii) Li + .H2O appear at the intermediate frequencies, and (iii) Li + appears at low frequencies (the slowest species). It is to be noted that the sign for the anion is negative this means that they are involved in the opposite flux of the two cations. Here, it could be hypothesized that the surface is initially positively charged (in a basic pH), so the negatively charged anions are predominantly adsorbed at the surface, these anions are then expulsed so that positively charged cations could be exchanged at the interface.

The Gi values determined from the ac-electrogravimetry study are related to the transfer resistance, ( ) which can explain the ease or the difficulty of the ionic/non-ionic transfer at the electrode/electrolyte interface. The transfer resistance, Rti, values follow the order which is the inverse of that observed for the kinetics parameters of transfer, Ki (Table III-1). In particularly, for both porous and highly porous TiO2 films, it pursues the order: Rti (Li + ) > Rti (ClO4 -) > Rti (Li + .H2O).

There are two cationic species (Li + and Li + .H2O) detected in both types of films. The kinetic parameters and resistance values for their interfacial transfer can be compared in Table III-1.

One of the noticeable differences is that the Rti (ClO4 -) value for porous TiO2 films is much higher than that for a highly porous film. This suggests that the transfer of perchlorate species at the interfaces is relatively easier in highly porous TiO2 thin films than in porous counterparts.

Thus, the transfer of large anions is favored when TiO2 thin films are more porous. Based on the Ki values, the Li + species are transferred slowly in both types of films. This could be is related to the ease of dehydration, the hydrated Li + transfer is easier compared to fully dehydrated Li + as the latter needs more energy to lost its solvation shell. The easiest species to transfer is Li + .H2O and its transfer is slightly slower in porous films. These results indicate that highly porous films facilitate both ClO4 -and Li + .H2O transfer compared to porous TiO2 thin films.

Another important parameter to compare is the value which can be considered as the quantity of species transferred per potential unit at low frequencies of 4

ClO  i G 1 i i Rt FG  ( 0) ii i CG EK       modulation.
It is evident that the quantity of the cationic species transferred per potential unit is clearly higher in highly porous TiO2 thin films than in porous films, a factor two is obtained in this case. Yet, the two films are similar in a way that for both porous and highly porous films, the higher capacitance related to the cations is obtained for Li + .H2O. Also, the quantity of the Li + transferred per potential unit is remarkably higher for porous films, which is relevant by the fact that the pore volume is increased. The contribution of anions is rather small based on the quantity transferred per potential unit (see Table III-1) ten times less compared to Li + contribution. This observation is contradictory with the kinetical information obtained for the anion. Despite the fact that the anions are more rapid compared to the cationic species in this study, only a small quantity of them are transferred at the interface. This is probably due to the large ionic radius of anions that prohibit their involvement in the charge compensation process of these films in a large quantity. It could be speculated that anions are rapidly transferred as they interact only with the film surface and for this reason, a saturation state is rapidly reached. Key parameters were also obtained for each potential as presented in figure III-10.

The characteristic frequencies, fi, extracted from ac-electrogravimetric results reveal the transfer rates of species at the electrode/electrolyte interfaces (fig III-10a and III-10e). Both for porous and highly porous TiO2 thin films, similarly: (i) species contribute at high frequencies (the fastest species), the results of our study for highly porous film show the presence of anions only at two potentials (ii) hydrated lithium ion (Li + .H2O), appear at the intermediate frequencies, and (iii) Li + appear at low frequencies (the slowest species).

A very useful information that could be obtained is the instantaneous capacitance, Capi, of each Similarly, in highly porous TiO2 the highest capacitance values are attributed to both Li + and Li + .H2O. Moreover, compared to less porous film, the capacitances of these cationic species are relatively higher. This could be attributed to the larger surface area created by the pore volumes.

Also, similar to porous TiO2 the smallest capacitance belongs to anions (fig. III-10f). The evolution of the transfer resistance, Rti, as a function of the potential is shown in fig. III-10c and III-10g. The observation could be classified as the following: (i) in both types of films studied, the lowest transfer resistance belongs to Li + .H2O, contrary to (ii) the transfer of the sole Li + is more difficult compared to Li + .H2O, this could suggest that the transfer of small Li + ions is facilitated when they are hydrated. (iii) Large ClO4 -anions are the most difficult ions to be transferred at the interface of porous TiO2 electrode, their transfer resistance decreases in highly porous TiO2. This suggests that the developed surface area due to the accumulated pores in this latter film favors a larger charged species transfer.

To quantify the role of each species, has been estimated as a function of the applied potential. The integration of against potential gives the insertion isotherm. it is actually ~2 times higher in highly porous film compared to the porous TiO2. It is important to note that the kinetics of transfer values for Li + species were slower in the studied films compared to Li + .H2O, also their transfer resistance was higher compared to other species. This point underlines the differences between kinetics and thermodynamics related to the transferred species. However, their final concentration variation is ~ 2 times higher in highly porous films than that in the porous films. Despite the differences in their dynamics of transfer, the final amplified concentration variations in highly porous TiO2 thin films corresponds to cationic species. It should be noticed that these subtleties are underlined for the very first time for these two different morphologies of amorphous TiO2 films. The Li + .H2O ions are transferred easily and in higher quantities when TiO2 films are more porous. The (Ci-C0) value for anions remains low compared with the cationic species in both types of films. Thus, only a small quantity of the anions are transferred, even if the kinetics of transfer is fast. To conclude this section, the contribution of the charged species is certainly magnified in highly porous TiO2 films compared to the porous films. This qualitative and quantitative study of ionic and nonionic species contribution in the charge compensation process, together with dynamic

0 ii i CG E K     0 i C E    4 ClO  4
ClO  information of their interfacial transfer further proves the advantageous nature of porous structure TiO2 films for storage applications. The beneficial aspect of highly porous TiO2 films is more likely related to the better accommodation of both Li + and Li + .H2O cations.

Particularly, hydrated lithium species Li + .H2O are transferred rapidly and easily at the highly porous electrode/electrolyte interfaces, and their concentration variations in the electrode is significantly increased with respect to that in their porous analogues.

IV-2. ac-electrogravimetry studies of Porous and Highly Porous TiO 2 Thin Films in 0.5M aqueous solution of NaClO 4

Ac-electrogravimetry measurements were then performed in 0.5 M NaClO4 aqueous solution at the stationary potential values from -0.7 V to -1 V vs SCE. Prior to discussing the acelectrogravimetry results in this section, the classical EQCM results of porous and highly porous TiO2 film tested at room temperature in aqueous 0.5M NaClO4 electrolytes are presented in Fig. III-11. Similar to the CV curves observed in LiClO4, the CVs presented in figure III-11 show a capacitive response in the anodic region whereas the redox reaction which is observed in the potential range from -0.1 V to -1.1 V vs ECS. The same asymmetric pattern for the CV is obtained with a broad anodic response. The capacitive behaviour is more pronounced in the CV curve of the highly porous TiO2 film compared with that for porous films (Fig. . This proposes a high contribution of surface electroadsorption process which is also accompanied with a faradaic response (shown by red arrows in Fig. in the case of highly porous TiO2 thin films. Both cathodic and anodic current density of the higher porous film are higher than those observed for less porous films, this indicates faster ions transfer kinetics. The mass variations are also influenced by the in the case of highly porous film. Moreover, in highly porous TiO2, the mass response is completely superimposed in the two directions which indicates a completely reversible process. This enhanced behaviour can probably be attributed to the increased specific surface area and the porous structure. The network of the pores provides a wide accessibility of electroactive sites and has an advantageous effect on the species exchange process. The results of the acelectrogravimetry study of porous and highly porous TiO2 thin films at -0.9 V vs SCE in aqueous 0.5 M NaClO4 electrolyte are summarized in figures III-12, III-13 and Table III- impossible to distinguish between the anion and the cation contributions and to determine the nature of the ionic species involved. Furtherly, the Ki and Gi constants were determined for two species in case of porous and three species in case of highly porous TiO2 (Table III-2) and they were used in the following fittings.

q () E

   q () E

   q () E

   q () E

  

Furtherly, to identify and clarify the contribution of the charged and also the uncharged species (i.e. free electrolyte molecules), the mass/potential transfer functions, are determined.

In the mass/potential TF, , Fig. III-13a and III-13b, one loop appears in the third quadrant at medium and low frequencies (MF and LF). This loop can be attributed to either two species or to three species where their time constants are not sufficiently different from each other. Mostly, the loops in the third quadrant are characteristic for cation contributions or free solvent molecules in the same flux direction. For the exact identification of these loops several configurations were tested using theoretical functions (theoretical chapter) to determine the exact contribution of each species. The mass response of porous TiO2 were fitted by considering only two species including a cation (c1 = Na + .H2O), and an anion (a = ClO4 -). In the case of highly porous TiO2, the mass responses were fitted by considering three species cation 1 (c1 = Na + .H2O), cation 2 (c2 = Na + ) and also free solvent molecule (s = H2O). ) and (b) highly porous TiO 2 films (involving three species, specifically Na + , Na + .H 2 O and ClO 4 -), respectively. The measurements are performed in aqueous 0.5 M NaClO 4 electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).

According to fi values presented in table III-2, in porous TiO2 the hydrated sodium appears at MF and the anion is the slowest species appearing at relatively LF. For highly porous TiO2, the Na + .H2O is identified at MF and both Na + and H2O appear only at LF. For highly porous TiO2, the partial mass/potential TFs were analyzed to validate our previous hypothesis involving three different species for these films, respectively. Partial mass/potential TFs were estimated for these films (not presented here), by removing the c2 contribution, These TFs validate the hypothesis involving multiple species and they help to obtain a better separation of the various contributions.

f i (Hz) Cap i (mF cm -2 ) K i (s cm -1 ) G i (mol s -1 cm -² V -1 ) (Ω cm²) (mol cm -3 V -1 )
Porous TiO 2 c 1 (cation 1) : The Ki and Gi constants are determined by fitting the experimental data using the theoretical functions for , , and . The kinetic constants of transfer, Ki, obtained from ac-electrogravimetry at -0.9V vs SCE reveal the transfer rates of species at the electrode/electrolyte interfaces. For porous TiO2 thin film, similarly: (i) Na + .H2O species are faster, they appear at the intermediate frequencies (ii) ClO4 -species contribute at low frequencies (the slowest species) and for highly Porous TiO2 films: (i) Na + .H2O is relatively fast and appear at the intermediate frequencies, (ii) both Na + and free solvent molecules appear at low frequencies.

Na + . H 2 O 23+18 g mol -1
1 i i Rt FG  ii i CG () EK      4 ClO    q E      E I      m E   
The Gi values determined from the ac-electrogravimetric study are correlated to the transfer resistance, (

). The transfer resistance Rti values follow the order which is the inverse of that observed for the kinetics parameters (Ki) (Table III-2). Specifically, for the porous film Rti (ClO4 -) >> Rti (Na + .H2O), this clearly suggests that Na + .H2O are the easiest species to be exchanged at the interface contrary to the high transfer resistance of the anions. In the case of highly porous TiO2, the following order persists: Rti (Na + ) > Rti (H2O) > Rti (Na + .H2O). This suggests that the Na + species are not easily transferred slowly in this film and that Na + .H2O are transferred easily. Their transfer is facilitated compared to porous TiO2.

The instantaneous capacitance values, Capi, are also presented in table III-2. For porous TiO2 the major capacity is attributed to Na + .H2O and in the case of highly porous TiO2 both cationic species Na + .H2O and Na + have high capacitances. At this potential, the instantaneous capacitance attributed to the Na + .H2O ions is higher when TiO2 film is highly porous: a factor 1.5 times is estimated here.

Another important parameter to compare is the value which can be considered as the quantity of the species transferred per potential unit at low frequencies of modulation. As previously explained, it is related to the capability to store charged or uncharged species. Particularly in highly porous TiO2 the quantity of both cationic species and free solvent molecules transferred per potential unit are much higher. In porous TiO2, only a minor quantity of anions can be transferred and the hydrated sodium is the major quantity of charged species stored. Then, pertinent parameters, listed previously, were estimated over the potential as shown in figure III-14.

The characteristic frequencies, fi, extracted from ac-electrogravimetric results reveal the transfer rates of species at the electrode/electrolyte interfaces (fig III-14a and III-14e). For porous TiO2: (i) Na + .H2O are considered to be fast with a middle frequency contribution, (ii)

ClO4 -are the slowest species appearing at low frequencies. In highly porous TiO2, the anions do not participate but: (i) hydrated sodium ions Na + .H2O, appear at the intermediate frequencies, (ii) Na + ions are followed closely by H2O molecules as the slowest species, appearing at low frequencies.

It is also interesting to look into the variation of the instantaneous capacitance, Capi, of each species as shown in Fig. III-14b and III-14f. For porous TiO2 films, the high capacitance value belongs to Na + . H2O contrary to minor values obtained for ClO4 -. In the case of high porous TiO2 films, given in figure III-14f, both of the involved cationic species including Na + and

1 i i Rt FG  ( 0) ii i CG EK       123
Na + .H2O have high capacitance values. For Na + . H2O in highly porous TiO2, the capacitance values stand relatively higher compared to porous TiO2.

The evolution of transfer resistance, Rti, as a function of potential is shown in fig. III-14c and III-14g. In porous TiO2 (i) the lowest transfer resistance belongs to Na + . H2O and (ii) the highest to . In highly porous TiO2, (i) the easiest transfer happens for Na + . H2O (ii) the transfer of Na + ions is also considered to be relatively easy and (iii) the highest resistance of transfer in this films is related to the free solvent molecules. This demonstrates the preferable transfer of cationic species.

The relative concentration change, (Ci-C0) as a function of potential for porous TiO2 is shown in figure III-14d in which an important quantity of Na + . H2O are favorably transferred while the quantity of perchlorate anions remains negligible. Therefore, in this film both kinetics (fi vs E), (Rti vs E) and thermodynamics (Ci-C0 vs E) aspects are in relatively good agreement. The same concentration profile for highly porous TiO2 shows the important and close quantity of all the involved species being transferred. While from a kinetics point of view the free solvent molecules are slower and their transfer resistance values are higher than those of Na + or Na + .

H2O, the concentration profile shows a large contribution of the free solvent molecules (Fig.

III-14h

). This observation reveals that free solvent molecules even indirectly contribute in the charge compensation process and they are probably transferred by an electrodragging process.

At this point, it is interesting to note the main differences between the two studied electrolytes.

More precisely, by comparing first the porous TiO2 in both electrolytes one could notice the kinetical differences, while anions are the rapidest species in LiClO4 electrolyte they are the slowest in NaClO4 medium, furthermore, both solvated and desolvated cations participate in LiClO4 although the presence of only solvated cations are detected in NaClO4. Also thermodynamically, from the concentration variation profiles it is noted that the main population of species transferred belongs to both Li + and Li + .H2O while in NaClO4 the major species transferred at the interface are uniquely Na + . H2O. Then, with an overview through the results obtained for highly porous TiO2 in LiClO4 the involvement of fast anionic species is detected along with Li + and Li + .H2O which participate more slowly, on the other hand, in NaClO4 there is no trace of anions the rapidest species are Na + . H2O and there is also the participation of Na + and free solvent molecules each separately. Thermodynamically, the concentration variation profiles in LiClO4 show that the most population of species willing to be transferred at the interface are Li + .H2O when in NaClO4 medium both Na + and Na + . H2O

along with independent H2O molecules are transferred in close quantities to each other. Overall, it is concluded that in porous TiO2 due to the confined intergrain porosity the only major contribution belongs to hydrated sodium and that the transfer of anionic species is difficult and unfavourable. On the other hand, the enlarged surface area provided by accumulation of pore volumes in highly porous TiO2 provides enough space and relatively facile transfer. As a consequent all the species involved contribute fairly in the charge compensation process at the interface of this electrode.

IV-3. ac-electrogravimetric studies of Highly Porous TiO 2 Thin Films in 0.5M LiClO 4 . Comparison between Aqueous LiClO 4 (aq) and Organic LiClO 4 (PC) Solutions

In some reports, typical electrochemical studies were performed in organic solvents [13,17].

No clear explanation are discussed regarding this choice in the regular reports except the solvent degradation or the potential window offered. Sometimes, the reason is related to the fact that organic solvents have bigger molecular mass compared to water molecules, this could minimize the possibility of their interference with ions dynamic.

So, to better study the ambiguous impact of an organic medium on the ions dynamics, a comparative investigation was performed. In the previous sections, it was observed that a large contribution of species were involved with highly porous TiO2 and it was concluded that the porous morphology of TiO2 could be advantageous. Therefore, here, ac-electrogravimetric Based on the CV curves presented in figure III-15a, the capacitive response obtained in LiClO4/PC electrolyte is too small compared to the response in LiClO4 aqueous solution. The noticeable asymmetric voltammogram with a broad anodic response which was observed in aqueous medium do not exist in PC organic medium. The peak current observed at the reverse anodic scan at -1 V vs SCE is almost over hundred µA higher compared to the negligible anodic current in organic medium. This suggests a higher contribution of the surface electroadsorption process which is also accompanied with the faradaic response (shown by pink arrows in Fig.

measurements

III-15a

) for highly porous TiO2 thin films in organic medium.

The mass variations are also influenced by the nature of the electrolyte (Fig. III-15b), and the QCM response is magnified ~ 4 times in aqueous solution. This enhanced behaviour in aqueous medium suggests the involvement of large number of species in LiClO4 (aq). However, at this level their identification is not possible, so the ac-electrogravimetric studies were performed.

q () E    q () E    q () E    q () E    q () E

  

for three species in both studied electrolytes (Table III-3) and they were used in the following fittings.

Furtherly, to identify and clarify the contribution of the charged and also the uncharged species (i.e. free electrolyte molecules), the mass/potential transfer functions, were measured.

In the mass/potential TF of highly porous TiO2 in aqueous LiClO4 ( , Fig. III-17a) as previously discussed one big loop appears in the third quadrant. As already mentioned, the

ClO4 -appears at relatively HF, followed by Li + .H2O at MF and Li + at very low frequencies.

The mass/potential transfer function of highly porous TiO2 in organic medium, consists of two well separated demi-circles, one in the first quadrant corresponding to an anion (a= ) and another one in the second quadrant which is attributed to (c = Li + ) and (s = PC) in the same flux direction. The anion appears to be rapid and present at relatively HF, then, followed by Li + and PC detected (fig. III-17b). ). The measurements were performed at -0.9 V vs SCE (both experimental and theoretical curves are given).

  m E      m E    4 ClO  -1,2 -0,8 -0,4 0,0 -1,
K i (s cm -1 ) G i (mol s -1 cm -² V -1 ) (Ω cm²) (mol cm -3 V -1 )
In LiClO 4 (aq) c 1 (cation 1) : a (anion):

Li + . H 2 O 7+18 g mol -1
96 g mol -1
12,5 0,32 55×10 -4 -2,64×10 -7 39,27 0,48×10 -4 In LiClO 4 (PC) c (cation): Li + 7 g mol -1 0,18 1 0,46×10 -4 0,12×10 -7 825 -2,7×10 -4 solvent: PC 102 g mol -1 0,2 -0,49×10 -5 0.022×10 -7 4700 0,5×10 -4 a (anion):

96 g mol -1
7,5 0,2 18,9×10 -4 0,98×10 -7 105,7 -0,45×10 -4 Table. III-3. Estimated values for K i (kinetics of transfer), G i (inverse of the transfer resistance), R ti (transfer resistance) and -G i /K i (quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in 0.5M LiClO 4 aqueous and organic electrolyte at -0.9 V vs. SCE for highly porous TiO 2 films.

The Ki and Gi constants are determined by fitting the experimental data using the theoretical functions for , , and with the criteria of achieving a good agreement between the experimental and theoretical data (strictly for all of the TFs, including partial mass/potential TFs). The equivalent weight of the charged and uncharged species is determined by the electrogravimetric TF, which provide the identification of the species (Table III-3). As previously discussed for highly porous TiO2 thin films in aqueous solution: (i) ClO4 - species contribute at high frequencies (the fastest species), (ii) Li + .H2O appear at the intermediate frequencies, and (iii) Li + appears at low frequencies (the slowest species). In PC electrolyte (i) ClO4 -species are slower compared to aqueous solution, they contribute at middle frequencies, (iii) Li + and PC free solvent molecules are the slowest species appearing at low frequencies.

1 i i Rt FG  ii i CG () EK      4 ClO  4 ClO    q E      E I      m E      m E   
From the values, the transfer resistance, ( ) was determined. In aqueous solution, it pursues the order: Rti (Li + ) > Rti (ClO4 -) > Rti (Li + .H2O). In organic medium, the different order appears: Rti (PC) > Rti (Li + )> Rti (ClO4 -). The PC free solvent transfer resistance is much higher when compared with the Rti values of the other species (see the values in Table III-3).

Even the Rti values of Li + and ClO4 -in organic medium are noticeably higher than their resistances in aqueous solution. Therefore, globally it could be concluded that the transfer of charged species is much easier in aqueous solutions.

Another parameter to examine is the value which can be considered as the quantity of the species transferred per potential unit at low frequencies. The quantity of the transferred per potential unit is higher in aqueous solution compared to the contribution of anions which is similar, but rather small, in both types of electrolytes (Table III-3). Despite the fact that the characteristic frequency of the anion (in each of the studied electrolytes) is higher than other species, their transfer resistance is higher than cationic species. More importantly, the film doesn't show a remarkable instantaneous capacitance for these negatively charged species.

The results obtained from the measurements at -0.9 V vs SCE, when first indicates the absence of hydrated lithium ions (Li + .H2O) in organic medium and it is the free PC molecules that to accommodate the positively charged species as following a potential step is much higher when the electrolyte was aqueous. While the capacitance of the anion remains small in both cases, the capacitance of positively charged lithium ions are magnified over ~ 5 times in

aqueous solution. i G 1 i i Rt FG  ( 0) ii i CG EK       Li  4 ClO  131
The evolution of the transfer resistance, Rti, as a function of potential are shown in fig. III-18c and III-18g. Indeed, in organic medium the transfer resistance of all the included species are much higher than what is estimated in aqueous solution.

This involves Rti (Li + )PC > Rti (Li + )aq and Rti ( )PC > Rti ( )aq. Specially, the transfer resistance of PC is very high. This could be related to the fact that the dynamic viscosity of PC (0.042 Pa. s) is almost 47 times more that water (8.9 ×10 -4 Pa. s) and this would clearly influence on the transfer resistance of the species.

The relative concentration change, (Ci-C0) as a function of applied potential (presented in fig III-18d and III-18f) quantifies the contribution of the species. In aqueous solution the major contribution belongs to both cationic species: Li + and Li + .H2O, the number of anions in µmole per cm 3 transferred at the interface being negligible. In organic PC solution, the only noticeable ions transferred at the interface are Li + , compared to this, the contribution of PC and are small. When both LiClO4 (aq) and LiClO4 (PC) electrolytes are compared, the amount of the anions contribution in both types of medium is similarly minor, but the small Li + ions contribute more (almost 2 times) in aqueous solution since the electrolyte is less viscous. Overall, in this section for the first time the impact of an organic solvent on the dynamics of transferred species was investigated both kinetically and thermodynamically. In a global point of view, these results are more satisfactory when the LiClO4 electrolyte is aqueous for the following reasons: i) the value of the anodic capacitive current (CV curves) is higher in aqueous solution, ii) the instantaneous capacitance of the species willing to be transferred at the interface of highly porous TiO2 electrode, are much higher when the electrolyte is aqueous, iii) due to the high dynamic viscosity of organic solvents the transfer resistances of species are more difficult in PC electrolyte, iv) more amount of charged species are transferred in porous TiO2 electrode when the electrolyte is aqueous. The free water molecules are not directly involved in the charge compensation process but PC molecules participate as free solvent at very low frequencies.

V. Conclusion

The results presented in this chapter for amorphous porous TiO2 thin films establish that the pseudocapacitive charge-storage mechanisms can be monitored in a deep manner by acelectrogravimetry. The technique provides the exact identification and kinetic information on the charged and uncharged species involved in the charge storage process, which is not possible with classical EQCM measurements. Electrochemical behavior of porous and highly porous TiO2 thin films in LiClO4 and NaClO4 aqueous solutions involves Li + ions, Na + ions, their respective hydrated ionic species as well as anions which were detected by our acelectrogravimetric studies. A detailed comparison was then performed in both aqueous and organic solution of LiClO4 to investigate precisely the impact organic solvent on the ion dynamics transfer. The kinetics, fi, the transfer resistance, Rti, the instantaneous capacitance of the involved species, Capi, and the variation of the relative concentration of the species (Ci-C0) of the different species transferred at the electrode/electrolyte interfaces were estimated for each studied case from our ac-electrogravimetric study.

In LiClO4 aqueous electrolyte, the contribution of the charged species is magnified for high porous TiO2 films compared to the porous films. This qualitative and quantitative study of ionic and non-ionic species contribution in the charge compensation process, together with dynamic information of their interfacial transfer further proved the advantageous nature of porous structures of TiO2 films for storage applications. The beneficial aspect of more porous TiO2 films was more likely related to the better accommodation of both Li + and Li + .H2O cations.

Particularly, hydrated lithium species Li + .H2O were transferred rapidly and easily for highly porous films, and their concentration variations in the electrode were significantly higher with respect to that in their less porous analogues.

From the results obtained in NaClO4 aqueous electrolyte, it has been concluded that in porous TiO2, because of the confined intergrain porosity, the only major contribution belonged to hydrated sodium and that the transfer of anionic species are difficult and unfavourable. On the other hand, the enlarged surface area provided by accumulation of pore volumes in highly porous TiO2 provides enough space and facilitate a relatively easy transfer. Consequently, all the species involved contributed fairly well in the charge compensation process at the interface of the highly porous electrode.

The last section is dedicated to a comparison between aqueous and organic electrolytes. The impact of organic solvent on the dynamics of transfer of the species was investigated for the first time both kinetically and thermodynamically. Globally, the obtained electrochemical results were more satisfactory when the LiClO4 electrolyte was aqueous. The instantaneous capacitance values of the species willing to be transferred at the interface of highly porous TiO2 electrode, were much higher when the electrolyte was aqueous. These results may be are due to the high dynamic viscosity of organic solvent. In the same way, the transfer resistance of the species were more difficult in the organic solvent as more charged species were transferred in porous TiO2 electrode. On the one hand, the free water molecules were not directly involved in the charge compensation process, and the Li + .H2O ions were hypothesized to be partially dehydrated. On the other hand, in organic electrolyte, PC molecules participate only as free solvent molecules. This indirectly influenced on the Li ions dynamics and slowed down their transfer.

Finally, to our knowledge, this is the first time that a fair and in situ determination of asdescribed parameters has been clearly demonstrated for different morphologies of amorphous TiO2.

These results are exciting, and the combination of fast QCM with electrochemical impedance spectroscopy offers a great opportunity for a better understanding of the ions transfer and extent of solvent molecules impact on porous materials which is not possible with single EQCM measurements. Therefore, the establishment of the ac-electrogravimetric characterization in the energy materials domain is significant for designing optimized materials for the next-generation of high energy density supercapacitors. The use of metal oxide thin films with nanoscale porosity for diverse electrochemical applications, e.g. energy storage, electrochromic devices, etc. has become a subject of growing interest [1][2][3][4]. Among these materials, tungsten (VI) oxide (WO3) is a particular metal oxide which can offer a wide range of technological applications. It is a representative metal oxide of a group of chromogenic materials due to the coloration effects associated with various processes. Aside from its potential applications including Li-ion batteries [5][6][7], supercapacitors [8][9][10][11][12][13][14][15][16][17][18][19], photoelectrochemical and solar [20][21][22][23], and fuel cells [24][25][26], WO3 has been extensively studied as a promising electrochromic material. Meanwhile, WO3 has already been integrated in low-voltage electrochromic devices for smart windows, which emphasizes the high technological relevance of this kind of material. Thus, new developments and approaches to improve such systems may have a direct technological impact.

Résumé du

The reversible electrochemical insertion or intercalation of electrolyte ions into an electrode material is the fundamental operation principle of WO3 based electrochemical devices, this includes the simultaneous insertion of cations and electrons into the inorganic matrix during the reduction step (W +6 /W +5 ), and the subsequent formation of coloring centers (W +5 ). Therefore, it is crucial to optimize the interactions between electrolyte ions and electrode materials.

For the improvement of the performance of metal oxide based electrodes, main attention has been attributed to their nanostructuration with various morphologies due to the unique properties and functionalities that can effectively be exploited in electrochemical devices. As previously discussed in the experimental chapter, electrochemical synthesis remains to be a fast, simple, low-cost and low-temperature technique which may also lead to the formation of homogenous nanoscale films with desirable qualities [27][28][29][30][31]. This approach manipulates surfactant-inorganic assemblies only in the thin interfacial region by electrochemically controlling surface interactions, which allows the formation of nanostructured films from dilute surfactant solutions. After deposition, surfactants can be easily removed from the pores by washing with a suitable alcohol, leading to the porous inorganic replicas of the surfactant phases [21]. These nanostructures, with small sizes, and large surface area to volume ratios, are expected to facilitate the ion intercalation/extraction process. These improvements are often attributed to (i) a facilitated transfer and short diffusion length for ions transport, (ii) a high electrode/electrolyte contact area, and (iii) a better stress/strain management of the material during ion intercalation/extraction.

The morphology dependent performance and ion intercalation behaviour of WO3 thin films have been investigated by several in situ or ex situ characterization techniques [32][33],

including electrochemical and optical methods [34,35,22], wide-angle X-ray scattering combined with electrochemical studies [37], Raman spectroscopy [26], and X-ray photoelectron spectroscopy studying electrochromic materials before and after cation intercalation [34,38]. However, none of these methods alone provide the information on the exact identification of the intercalated ionic species, their dynamics of transfer at the interfaces, as well as the role of electrolyte composition and the effect of ions solvation on the intercalation/extraction phenomena. The status of inserted ions is not a quite solved problem and the characterization of their transfer dynamics is not straightforward using conventional characterization tools. There is always a challenge to find an eligible technique offering mechanistic solutions in a single body that can be used to study ion intercalation phenomena in-situ and in contact with an electrolyte. There have been studies using quartz crystal microbalance (QCM) as an in situ gravimetric probe to study the insertion and/or electroadsorption of ions in metal oxide or carbon based electrodes [39][40][41][42][43][44]. These deposited materials are then studied in terms of mass changes during the electrochemical processes.

EQCM gives a global response corresponding in fact to several possible pathways such that ions, ions with solvation shells and even indirectly free solvent molecules which can contribute to the electrochemical process. Additionally, ions may lose a part of their solvation to access to the sites in smaller nanopores [44]. These possible pathways, and kinetic or dynamic aspects of the ion intercalation/extraction processes have never been characterized in the previous EQCM studies due to the limitations of the technique.

As a consequence, based on what was previously explained in the introduction part of previous chapter regarding to the originality of ac-electrogravimetry for the investigation of TiO2, in the previous chapter, this coupled methodology is exploited to study the ion intercalation/extraction behaviour of mesoporous WO3 films. Here, we particularly focus on the amorphous materials rather than crystalline ones to emphasize its role on the electrochemical performance of WO3 films [5,36]. For their fabrication, previously introduced electrochemical pathway so-called surfactant-assisted electrodeposition was chosen [21,27,29,30], which provides a facile, low

II: Structure and Morphology Study of Dense and Mesoporous Thin Films

The morphology of the electrochemically synthesized WO3 thin films was characterized by FEG-SEM and HR-TEM. In the absence of the surfactant molecules, fairly dense thin films composed of sphere-like shape nanoparticles of WO3 are obtained, which is consistent with greatly well with the reported values for the W 6+ oxidation state, indicating that the synthesized WO3 is stoichiometric [38].

III: Electrochemical studies Study of Dense and Mesoporous WO 3 Thin Films

The optical variation of the WO3 can be controlled by the application of a reversible voltage based on the double intercalation/extraction of cations and electrons into/out from the material.

The general coloration process of WO3, which is a cathodic coloring electrochromic material, is often presented in the literature by the following equation:

WO3 (colorless) + xe -+ xM + → MxWO3 (blue) (1)
where M + refers to a non-solvated cation such as H + , Li + , Na + . This simplified intercalation/extraction mechanism is based on the charge compensation process by cations.

When applying a negative voltage on WO3 layer, electrons and cations are inserted, and the electrons reduce the W 6+ ions to W 5+ . Whereas by applying a positive voltage, electrons and cations are extracted, and W 5+ ions are oxidized to W 6+ . The general view in the literature is that the integrated cathodic current density over time equates to the amount of cation intercalated to form tungsten bronze MxWO3 (Eq. 1), indicating that a higher current density means faster cation intercalation kinetics [46]. However, this simplified scheme does not take into account of (i) the ion solvation effect, (ii) the possible presence of more than one ionic species which may favour/disfavour the kinetics of the electrochromism and charge/discharge rates, and (iii) the influence of free electrolyte molecules that can interact, indirectly, with porous electrodes. Although often stated as a paradigm, to the best of our knowledge, the indirect effect of the solvent molecules on the charge compensation mechanisms has not been thoroughly studied. In the following part, these aspects of the intercalation/extraction mechanism will be discussed in detail by EQCM and ac-electrogravimetric characterizations for both dense and mesoporous amorphous WO3 thin films in aqueous LiClO4 electrolytes.

III.1. The cyclic voltammetry and EQCM study

The EQCM is a simultaneous measurement of the resonant frequency variation of a quartz resonator determined by QCM during CV measurements. A typical EQCM curve gives the potential vs current profile, simultaneous to the frequency variation vs potential response. The quartz resonant frequency variations are converted into mass changes of the electrodes by Sauerbrey relation (Eq. 1 chapter II), e.g. the mass variations of the WO3 electrodes during coloration (reduction bias) and bleaching (oxidation bias) can be monitored. The molecular mass of the species (cations and/or the other ionic/non-ionic species if present) involved in the charge compensation can be obtained roughly with further calculation. To do so,

m F q    function was determined ( / / m m t F F q Q t        
) from the EQCM data. Fig. IV-6 depicts the variation of

m F q   
values as a function of the applied potential for a dense and a mesoporous WO3 thin film. According to this calculation, an absolute molecular mass value of ~ 5-6 g mol -1 was obtained for dense or mesoporous films measured in 0.5 M aqueous solutions of LiClO4 with a scan rate of 50 mV s -1 , which is close to the molecular weight of Li + . If there is strictly one species involved, the

m F q   
function should be equivalent to the molecular mass of the species transferred. However, for a complex electrochemical system, these values correspond to an average molecular weight related to the various species, and it is actually an average in terms of mass and kinetics. Therefore, at this point, one can arguably discuss that at this fast scan rate (50 mV s -1 ), Li + ions are exclusively involved in the charge compensation process. However, it cannot guarantee the absence of any other species which may have different time constants and cannot be detected at this scan rate (such as heavier ions including , hydrated forms of lithium ions, or free water molecules). Indeed, these results

show the limitations of the classical EQCM technique. The EQCM gives a global response, and does not provide unambiguous information on which of the possible scenarios actually takes place. To investigate the subtleties that cannot be reachable by EQCM method, an ac-

III-2. ac-electrogravimetric study of dense and mesoporous WO 3 films

To be able to have a resolution at the temporal level in the intercalation/expulsion mechanism, ac-electrogravimetry was used to characterize WO3 films. Ac-electrogravimetric measurements were performed in aqueous 0.5 M LiClO4 solution, at stationary potential values in the range of 0.1 V to -0.4 V vs Ag/AgCl. ), are reported on the same graphs; a good agreement between the two sets of data is evident in term of shape and frequency distribution (Fig. IV-7). It should be noted that there is no evident part with a slope equals to 45° or below in the electrochemical impedance response; therefore, the rate limiting step is not the mass transport in the films or in the solution but rather ionic transfer between the solution and the film [42]. Re(m/E)/g cm -

(i) Ac-electrogravimetric exploration at -0.3V vs Ag/AgCl:

Gi

(mol s -1 cm -² V -1 ) -1 0.275 0.5 5.2×10 -5 0.01×10 -6 1175.6 1.1×10 -4 s (solvent):

1 i i Rt FG  (Ω cm²) i i i C G () E K      (mol cm -3 V -1 ) Dense WO3 c 2 (cation 2): Li + . H 2 O 7+18 g mol
H 2 O 18 g mol -1
3 -57.8×10 -5 1.96×10 -6 5.3 10.7×10 -4 c 1 (cation 1):

Li + 7 g mol -1
9.5 4.36 179×10 -5 2.69×10 -6 3.9 3.9×10 -4

Mesoporous WO3

c 2 (cation 2) :

Li + . H 2 O
7+18 g mol -1 0.425 6.5 8.0×10 -5 0.18×10 -6 57.5 18.6×10 -4 s (solvent):

H 2 O 18 g mol -1
1.75 -33.0×10 -5 1.32×10 -6 7.9 15.6×10 -4 c 1 (cation 1):

Li + 7 g mol -1
3.6 18 67.4×10 -5 4.10×10 -6 2.5 12.7×10 -4 a (anion):

96 g mol -1 0.15 1.8 2.8×10 -5 -0.02×10 -6 592.2 -1.6×10 -4
Table IV-1. Estimated values for f i , Cap i , K i (kinetics of transfer), G i (inverse of the transfer resistance), R ti (transfer resistance) and -G i /K i (the quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in aqueous 0.5M LiClO 4 at -0.3 V vs. Ag/AgCl for dense and mesoporous WO 3 films.

  q E    ,   E I   
, and

  m E   
with the criteria of achieving a good agreement between the experimental and theoretical data (strictly for all of the TFs, including partial mass/potential TFs).

The Gi parameters permit to calculate the transfer resistance (Rti) for each species. The kinetic constants (Ki) obtained from ac-electrogravimetry at -0.3V vs Ag/AgCl reveal the transfer rates ) which can explain the ease or the difficulty of the transfer of the ionic or nonionic species at the electrode/electrolyte interface. The transfer resistance, Rti, follow the order which is the inverse of that observed for the kinetics parameters (Ki) (Table IV ClO  anions exhibiting the highest transfer resistance.

There are two cationic species (Li + and Li + .H2O) detected in both dense and mesoporous thin films. The kinetic parameters and resistance values for their interfacial transfer can be compared in Table IV-1. One of the most remarkable differences is that the Rti (Li + .H2O) value for dense films is much higher than that for a mesoporous film. This strongly suggests that the transfer of hydrated lithium species (Li + .H2O) at the interfaces is much easier in mesoporous WO3 thin films than in dense counterparts. Thus, the transfer of larger hydrated lithium species (Li + .H2O) is favored when WO3 thin films are mesoporous. Based on the Ki (or fi ) values, the species are transferred slightly slower in the case of mesoporous films but their transfer resistance, Rti, is in the same order of magnitude, or even slightly lower than that in dense films. These results indicate that mesoporous films facilitate both (Li + and Li + .H2O) transfer compared to dense WO3 thin films. The anions contribution was detected in mesoporous films, but their transfer is slow and more difficult compared to other species.

These observations are well harmonized with the estimated instantaneous capacitances, Capi, which is the capacity of the film to accommodate each involved charged species as a consequence of a potential jump. Here, they were estimated at a chosen applied potential of 03 E . V  vs. Ag/AgCl for both dense and mesoporous WO3 (see table IV-1). This transparent criterion shows an advantageous aspect of the mesoporous film. In fact, by comparing the values, it could be easily noticed that this instantaneous capacitance is magnified over 4 times The transfer kinetics and the resistance of H2O molecules are somehow similar to those Li + of species in both dense and mesoporous films, suggesting that these are the water molecules accompanying the transfer of Li + species most likely due to the electrodragging (Table IV-1).

The quantity of the water molecules transferred per potential unit is slightly higher for mesoporous films, which is in agreement with the increased pore volume.

The results obtained from the measurements at 03 E . V  vs. Ag/AgCl, first of all indicate that there are other species than only Li + ions which intervene in the electrochemical process; such as hydrated lithium ions (Li + .H2O), free electrolyte molecules (water in the present case) or even anionic species present in the electrolyte which may contribute to the charge compensation but only in the case of mesoporous WO3 thin films. In the following, the kinetic parameters (Ki) and the transfer resistance (Rti) of the species are investigated as a function of the applied potential. There are two different cation populations (Li + and Li + .H2O) for both dense and mesoporous films at all the potentials studied. Compared to the dense films, the kinetics of transfer for Li + ions is slower in the mesoporous films and this could be related to the morphology of the films.

(ii) Ac-electrogravimetric measurements versus potential:

The hydrated lithium ions Li + .H2O in the electrolyte lose their hydration shell and get transferred at the interface, (bulk electrolyte/dense WO3 film interface). But if this transfer happens at an electrode/electrolyte interface of a confined pore wall (as in the case of a mesoporous WO3 film), the dehydration of the hydrated lithium ions in a small confined space may occur slower than that may happen in the bulk of the electrolyte. Therefore, one can arguably discuss that the different dehydration kinetics may be responsible for the differences in the   process. At all potential values studied, independent from the film morphology there are two types of cations, specifically fully dehydrated and partially dehydrated lithium species.

However, the transfer resistance values reveal significant differences between mesoporous and dense WO3 thin films (Fig.

IV-11C and IV-11D). Both Li + and Li + .H2O have lower transfer resistance, indicating the ease of their transfer at the electrode/electrolyte interfaces when the WO3 films are mesoporous. A more significant difference is observed for the larger and partially dehydrated Li + .H2O ions, suggesting that increased surface area and pore volume, created by the mesoporous morphology, favor the larger charged species transfer.

To quantify the role of each species,

0 ii i CG E K     
has been estimated as a function of the applied potential. The integration of the to note that the kinetics of transfer values for Li + species were higher (faster kinetics) in dense films compared to that in mesoporous films, and their ease of transfer was in the same order of magnitude (Fig. IV-11A, B andC). This point underlines the differences between kinetics and thermodynamics related to the transferred species. However, the final concentration variation is ~ 4 times higher in mesoporous films than that in the dense films. Despite of the differences in their dynamics of transfer, the final concentration variations are magnified in the mesoporous WO3 thin films. It should be noticed that these subtleties can be only underlined and for the very first time for both dense and mesoporous WO3 films. The (Ci-C0) values for Li + .H2O present a drastic difference between the two films, and it is ~10 times higher in mesoporous films compared to the dense WO3. Their transfer resistance at the interfaces was also significantly smaller in mesoporous films (Fig. IV-11D), indicating that these large and partially dehydrated Li + .H2O species are much easier transferred. In other words, Li + .H2O ions are easily transferred in higher quantities when WO3 films are mesoporous.

The (Ci-C0) values for water molecules are in the same order of magnitude, or no significant difference is observed. The (Ci-C0) value for anions is low compared with the cationic species, thus only a small quantity is transferred. Their kinetics of transfer was also very slow and difficult as it was shown in Table IV

-1.
Overall, the contribution of all the charged species is magnified in mesoporous WO3 films compared to dense films. This qualitative and quantitative study of ionic and non-ionic species contribution in the charge compensation process, together with dynamic information of their interfacial transfer further proves the advantageous nature of nanostructuration of WO3 films for potential applications. For most of these application (e.g. in electrochromism), it is important to have a fast switching during the coloration/decoloration process which is related to the charge compensation of the redox reaction between W 6+ / W 5+ . The beneficial aspect of Li + .H2O cations. Particularly, hydrated lithium species Li + .H2O are transferred rapidly and easily at the mesoporous electrode/electrolyte interfaces, and their concentration variations in the electrode is significantly higher with respect to that in their dense analogues.

IV. Conclusion

Mesoporous WO3 thin films were synthesized by surfactant assisted electrodeposition method.

The idea of using an ionic surfactant (SDS) during the electrochemical preparation of WO3 films led to the creation of ~5 nm spherical mesopores which are templated by the corresponding spherical micelles. The dense analogues were also electrochemically synthesized under similar conditions but in the absence of SDS templates.

The electrochromic behavior related to the cation intercalation/extraction in amorphous mesoporous and dense WO3 thin films was investigated by coupled time resolved characterization methods (fast QCM/electrochemical impedance spectroscopy). The chemical nature and the role of each species (ions, solvated ions, and free solvent molecules), directly or indirectly involved in the electrochemical processes were estimated for the very first time.

Our study identifies the involvement of several charged species (Li + , Li + .H2O) in the charge compensation, and H2O molecules indirectly contribute to the process in both dense and mesoporous WO3 thin films. Even a slight contribution of ions was detected in the case of mesoporous analogues.

Compared to the dense films, the kinetics of transfer for Li + ions are slower in the mesoporous films. This surprising result can be attributed to the transfer of ions occurring at different sites in the films. This transfer probably happens at an electrode/electrolyte interface of a confined pore wall (as in the case of a mesoporous WO3 film), the dehydration of the hydrated lithium ions in a small confined space may occur slower than that may happen in the bulk of the electrolyte. Therefore, the different dehydration kinetics may be responsible for the differences in the

  i meso K Li  and   i dense K Li 
. The transfer kinetics of the larger, partially dehydrated Li + .H2O is in the same order of magnitude in both mesoporous and dense films, indicating that these larger ions interact with the surface or close to surface sites of the mesoporous WO3 films.

Contrary to the kinetics of transfer, both Li + and Li + .H2O have lower transfer resistance, indicating the ease of their transfer at the electrode/electrolyte interfaces when the WO3 films 4

ClO  are mesoporous. Also, the instantaneous capacitance of both Li + and Li + .H2O are noticeably magnified in mesoporous WO3. A more significant difference is observed for the larger and partially dehydrated Li + .H2O ions, suggesting that increased surface area and pore volume created by mesoporous morphology facilitate the larger charged species transfer.

The relative concentration changes of Li + and Li + .H2O cations are also magnified for the mesoporous films. The final concentration variation for Li + species is ~ 4 times higher in mesoporous films than that in the dense films. For Li + .H2O, this value is ~ 10 times higher in mesoporous films compared to the dense WO3.

This qualitative and quantitative study of ionic and nonionic species contribution in the charge compensation process, together with dynamic information of their interfacial transfer further proves the advantageous nature of nanostructuration of WO3 films for potential applications.

The results of the study indicate that the transfer resistances of the cations are much lower when the WO3 films are mesoporous. This observation is probably in agreement with the previous reports in the literature indicating a fast switching during the coloration/decoloration process of the mesoporous films. Another beneficial aspect of mesoporous WO3 films is related to the better accommodation of both Li + and Li + .H2O cations. Particularly, hydrated lithium species Li + .H2O are transferred rapidly and easily at the mesoporous electrode/electrolyte interfaces, and their concentration variations in the electrode is significantly higher with respect to that occurs in their dense analogues. To the best of our knowledge, an unambiguous identification of species other than Li + ions, the information on their transfer dynamics and quantification of the transferred species have never been reported in the literature.

This study particularly focuses on the investigation of amorphous mesoporous and dense WO3 thin films. The fact that crystalline materials increase the energy barrier for lithium ions, and thus, their electrochemical capacity may be inferior compared to their amorphous analogues has been discussed in the literature [36]. The aspect of crystallinity of the films can also be studied when WO3 thin films thermally treated at different temperatures, thus possessing different degree of crystallinity. However, such an electrogravimetric study requires the utilization of the resonators as substrates that have better thermal resistance than quartz crystals, and will be the subject of a further study.

Our exiting results suggest that the establishment of the ac-electrogravimetry characterization in the nanostructured, ion-insertion materials is significant for designing optimized materials for the next generation electrochromic and energy storage devices.

Résumé du

I. Introduction:

The importance of the electrochemical capacitors based on RuO2 was previously discussed in bibliographic chapter. Briefly, RuO2 exhibits a much higher specific capacitance than any other metal oxide or various types of carbon materials. Such a superior energy-storage property is believed to be due to pseudocapacitance properties via reversible redox/capacitive reactions.

This material has also a high metallic conductivity and a low internal resistance, which can cause a rapid charge-discharge process [1][2][3][4]. However, similarly to previously studied MOx films (WO3 and TiO2), the majority of reports propose only new synthesis possibilities for reaching higher specific capacitance and one could feel the lack of powerful diagnostic techniques being able to bring information about the essential factors for which these new nanostructures are preferable [5][6][7]. For our better understanding in the first section of this chapter, both classical EQCM and EIS techniques were exploited to study the ion transfer behaviour of as-prepared mesoporous hydrous RuOx.nH2O films. For their fabrication, similar to previously discussed WO3 chapter, surfactant-assisted electrodeposition was chosen which provides a facile, low temperature and rapid alternative to the mesoporous thin film synthesis.

The structure, the morphology and the composition of these mesoporous electrochemically synthesized films were characterized, and compared with their compact counterparts. The electrochemical performance and ion intercalation/electroadsorption mechanisms were studied in aqueous H2SO4 and Na2SO4 electrolytes by electrogravimetric methods (EQCM and ac-electrogravimetry). A particular attention was paid to some ambiguous aspects, such as the nature of the ions involved in the charge compensation process, the solvation effects and the role of the electrolytes associated to the dynamic of ions transfer at the electrode/electrolyte interface. It has been demonstrated herein that the ac-electrogravimetric responses of the electrodeposited RuOx.nH2O thin films can serve as an attractive probe to study the complex H + and Na + transfer mechanisms and to extract subtleties unreachable with classical tools. So, the first part is attributed to the influence of nanostructuration on the dynamics of ions transfer.

Furtherly, the studies are completed by investigating the impact of the electrolyte's cation size.

Another interesting aspect that would be discussed is the impact of CNTs as a supporting electrode. A 3D array of electrode allows more active materials to be loaded per unit area. An attractive approach to increase the capacitance is to deposit a pseudo-capacitive material onto a high surface area structured support. So, the second part of this chapter includes the electrogravimetric investigations of CNTs/RuOx•nH2O composite electrode by using the previously mentioned classical and non-classical diagnostic tools in order to pursue the ion's kinetics evolution involved with this 3D structure. The composite film is made from a very thin layer of hydrous ruthenium oxide RuOx•nH2O electrodeposited onto CNTs layers for the purpose to combine the high pseudocapacitance (also called redox-type capacitance) of RuOx•nH2O with the double-layer capacitance of carbon layers [8][9][10][11]. By this way, electrodes with low contents in RuOx•nH2O were prepared with the instruction already explained in the experimental section. Also, the evolution of different key parameters, already seen, are also investigated for bare CNTs and bare RuOx•nH2O which will provide a complete comparison for our better understanding. To do so, a composite of SWCNTs/RuOx.nH2O prepared simply via the electrodeposition of a fine layer of RuOx.nH2O onto SWCNTs/Au/AT-cut 9MHz quartz crystal is studied to understand the synergic effects of CNTs.

II. Structural Characterizations:

Prior to electrochemical characterizations, the as-prepared hydrous ruthenium oxide, partially dehydrated ruthenium oxide (heated at 150°C) and anhydrous ruthenium oxide (heated at 450°C), were studied by different structural characterization techniques including XRD, XPS, SEM-FEG, TEM, SAED and HR-TEM. In order to easily distinguish the terminology used for studied hydrous and anhydrous films, the RuOx.nH2O formula is used whenever hydrous asprepared and hydrous 150°C heated ruthenium oxide films are investigated. The RuO2 formula is employed only when the sample is heated up to 450°C and therefore completely anhydrous.

II-1. XRD Characterization of as-prepared RuO 2 .xH 2 O and RuO 2 heated at 450 °C:

Both as-prepared RuOx.nH2O and anhydrous RuO2 films crystallinity were analyzed using Xray diffraction. The films were prepared at different deposition times on large-surface Au substrates as described in chapter II. The X-ray diffraction spectra are shown in Fig. V-1. In order to minimize the peak intensities of Au substrate the results of a thick film deposited during 60 min were chosen. Nevertheless, the presence of pronounced peaks at 38°, 45° and 65°coming from Au substrate are inevitable. The apparition of peaks at 58° and 70°, indicates clearly that the as-deposited film is not amorphous, contradicting the observations made by Zhitomirsky et al. [12] and Hu et al. [13,14]. Based on previous XRD analysis for RuO2, the presence of peaks at 58°, 70° could be attributed to the both hexagonal ruthenium oxide and also metallic ruthenium [12,14,15]. The broadening of RuO2 peaks suggests that the deposited films consist of grains with nanometer size. The crystallographic state of as-prepared RuOx.nH2O is not clearly the same as annealed RuO2 and this is mainly due to the presence of structural water.

Therefore, it could be concluded that in as-prepared samples both RuO2 and Ru peaks exist, the structural evolution happens when the sample is annealed in air up to 450°C, as a result the appearance of peaks at 28°, 35° and 54.4° correspond to rutile RuO2. Also the hidden low intensity peak at 42° in both cases is related to hexagonal structure of Ru.

II-2. SEM-FEG Characterization:

(i) Compact and Mesoporous RuO x .nH 2 O:

All RuOx•nH2O deposits were examined by SEM to examine the film morphologies. It should be noted that in compact RuOx•nH2O (figure V-2a and V-2b), the surface morphology seems quite different than that of mesoporous RuOx•nH2O prepared by surfactant assisted deposition (as shown in figure V-2c and V-2d). Network-like morphology with a forest like branches in as-prepared RuOx•nH2O give their place to attached-spherical like grains with larger domains of intergrain porosity in mesoporous counterparts. This could be related to the impact of surfactant CTAB molecules in order to procure controlled porosity. The SEM-FEG results highlight that morphologies of RuOx•nH2O are also affected by the rate of deposition. In the absence of CTAB molecules this rate is very high and the film thickness continues to grow fast (based on EQCM results not show here) (figure V-2a and V-2b). On the other hand, in the presence of CTAB the formation of cationic spherical micelles at the interface forms an inhibitor layer so that the electrodeposition slows down as it could only take place around these spherical micelles [16,17]. After the deposition, when the sample is rinsed properly and dried in air for CTAB removal, a porous morphology is obtained. These obtained three-dimensional (3D) porous RuOx•nH2O are known to enable the ions transport by providing pathways between the material and the electrolyte for the sake of enhancing the pseudocapacitance. As it could be seen in figure V-3, the film thickness estimation of as-prepared RuOx•nH2O is not easy since the film is not homogenous, the average thickness is estimated for different deposition times revealing the spontaneous growth of the film (figure V-3).

(ii) SWCNTs / RuO x .nH 2 O:

The preparation of the composite film was previously explained in the experimental section.

II-3. Targeting Evolution of Morphology and Crystallography by TEM & SAED: The effect of calcination

The XRD results do not give a clear idea of amorphous and/or crystalline properties for asprepared RuOx.nH2O. However, contradicting what is reported in several publications about the amorphousness of RuOx.nH2O [12][13][14], the appearance of even small peaks in previously discussed XRD results proves the existence of crystalline domains. Therefore, SAED studies are pursued for further investigation of this aspect.

(i)

The Effect of Heat Treatment on Compact Ruthenium oxide: the corresponding electron diffractions where diffuse rings at 150°C (because of small size of crystallites) turn to very well pronounced distances for the calcined analogues at 450°C. In this case, nanoscale domains create a network of highly porous structure as already mentioned [18,19]. We note also the change of the crystallographic structure of the film (Ru (hcp) to RuO2

(tetragonal) like the compact film.

(iii) The Effect of Structuration on Hydrous Ruthenium Oxide Films:

Finally, a comparison between both compact and mesoporous RuOx.nH2O is shown in figure V-7 in which both morphological and crystallographic information are shown. There is no trace of small nanosize domains with intergrain porosity in compact film, the SAED pattern on the other hand reveals more clear rings with measurable distances in compact film suggesting that the compact RuOx.nH2O is more crystalline.

II-4. HR-TEM Results

(i) Mesoporous Ruthenium oxide:

In order to observe more precisely the pore characteristics, HR-TEM images of both non-porous and mesoporous RuOx.

II-5. XPS Characterization, The impact of Heat Treatment

As previously discussed in the experimental section the mechanism of RuOx.nH2O electrodeposition is not fully understood [12][13][14]20,21]. Hydrated ruthenium chloride, the salt used in the solution of electrogeneration, is a heterogeneous ionic material with an average ruthenium oxidation state between 3 and 4, close to 4. The oxidation degree of annealed RuO2 ) and anhydrous RuO2. Hydrated RuO2 exhibit a broad peak envelope whilst rutile RuO2 is composed of sharp, asymmetric narrow features reminiscent of metallic ruthenium. There is no apparent difference for the Ru (3p) level, with identical peak shapes and BEs observed (not presented here). The broader 3d peak structure of the hydrate initially suggests the presence of multiple oxidation states, and many have assigned higher BE features to the presence of RuO3.

However, RuO3 is known not to exist in a stable bulk phase and previous reports have relied on its isolation in the physisorbed state [25]. Kim et al. [26] studied carbon-free, stoichiometric

RuO2 and determined the broad structure of the Ru (3d) to be due to satellite structure from core-hole screening rather than mixed oxidation states. This process is also applied to the O (1 s) region, with a Shirley background, lattice oxygen and satellite component line shapes equivalent to those used for the Ru (3d) level. This methodology has been previously applied to conducting oxide systems including RuO2 [15]. OH groups for the anhydrous sample is low. Therefore, it is proposed that the majority of the intensity of this feature for the anhydrous oxide is primarily due to many-body screening effect of the conduction electrons as observed.

In respect of the hydrated oxide (figures V-11 and V-12), the reverse is true, and the major intensity of this peak is due to hydroxyl groups; however, a small percentage of this overall intensity, as for the anhydrous rutile oxide, is attributed to the screened structure. Clearly, the model applied herein for both anhydrous and hydrated ruthenium oxide is in excellent agreement with the expected Ru/O stoichiometry supporting the peak shapes and assignments recently published in ref [15] (see Table V-1). Therefore, in the confirmation of previously discussed results of conventional XRD and SAED on heated samples, herein our XPS spectra also confirmed the presence of hydrated ruthenium oxide in the surface of both as-prepared and 150°C heated samples. The annealed samples at 450°C confirm the existence of anhydrous RuO2 with rutile structure. . By this way, the mass changes of the electrodes during ions transfer can be monitored.

III. Electrochemical Characterization: Cyclic Voltammetry and Classical EQCM Study

It is to be noted that most effective electrochemical behaviour for RuOx.nH2O especially in terms of specific capacitance is reported in H2SO4. Even though, the same high value of current is not observed in other sulfate mediums including Li2SO4, Na2SO4 or K2SO4, here, the electrochemical behaviour is also studied in Na2SO4 in order to study the cation size effect. following observations can be extracted. On the one hand, in compact RuOx.nH2O, the mass variations in H2SO4 are 1.5 times more important than in Na2SO4: it could be assumed that the amount of small ionic radius H + ions transferred at the interface is more important than larger Na + ions. Maybe it is mainly due to confined intergrain species in compact RuOx.nH2O compared to mesoporous film. This assumption could be also supported by previously shown HR-TEM images. On the other hand, mesoporous RuOx.nH2O, with a larger specific surface area developed by nanometric pore volumes accommodate equally even larger species including Na + whether hydrated or accompanied by free solvent molecules. As a consequence, the same quantity of mass variation is observed for both H2SO4 and Na2SO4 medium.

Among similar works there are only few reports on the use of classical EQCM as an electrochemical tool to study Ru/RuO2 behaviour. J. Juodkazyte et al. [20] studied and compared the voltammetric and microgravimetric behavior of active Ru, electrochemically passivated ruthenium (Ru/RuO2) and thermally formed RuO2 electrodes in a H2SO4 electrolyte.

In their study, cycling the potential of thermally formed RuO2 electrode led to continuous decrease in electrode mass, this has been attributed to irreversible dehydration of RuO2 layer.

M. Vukovic at al. [28] used cyclic voltammetry and EQCM measurements for the characterization of electrodeposited ruthenium under the conditions of repetitive potential cycling in 0,5 M sulfuric acid solution. Several types of non-stoichiometric surface reactions, which include the formation of various ruthenium oxyhydroxide species, were proposed. The stability of the electrodeposited ruthenium layer (prepared galvanostatically) was investigated.

Their electodeposited Ru on gold plated quartz crystal exhibited a capacity of 870 F g -1 which is comparable with the capacitances reported for hydrous ruthenium oxide [22][23][24].

III-2. Specific Capacitance Calculation

Also, as previously mentioned in the bibliography section and reported by several publications, it is in its hydrous form (RuOx.nH2O) that this oxide exhibits the highest capacitance values that have been described. Recently, Zhang et al. [24] attributed the increase of the specific capacitance to a contribution of the RuO2 bulk: the bulk of RuOx.nH2O can be permeable to the electrolyte ions due to some highly hydrated channels. The specific capacitance of RuOx.nH2O films could be calculated from previously shown CVs by the following equation [25]:

𝐶𝑠 = 𝐼∆𝑡 𝑚∆𝑉
where Cs is the specific capacitance calculated from I, applied current (A) divided by scan rate (V s -1 ) and normalized by the quantity of mass (g) electrodeposited. It is to be mentioned that mesoporous films are produced by surfactant assisted electrodeposition and that the mass of mesoporous film is calculated after rinsing and thermal treatment of the film for CTAB removal. Since this step is not controlled electrochemically the quantity of mass deposited might not be the exact value as the mass obtained by classical electrodeposition. The estimated instantaneous specific capacitance for two types of films are presented in Fig. V-16. A specific capacitance of ~ 300 F g -1 for non-porous RuOx.nH2O is obtained in acid medium which is over 6 times higher than the value ~ 40 F g -1 obtained in Na2SO4. For mesoporous RuOx.nH2O the estimated specific capacitance is 818 F g -1 . This value is much more important than ~280 F g -1 which are calculated in Na2SO4 for the same film and over 2 times higher than the value estimated for compact RuOx.nH2O in H2SO4. Also, the obtained value for mesoporous film stands higher and/or in some cases as high as other estimations reported for hydrated RuO2 in the literature (see Chapter I) [23,24,[29][30][31]. What could be concluded from these estimations is the advantageous aspect of mesoporosity. Having larger surface area due to pore volumes obviously provides easiness of transfer and transport for the involved species and facilitates their transfer/transport. constants and cannot be detected at this scan rate (such as heavier ions including SO4 2-, hydrated forms of proton or sodium ions, or free water molecules).

In a similar report, M. C. Santos et al. [21] used EQCM for the study of RuO2 thin films, prepared by a sol-gel precursor method. According to their study, the CV corresponded to different redox transitions including: Ru 2+ /Ru 3+ , Ru 3+ /Ru 4+ and Ru 4+ /Ru 6+ with formal redox potentials of 0.56, 0.85 and 1.2 V vs NHE. From their EQCM measurements performed in acidic medium (H2SO4) at 25°C, the relative molecular mass of the transferred species was calculated from the slope of ∆m vs ∆Q, (the mass variation as a function of charge transferred in RuO2 thin film electrodes). Their results showed that the proton identification occurs only in the intermediate potentials (in their case 0.8-1.1 V vs NHE) associated with the Ru 3+ /Ru 4+ transition. They also suggested that hydroxide ions can also participate even with this same negative slope. This result is in fact debatable since this approach cannot discriminate clearly the ion contribution. Also, for more cathodic potentials a molecular mass of 32 g mol -1 was obtained which is attributed to water molecules detection, but this is not a precise identification.

Indeed, these results show the limitations of the classical EQCM technique. The EQCM gives a global response, and does not provide unambiguous information on which of the possible scenarios actually takes place. To investigate the subtleties that cannot be reachable by EQCM method, ac-electrogravimetric studies were performed on mesoporous RuOx.nH2O films and compared with their compact analogues.

IV. ac-electrogravimetric results for compact and mesoporous RuO x .nH 2 O

To further investigate and identify the nature of species involved in the charge compensation process at the interface of compact and mesoporous RuOx.nH2O, ac-electrogravimetric results are presented in this section.

IV-1. ac-electrogravimetric results for compact and mesoporous RuO x .nH 2 O in H 2 SO 4 0.5 M aqueous solutions:

For a chosen potential, for example 500 mV, the charge/potential transfer functions (TFs),   q E    , are given in Fig.

V-18a and b. These TFs allow the ionic contribution without any possibility to identify the ionic species involved to be done. Here, the contribution of a parasitic reaction, occurring at very low frequencies, was removed for keeping only the ionic transfer response. A large and slightly suppressed loop was obtained for both compact and mesoporous RuOx.nH2O thin films without a fair separation of different ionic transfers. From the theoretical functions (continuous line in fig.

V-18) it seems that there are more than one charged species involved in both cased. However, the time constants corresponding to each ionic transfer appear to be very close to each other. At this level, it is not possible to distinguish whether the contribution of the involved species correspond to anions or cations. Meanwhile, the Ki and Gi constants were determined for two ions (for compact) and three ions (for mesoporous). The values of these parameters are shown in Table V-2 and were used in the following fittings. This set of parameters were kept for all the TF fitting for a certain film.

The i K and the i G constants are determined by fitting the experimental data using previously defined theoretical functions for

  q E    ,   E I    and   m E   
with the criteria of achieving a good agreement between the experimental and theoretical data (strictly for all of the TFs, including partial mass/potential TFs). The equivalent weight of the charged and uncharged species is determined by the electrogravimetric TF,

  m E   
which provides the identification of the species (Table V-

Gi

(mol s -1 cm -² V -1 ) Then, to identify and clarify the contribution of the charged and also the uncharged species (i.e. determined. Indeed, the apparent mass of H + is negative due to the method of calculation of the partial TFs; a negative value given by 1-19= -18 g mol -1 must be used in this case for representing the H + gravimetric response which leads to an apparent anion response located in the fourth quadrant. The characteristic frequencies, fi, obtained from ac-electrogravimetry at 500 mV vs Ag/AgCl reveal the transfer rates of species at the electrode/electrolyte interface. For both dense and mesoporous RuOx.nH2O thin films: (i) H + species contribute at high frequencies (the fastest species), (ii) free water molecules appear at the intermediate frequencies, and (iii) H3O + appears at low frequencies (the slowest species). In the case of mesoporous RuOx.nH2O thin films, an additional contribution is observed at the lowest frequency range corresponding to the anions transfer (SO4

1 i i Rt FG  (Ω cm²) ii i CG () EK      (mol cm -3 V -
q () E      m E    193 0 1 2 3
  m E      m E    instantaneous capacitances, Capi, presented in Table V-2,
values are quite identical for the two films. The major contribution is due to the H + species with the highest values 6 and 10 times higher compared to capacitance of H3O + for the compact and mesoporous films respectively.

The faster species transferred are the smaller one, H + , this could indicate that it is related to electroadsorption process. On the contrary, the slowest transferred species, i.e. H3O + , can be associated to a redox process. To confirm this hypothesis, the transfer resistance, Rt, of H3O + for the compact film reaches the biggest value (366  cm +2 ) as a very small value is obtained in the case of H + for mesoporous films (0.26  cm +2 ).

To explore more deeply the global electrochemical process in the whole potential range, the electrogravimetric evolution for each applied potential was examined. According to TFs, for compact RuOx.nH2O at 300 mV, there is no trace of solvent and two cations are identified: H + , at a few Hz which is the main contribution and H + again around 0.1 Hz. The partial mass/potential transfer functions give nothing since here the two cations involved are identical. It could be suggested at this stage that one of these H + corresponds to the redox sites and another one to the capacitive sites. The instantaneous capacitance, Cap, related to the faster H + is 18 mF cm +2 and for another 4.5 mF cm +2 . Similarly to the experiments shown previously at 500 mV, the main contribution is related to the fastest species. At 400 mV, the same conclusion as at 300 mV persists with the exception of a small solvent contribution. At 500 mV, same conclusions as for the previous potential: at HF, H + is detected around 6 Hz with an associated capacitance of 17 mF cm +2 , however, the other H + cation, around 0.15 Hz, is now hydrated. Free solvent is also detected with the same magnitude as at 400 mV. At 600 mV: the same conclusion persists compared to 500 mV. At 700 mV, anion contribution is detected at HF and is followed by an H + response. It should be noted that the anion contribution is around 0.1 mF cm +2 and therefore very small compared to H + contribution, 13 mF cm +2 . At 800 mV, the observation is similar compared to 700 mV.

For mesoporous RuOx.nH2O, , TFs were also studied for the same potential window.

At 300 mV, the participation of 4 species are detected with the following order: H + is observed around 40 Hz with an instantaneous capacitance of 13 mF cm -2 , then, at middle frequencies around 13 Hz free solvent appears. At LF, H3O + is identified with an instantaneous capacitance of 2.4 mF cm -2 , and finally at very LF there is a slight participation of anion with only a

  m E      m E   
capacitance value of 0.07 mF cm -2 . This sequence in terms of rate of transfer is illustrated in figure V-20. For all the other potentials, the same configuration of 4 species persists. By comparing these values in the case of compact RuOx.nH2O film, it could be seen that the most important capacitance belongs to H + ions meaning that compact film having still nanometric intergrain spaces could more easily accommodate small protons but since the hydrated ions have larger ionic diameter the capacitance values remain somehow small for H3O + . The anions appear only for the last two anodic potentials and the instantaneous capacitance attributed to them remains very small. The similar sequence is observed for mesoporous RuOx.nH2O with instantaneous capacitances in the same order of magnitude.

The Gi parameters permit to calculate the transfer resistance, Rti, of each species (Fig. V-22).

The Gi values determined from the ac-electrogravimetric study are related to the transfer resistance, (

1 i i Rt FG 
) which can explain the ease or the difficulty of the ionic/non-ionic transfer at the electrode/electrolyte interface. The transfer resistance, Rti, values follow the order which is the inverse of that observed for the kinetics parameters (Ki) (Table V-2). Specifically, for compact films, it pursues the order: Rti (H3O + ) >Rti (H2O) >Rti (H + ), and for mesoporous films the similar order persists: Rti (SO4 2-) >Rti (H3O + ) >Rti (H2O) >Rti (H + ), except the presence of additional SO4 2-anions exhibiting the highest transfer resistance. There are two cationic species (H + and H3O + ) detected in both dense and mesoporous thin films. The kinetic parameters of transfer, fi and the transfer resistance, Rti, values for their interfacial transfer can be compared in Fig V-20 and V-22. One of the most remarkable differences is the Rti values associated to H3O + for compact films which are higher than that of mesoporous film. This strongly suggests that the transfer of hydrated proton species at the interface is much easier in mesoporous RuOx.nH2O thin films than in compact counterparts. Thus, the transfer of larger hydrated proton species H3O + is favored when RuOx.nH2O films are mesoporous. Based on fi values, the H + species are transferred rapidly in the case of mesoporous films but their transfer resistance is in the same order of magnitude compared to compact films. These results indicate that mesoporous films facilitate both H + and H3O + transfer compared to compact RuOx.nH2O films. The Rti (H2O) is higher in mesoporous film suggesting that mesoporous film selectively favors ionic species participation but not free solvent molecules. The SO4 2-anions contribution was detected in mesoporous films for all the potentials, but their transfer is slow and more difficult compared to other species. CC  ) values for H + and H3O + cations are magnified for mesoporous films. Specially, the number of exchanged H + ions are increased for ~ 3 times in mesoporous films. It is important to note that the characteristic frequency values, fi, for H + species were higher (faster kinetics) in mesoporous films compared to compact films, and their ease of transfer was in the same order of magnitude (Fig. . This point underlines a good agreement between kinetics and thermodynamics related to the transferred H + species. However, despite the relative rapidity of H3O + and H2O in mesoporous film compared to compact film, in terms of thermodynamics the major contribution remains to be attributed to H + ions indicating that large number of these small species are transferred. The ( 0 i CC  ) values for H3O + are only slightly higher in mesoporous films than that in the compact films. The ( 0 i CC  ) value for SO4 2-anions is low compared with the cationic species, thus only a small quantity is transferred. Overall, the contribution of the charged species is magnified in mesoporous RuOx.nH2O films compared to the compact films. This qualitative and quantitative study of ionic and non-ionic species contribution in the charge compensation process, together with dynamic information of their interfacial transfer further proves the advantageous nature of structuration of RuOx.nH2O films for energy applications. The beneficial aspect of mesoporous RuOx.nH2O films is more likely related to the better accommodation of both H + and H3O + cations. Particularly, H + ions are transferred rapidly and easily at the mesoporous electrode/electrolyte interfaces, and their concentration variations in the electrode is significantly higher with respect to that in their compact analogues. The resulted deconvolution of species from our ac-electrogravimetric results led to distinguish and attribute the two cationic species with different time constants to two possible reactions at the interface of (pseudo)capacitive RuOx.nH2O. Indeed, the interaction of these two species occurs undoubtedly at two different sites in the film, since H + ions are the fastest species they could be attributed to fast capacitive reactions and the slower H3O + ions to the faradaic reaction.

IV-2. ac-electrogravimetric results for compact and mesoporous RuO x .nH 2 O in Na 2 SO 4 0.5 M aqueous solution:

It is to be pointed out that in the majority of reports covering pseudocapacitive behavior of hydrated ruthenium oxide as a subject, the most important specific capacitance values are reported in H2SO4 electrolyte [6,20,21]. In previously discussed section, it was concluded that small protons are kinetically favorable, they are more easily and rapidly transferred at the mesoporous electrode/electrolyte interface. In this part, in order to see the effect of cation size the same electrodes were studied in Na2SO4 electrolyte and the results of this investigation are presented and discussed. The Ki and Gi constants were determined for three/four species (for compact) and only two charged species (for mesoporous). The values of these parameters are shown in Table V- q () E

   q () E

  

Ac-electrogravimetric results of a compact RuOx.nH2O film were fitted by considering four species listed in term of rapidity: sulfate anions (a= SO4 2-), free solvent molecules (s= H2O) sodium cations partially dehydrated (c1= Na + ) and hydronium cations (c2= H3O + ). However, in the case of mesoporous RuOx.nH2O film, a completely different response was obtained. Only two charged species appear: cations (c1= Na + ) and anions (a= SO4 2-) appear at lower frequencies in the fourth quadrant (Fig. V-24d).

The different responses over the total applied potential window could be summarized as following. For compact RuOx.nH2O, at 300 mV, there is no trace of solvent and the anion appears at HF around 40 Hz. Two cations are identified: Na + at ~15 Hz with the main contribution and also a small one related to H + at 0.1 Hz. The instantaneous capacitance related to Na + is 4.3 mF cm +2 while for both H + and SO4 2-this capacitance is very small, 0.6 and 0.2 mF cm +2 respectively. At 400 mV, the same conclusion as at 300 mV persists. At 500 mV, an anion appears at HF with a very small instantaneous capacitance of only 0.24 mF cm +2 . Na + is detected at ~13 Hz with an associated capacitance of 4 mF cm +2 and now the other H + cation is now hydrated with an associated capacitance of 3.9 mF cm +2 . At 600 mV: the same conclusion persists compared to 500 mV. At 700 mV anion contribution at HF is followed by Na + around 21 Hz and finally, H3O + response at LF (0.4 Hz). At 800 mV, the observation is similar to 700 mV.

For mesoporous RuOx.nH2O the participation of only two charged species are detected for all the studied potentials. This includes Na + observed around 15 Hz with an instantaneous capacitance of ~5 mF cm -2 followed at LF by sulfate anion participation with a small instantaneous capacitance of ~ 0.3 mF cm -2 . The main difference between the two types of films The characteristic frequencies, fi, obtained from ac-electrogravimetry at 500mV (presented in fig.

V-25) reveal the rate of transfer over the applied potential. For compact RuOx.nH2O films:

(i) SO4 2-species contribute at high frequencies (the fastest species), (ii) Na + ions appear at the intermediate frequencies, and (iii) H3O + appears at low frequencies (the slowest species). In the case of mesoporous RuOx.nH2O thin films Na + is the rapidest species and the contribution observed at the lowest frequency range corresponds to the anions transfer (SO4 the most important values are attributed to Na + . Also, in mesoporous RuOx.nH2O, the instantaneous capacitance grows gradually and reaches a maximum of 5.2 mF cm -2 for the most cathodic potential at 300 mV. For the anions, this capacitance remains very small in both types of film suggesting that the film's capacity to accommodate SO4 2-species is not noticeable. The i G parameters were used to calculate the transfer resistance, Rti, for each species, (not shown here.). For compact films, it pursues the order: Rti (H3O + ) >Rti (SO4 2-) ≈ Rti (H2O) >Rti (Na + ), and for mesoporous films: Rti (SO4 2-) >Rti (Na + ), except the presence of additional SO4 2- 203 anions exhibiting the highest transfer resistance. These results indicate that for both films Na + transfer is facilitated. This explains why the number of H3O + species exchanged at the interface is smaller compared to Na + ions. This is also supported kinetically by already noticed high Rti of H3O + . The free solvent molecules appear for only three potentials with minor contributions. For SO4 2-anions, the concentration changes appear for all the potentials but with small changes. At the interface of mesoporous RuOx.nH2O electrode/electrolyte the major exchanged species are Na + and SO4 2- exchange remains very small. At this stage, when both kinetic and thermodynamic information are compared it could be suggested that the contribution of Na + may correspond to the redox sites while SO4 2-ions are related to the capacitive sites, and their identification is only due to their adsorption at the surface, therefore, the major role is owing to Na + ions.

To conclude this section, the major contribution in both compact and mesoporous RuOx.nH2O films is related to Na + cations. The qualitative and quantitative study of ionic and non-ionic species contribution in the electrochemical process in Na2SO4 solution doesn't clearly show the advantageous nature of RuOx.nH2O films structuration. First, this could be related to the neutral Although these values might not stand among the highest values reported in the literature for SWCNTs/RuOx.nH2O [8][9][10]33] composite which could be due to the simplicity of our preparation method and the small RuOx.nH2O quantities used here. But here the main goal was not to reach high performances rather to understand deeply the electrogravimetric behaviour of these films. So, what is promising here is the fact that electrodeposition of even a very thin layer of RuOx.nH2O on pure SWCNTs electrodes enhances the current values as well as the capacitances. It is also believed that this improvement in the electrochemical behaviour of the RuOx.nH2O/CNT film electrode is attributed to the large interfacial area between the ruthenium oxide and the solution due to the high surface area of the initial CNT film substrate.

In a recent report by I-H Kim et al. [33] an electrochemical route was employed to procure a 3D structure for RuO2. The author mentioned that a very thin, nanometric, ruthenium oxide layer on the CNTs substrate contributed to largely increase the specific capacitance. The author have also indicated that a large portion of RuO2 under the film surface layer is unreacted and left behind a dead volume, which eventually causes reduction of the specific capacitance.

Therefore, the RuO2/CNT films exhibit enhanced properties because of using the CNT film substrate which provides three-dimensionally interconnected nanoporous structure. When mass changes were recorded in aqueous 0.5M H2SO4 (fig.

V-28b) it could be seen that SWCNTs/RuOx.nH2O behaves similar to SWCNTs, meaning that when the potential is cycled from anodic to cathodic values, the frequency increases meaning that the mass of the film drops due to expulsion/desorption of charged species and/or free solvent molecules. Surprisingly, in 0.5M Na2SO4, the composite behaves differently corresponding to what was previously observed for RuOx.nH2O. In this case (the green curve in fig. 28b) when the potential is scanned to cathodic direction, the frequency drops so that the mass of the film increases, One could conclude that the SWCNTs/RuOx.nH2O composite behaves similar to pure SWCNTs electrodes in aqueous 0.5M H2SO4. In the contrary, its behaviour in 0.5M Na2SO4 looks like the typical responses for MOx electrodes.

V-2. ac-electrogravimetric study of SWCNTs/RuO x .nH 2 O film in H 2 SO 4 aqueous solution

Three different films (SWCNTs, RuOx.nH2O and SWCNTs/RuOx.nH2O) were tested here in order to provide a larger window for discussion and to follow the differences and/or similarities that comes with this new composite electrode. Similarly, to the observation for RuOx.nH2O, a large suppressed loop is obtained for both SWCNTs and SWCNTs/RuOx.nH2O films. The semi-circle is continued through the appearance of a separated very small loop at LF. The theoretical functions (continuous line in fig. V-29) could suggest that there is more than one charged species involved in both cases. At this stage, it is not possible to identify whether the contribution of the species correspond to the anions or cations, the only distinguishable difference between SWCNTs and SWCNTs/RuOx.nH2O films is the fact that the contribution of charged species in composite films is over 3 times larger than the corresponding for pure SWCNTs. For further investigation, the Ki and Gi constants were determined for three species in both SWCNTs and SWCNTs/RuOx.nH2O films. These parameters in aqueous 0.5M H2SO4 electrolyte are shown One could arguably discuss that this is the outer RuOx.nH2O layer of composite which gives a similar response as pure RuOx.nH2O. But there are visible differences between these two films.

q () E      m E    q () E    q () E    207 in Table V-
First, there is no trace of a second cation H3O + among the participating species in composite film and secondly, the anions which are detected only for two potentials in RuOx.nH2O are continuously present in composite films. So, the SWCNTs/RuOx.nH2O film has an intermediate behavior compared to pure SWCNTs and RuOx.nH2O. A common observation among all these three films is the low capacitance of the film against SO4 2-anions.

The evolution of the transfer resistance is shown in (Fig. V-30g, h and i) for the three films. In SWCNTs film, the following order persists: Rti (SO4 2-)>Rti (H + ) ≈ Rti (H2O),the similar order is pursued in SWCNTs/RuOx.nH2O composite film: Rti (SO4 2-)>Rti (H2O)>Rti (H + ) and in the case of pure RuOx.nH2O, differences are observed: Rti (H3O + )>Rti (SO4 2-)>Rti (H2O)>Rti (H + ).

These results indicate that H + ions are the easiest species to be transferred in all these types of films contrary to the transfer of SO4 RuOx.nH2O film, the concentration profile shows that small H + cations are the most populated number of ions that are transferred into the hydrated ruthenium oxide films. The SWCNTs film accommodates the same magnitude of H + cations. And interestingly, the most important number of inserted H + ions belong to SWCNTs/RuOx.nH2O composite films with an increase of over 3 times. Also, clearly the majority of the charged species participation belongs to cations since finally, a very minor number of anions seems to participate, and the values remain close to zero.

It is also noticeable to observe that finally for the composite films both kinetical (fig. V-30) and thermodynamic information go well in the same direction. From the evolution of characteristic frequency, fi, it was observed that H + cations are the fastest species compared to the anions which remain to be very slow over the whole potential window. Then from instantaneous capacitance, Capi, estimation and the evolution of the transfer resistance, Rti, it was furtherly concluded that the most important capacitance belongs to H + cations and these species are the easiest transferred species against bigger SO4 2-anions having high transfer resistances and negligible capacitances. Similar to these kinetical parameters, from a thermodynamic point of view, the concentration change profiles reveal that the H + cations are the majority of species exchanged with the film while the participation of SO4 2-anions remains minor.

VI. Conclusion

In the first part of this chapter an attempt was made to show the usefulness of fast electrogravimetric methods to provide a comprehensive comparison between compact and mesoporous hydrated ruthenium oxide. Mesoporous RuOx.xH2O thin films were synthesized by surfactant assisted electrodeposition method. The idea of using an ionic surfactant (CTAB) during the electrochemical preparation of RuOx.nH2O films led to the creation of ~7-10 nm mesopores which are templated by the corresponding micelles. The compact analogues were also electrochemically synthesized under similar conditions but in the absence of CTAB templates. The pseudocapacitive behavior of the hydrated ruthenium oxide films as their permeability related to the ions intercalation/electroadsorption for mesoporous and compact RuO2.xH2O thin films were investigated by coupled time resolved characterization methods (ac-electrogravimetric method). The chemical nature and the role of each species (ions, solvated ions, and free solvent molecules), directly or indirectly involved in the electrochemical processes were estimated for the very first time.

6 I- 1 . 9 I. 1 . 1 . 9 I . 1 . 2 29 III. 1 . 34 IV- 1 .

 61911912291341 Introduction ..............................................................................................................................1 Résumé du Chapitre I ..............................................................................................................................3 Chapter I: Bibliography ...........................................................................................................................6 I. Supercapacitors as Energy Storage Devices .........................................................................................Basic principle of Electrochemical Supercapacitors .......................................................................8 Two types of Electrochemical Supercapacitors ...............................................................................Electrostatic supercapacitors ................................................................................................Faradaic supercapacitors ........................................................................................................9 II. State of the Art of Different Types of Electrochemical Capacitors (ECs): .......................................10 II-1. EC based on Carbon materials ................................................................................................... 11 II-2. Pseudocapacitive oxide materials ............................................................................................ 14 II. 2. 1. WO 3 .................................................................................................................................... 14 II. 2. 2. TiO 2 .................................................................................................................................... 19 II. 2. 3. MnO2 .................................................................................................................................. 20 II. 2. 4. RuO 2 ................................................................................................................................... 21 II-3. Conducting Polymers ................................................................................................................. 23 II-4. Carbon-MO x Composites ........................................................................................................... 26 III. Strategies Toward New Ways of Materials Design for High Performance ECs ............................ Elaboration Methods and Process ........................................................................................... 29 III-2. Materials Nanostructuration for Development of Flexible Device Architectures ................... 31 IV. Diagnostics Tools for MO x based Electrodes for Energy Storage .................................................. Surface and Structural Analysis: SEM, TEM, XRD, XPS, FT-IR ................................................... 34 (i) SEM images .............................................................................................................................. 34 (ii) TEM images ............................................................................................................................. 36 (iii) XRD analysis ............................................................................................................................ 38 (iv) FTIR methods .......................................................................................................................... 38 IV-2. Electrochemical Tools .............................................................................................................. 39 (i) Cyclic voltammetry ................................................................................................................... 39 (ii) EIS technique ........................................................................................................................... 41 (iii) Quartz Crystal Microbalance .................................................................................................. 43 VII Chapter V: RuO x .xH 2 O ........................................................................................................................ I. Introduction .................................................................................................................................... II. Structural Characterizations .......................................................................................................... II-1. XRD Characterization of as-prepared RuO x .xH 2 O and RuO 2 heated at 450 °C ........................ II-2. SEM-FEG Characterization ....................................................................................................... (i) Compact and Mesoporous RuO x .nH 2 O .................................................................................. (ii) SWCNTs / RuO x .nH 2 O ............................................................................................................ II-3. Targeting Evolution of Morphology and Crystallography by SAED: The effect of calcination (i) The Effect of Heat Treatment on Compact Ruthenium oxide ............................................... (ii) The Effect of Heat Treatment on Porous Ruthenium oxide .................................................. (iii) The Effect of Structuration on Hydrous Ruthenium Oxide Films ......................................... II-4. HR-TEM Results ....................................................................................................................... (i) Mesoporous Ruthenium oxide .............................................................................................. (ii) SWCNTs / RuO x .nH 2 O ............................................................................................................ II-5. XPS Characterization, The impact of Heat Treatment ............................................................. (i) XPS results of RuCl 3 .xH 2 O Precursor ...................................................................................... (ii) RuO x .nH 2 O and RuO 2 .............................................................................................................. III. Electrochemical Characterization: The Cyclic Voltammetry and Classical EQCM Study .... III-1. Cyclic electrogravimetry ......................................................................................................... III-2. Specific Capacitance Calculation ............................................................................................ III-3. Relative Molecular Mass Estimation ...................................................................................... IV. ac-electrogravimetric results for compact and mesoporous RuO x .nH 2 O ........................... IV-1. ac-electrogravimetric results for compact and mesoporous RuO x .nH 2 O in H 2 SO 4 0.5 M aqueous solutions ...........................................................................................................................

  of materials with potential usefulness in energy storage devices. Different examples of each category of materials with emphasizing on MOx based devices are brought to attention. The recent utile elaboration methods for fabrication of MOx based electrodes are mentioned. The new ways of materials design in order to upgrade high performance in the electrodes are discussed and finally, the various diagnostics tools for MOx based electrodes including both structural and electrochemical techniques are introduced.

  dans les dispositifs de stockage d'énergie, notamment les supercondensateurs. Tout d'abord, le principe des supercondensateurs électrochimiques ainsi que les principales catégories de dispositifs sont brièvement présentées. Deuxièmement, les différentes catégories de matériaux qui présentent de grandes potentialités pour ces dispositifs les oxydes de métaux, les polymères conducteurs, les films carbone / carbone et les composites MO x -carbone, seront détaillés avec différents exemples pour chacune des catégories. Le sujet de thèse met l'accent principalement sur les systèmes à base de MOx où différents exemples d'oxydes métalliques sont discutés. Schéma de principe d'un condensateur électrostatique (A), d'un condensateur à double couche électrique (B), d'un pseudocondensateur (C) et d'un condensateur hybride [9]. Pour améliorer les performances d'électrodes à base d'oxyde métallique, une attention a été portée sur l'effet de la nanostructuration de ces films, selon diverses morphologies et propriétés pour la mise au point de dispositifs de stockage d'énergie électrochimique. De nouvelles nanostructures, avec des pores de petite taille et de grands rapports surface sur volume, sont censées faciliter les processus de transfert d'ions à l'interface film structuré/électrolyte. En effet, ce phénomène est essentiel car il intervient dans tous les dispositifs de stockage d'énergie y compris les supercondensateurs. Ces améliorations peuvent être attribuées à (i) un transport facilité avec une très faible longueur de diffusion, (ii) une zone de contact électrode/électrolyte élargie, et (iii) une meilleure gestion du stress mécanique/déformation du matériau lors de l'intercalation/l'électroadsorption d'ions. En conséquence, divers procédés de synthèse ont été développés et sont mentionnés dans une section appropriée. Dessin idéal d'un matériau d'électrode pour des supercondensateurs de type RuO 2 .xH 2 O nanotubulaires. L'architecture mésoporeuse, la nature hydratée des surfaces, et la conductivité métallique fournissent aux protons et aux électrons des "autoroutes" qui doivent favoriser les différents processus électrochimiques et ainsi permettre d'obtenir des condensateurs très efficaces [68]. Dans une seconde partie de ce chapitre I, les différentes techniques d'imagerie et les outils de diagnostic électrochimique pour des électrodes à base de MOx sont présentés. Image HR-TEM d'un échantillon RuO 2 •xH 2 O synthétisé en utilisant un agent tensio-actif pour nanostructurer le film [74]. Une méthodologie attractive pour étudier l'intercalation / l'électroadsorption des ions au sein de ces matériaux est basée sur des dispositifs de type microbalance à quartz (QCM). Il y a eu diverses études utilisant une microbalance à quartz comme sonde gravimétrique in-situ afin d'étudier ces phénomènes au sein d'oxydes métalliques ou d'électrodes à base de carbone. Caractérisation EQCM d'un film de Li-MnO 2 de type Birnessite dans des électrolytes aqueux de LiClO 4 et NaClO 4 [107]. Malgré les informations utiles données par EQCM lorsqu'il s'agit de décrire les mécanismes d'intercalation ou d'électroadsorption ioniques, impliqués lors du stockage de charges dans des matériaux capacitifs, quelques limitations apparaissent. Les microbalances à quartz classiques donnent une réponse globale correspondant en fait à plusieurs processus possibles et plus ou moins simultanés. Des ions nus, des ions avec des coquilles de solvatation et des molécules de solvant libre peuvent ainsi être associés, directement ou indirectement, aux différents processus électrochimiques. En outre, les ions peuvent perdre une partie de leur solvatation pour accéder aux sites situés dans les plus petits pores. Ces différentes voies possibles associées à des aspects cinétiques n'ont jamais été suivies à l'aide de dispositifs classiques d'EQCM.

  categories are briefly introduced. Secondly, different categories of materials with great potentialities in these devices are mentioned including metal oxide, conducting polymers, carbon/carbon and MOx-Carbon composites based supercapacitors. Different examples of each category are brought to attention. Since the thesis subject emphasizes mainly on MOx based devices, a few examples of different metal oxides are also discussed. Then, the recent utile elaboration methods for fabrication of MOx based electrodes are mentioned. Another alternatively interesting followed aspect is the new ways of materials design in order to upgrade high performance in the electrodes. Finally, the various diagnostics tools for MOx based electrodes including both structural and electrochemical techniques are introduced and based on these methodologies the scope of this thesis project is presented.

Fig. I- 1 .

 1 Fig. I-1. Principles of a single-cell double-layer capacitor and illustration of the potential drop at the electrode/electrolyte interface [11].

  material) have been extensively studied recently to capitalize on both electrode materials advantages in improving overall cell voltage, energy, and power densities. In this kind of hybrid supercapacitor, both electrical double-layer capacitance and faradaic capacitance mechanisms occur simultaneously, but one of them plays a greater role. The different configurations are presented in figure I-2.

Fig. I- 2 .

 2 Fig. I-2. Schematic diagram of (A) an electrostatic capacitor, (B) an electric double-layer capacitor, (C) a pseudocapacitor, and (D) a hybrid-capacitor [9].

  . I-3), usually exhibit good stability but limited capacitance values. It is clear that EDLCs processes are surface phenomena, and hence the performance greatly depends on the electrolyteaccessible surface area. The micropores in carbon materials are inaccessible by the electrolyte, resulting in the inability of the double layer to be formed inside the pores. This result leads to a decrease in the capacitance value (10-20% of the 'theoretical' capacitance) of ACs. Good electrical conductivity, high chemical and mechanical stability, and an optimized nanostructure are also other important factors that are responsible for achieving high capacitance values. The potential windows in nonaqueous electrolytes are generally larger than those obtained in aqueous media, although the overpotential of hydrogen evolution on carbons is high, especially in neutral electrolytes.

Fig. I- 3 .

 3 Fig. I-3.The most common carbon materials classified based on their bonding (hybridization of orbitals of carbon atoms) and dimensionality (i.e., the number of dimensions not confined to the nanoscale). Whereas graphite, carbon fibers, glassy carbon, activated carbons, carbon black, and diamond are already widely used in industry, fullerenes and fulerides, carbon onions (multishell fullerenes), nanotubes, whiskers, nanofibers, cones, nanohorns, nanorings, nanodiamonds, and other nanoscale carbons are being explored for future technologies. Note: 0D, zero-dimensional; 1D, one-dimensional;

Fig. I- 4 .

 4 Fig. I-4. Capacitance change versus current density for laboratory cells assembled with CDCs with various pore sizes [55].Many attempts have been made to increase the specific capacitance of carbon nanotubes (CNTs). Electrochemical enhancement by adding redox active functional groups on CNTs increases the specific capacitance, while excessive oxidation decreases conductivity and leads to poor cycle life. X. Xiao et al.[37] reported on the electrochemical enhancement methods followed by annealing at different temperatures in air to add and adjust the redox active functional groups. Functionalized freestanding CNT films were used as positive electrodes, assembled with freestanding CNT/MoO3_x negative electrodes to fabricate carbon nanotubebased solid-state asymmetric supercapacitors (ASCs).

Fig. I- 5 .

 5 Fig. I-5. (a) Schematic of the fabrication procedure for functionalized free standing CNT films. (b) Cross section SEM image of the functionalized freestanding CNT film. (c) Enlarged cross-section SEM image of the functionalized free standing CNT films. The inset is a digital image of a functionalized freestanding CNT film [56].

  specific structures. According to this report performance could be improved when an assembly structure of hexagonal phase WO3 (h-WO3) nanopillars is synthesized which favors enhanced proton insertion mechanism. As it is demonstrated in Fig. I-6 d high capacitance of up to 422 F g -1 under the current density of 0,5 A g -1 could be achieved by this electrode (Table I-1).

Fig. I- 6 .

 6 Fig. I-6. CV curves (a), profiles of capacitance versus potential (b), and charge-discharge profiles (c) measured at different rates and (d) cycling stability of the as-synthesized h-WO 3 nanopillars [57].

Fig. I- 7 .

 7 Fig. I-7. (a) Low and (b) High magnification SEM images; (c) TEM image of a single WO 3 microsphere; (d) HRTEM image of WO 3 nanofibers. The inset is selected area electron diffraction (SAED) of the selected area in (d) [58].

Fig. I- 8 .

 8 Fig. I-8. (a) Cyclic voltammograms of Ti/RuO 2 +TiO 2 substrate, nano-WO 3 -H 2 O, MnO 2 and NWMO within a potential window of -0.1 -0.9 V at 5mVs -1 scan rate (b) cyclic voltammograms of NWMO at different scan rates [59].Based on their electrochemical characterizations (Fig.I-8), this new electrode exhibits excellent capacitive performance including high specific capacitance of 363 F g -1 and long-term stability, which is resulted from this special nanostructure[START_REF] Yuan | Anodic deposition and capacitive property of nano-WO3•H2O/MnO2 composite as supercapacitor electrode material[END_REF].

Fig. I- 9 .

 9 Fig. I-9. (a) SEM image of as-synthesized h-WO 3 nH 2 O particles. (b) High-resolution TEM image and fast Fourier transform (FFT) images (inset) of a single h-WO 3 nH 2 O nanorods [21].

Fig. I- 10 .

 10 Fig. I-10. Electrochemical performance of h-WO 3 •nH 2 O electrodes. (a) CV curves of h-WO 3 •nH 2 O electrodes at voltage sweep rate of 10 mV s -1 in 0.2 M H 2 SO 4 , Li 2 SO 4 and Na 2 SO 4 electrolytes in threeelectrode cells with Ag/AgCl and Pt foil as the reference and counter electrode, respectively. (b) Comparison of electrochemical capacitive performance of our h-WO 3 •nH 2 O with other WO 3 structures (h-WO 3 with CNT, h-WO 3 bundle structure, hexagonal-cubic mixed phase WO 3 , monoclinic WO 3 thin film) [21].

Fig. I- 11 .

 11 Fig. I-11. Capacitance variations of MnO 2 nanorods at different scan rates in 0,5 mole L -1 aqueous Li 2 SO 4 , Na 2 SO 4 , and K 2 SO 4 electrolytes [67].

(

  currently at ~2000 USD per kg) makes devices based on RuO2 impractical for widespread application, except in small-size devices such as microsupercapacitors. Nevertheless, the behavior of hydrous RuO2 first demonstrated that in certain systems, reversible faradaic reactions can result in similar electrochemical features as those of a capacitor. The study of RuO2 also led to the understanding of what constitutes an ideal pseudocapacitive material in aqueous electrolytes.

Fig. I- 12 .

 12 Fig. I-12.The general electrochemical features of pseudocapacitive materials. (a) In a cyclic voltammetry experiment, the shape is rectangular and if peaks are present, they are broad and exhibit a small peak-to-peak voltage separation. (b) In a galvanostatic experiment, the shape is sloping so that a capacitance value, dQ/dE, may be assigned at each point, and the voltage hysteresis is small. Here, Q is the capacity and E is the potential window. (c) In an AC impedance experiment, the Nyquist representation will contain a vertical line with a phase angle of 90° or less. A semi-circle at high frequencies, associated with charge-transfer resistance, may also be present[27].

Fig. I- 13 .

 13 Fig. I-13. Scanning Electron Microscopy images of; a) H-RuO 2 , b) PANI, c) RP30 (Electrodeposition of PANI was performed at a constant potential of 0.7 V for 30 min at room temperature) and d) X-ray diffraction patterns of electrodes [25].B-X Zou et al.[START_REF] Zou | Electrodeposition and pseudocapacitive properties of tungsten oxide/polyaniline composite[END_REF] have reported on the pseudocapacitive properties of WO3/PANI composite films electrodeposited by cyclic voltammetry in solutions of aniline and precursor of the oxide prepared from tungstic acid and H2O2. These composite films exhibited good pseudocapacitive performance in a wide potential range of -0,5 to 0,7 V vs. SCE due to the electroactivities of WO3 in negative potential range and its fine distribution in PANI matrix. Fig. I-14 presents the specific capacitance of WO3, PANI and WO3/PANI composite (WP) with different mass of films. It is assumed that with the mass of films increasing, the specific capacitance of WO3

Fig. I- 15 .

 15 Fig. I-15. SEM images of (a) acid-treated CNTs, (b) Al 2 O 3 /CNTs, (c) Ni-Al LDHs/CNTs and (d) TEM image of Ni-Al LDHs/CNTs [81].

Fig. I- 16 .

 16 Fig. I-16. ZrO 2 -SiO 2 sheets impregnated with WO 3 nanoparticle electrode [19].

C- C

 C figure I-17.

Fig. I- 17 .

 17 Fig. I-17. An ideal design of the electrode material for next generation of supercapacitors, RuO 2 .xH 2 O nanotubular arrayed electrode. The mesoporous architecture, hydrous nature, and metallic conductivity provide the proton and electron "superhighways" for the extremely rapid charge/discharge processes [68].

Fig. I- 18 .

 18 Fig. I-18. (A) The bright-field and (B) high-resolution TEM images of RuO 2 .xH 2 O NTs annealed in air at 200 °C for 2 h. The inset of electron diffraction pattern shows typical diffraction rings of RuO 2 polycrystals in the rutile form [68]. This ordered, 3D, porous architecture is favorable for the penetration of electrolytes into the whole oxide matrix, and the hydrous structure shortens the proton diffusion distance (Fig. I-

Fig. I- 19 .

 19 Fig. I-19. SEM images of (a) the pristine CNTs, (b) low-magnification, and (c) high-magnification view of MnO 2 /CNTs composite [42]. Flower-like WO3•H2O/reduced graphene oxide composites have been synthesized through a mild hydrothermal approach by L. Ma et al. [78]. In this work SEM results manifest that the WO3•H2O in the composites displays a 3D hierarchical flower-like morphology with uniform sizes and are well dispersed and closely anchored on the flexible reduced graphene oxide as given in figure I-20.

Fig. I- 20 .

 20 Fig. I-20. SEM images of the as-prepared (a, b) bare WO 3 •H 2 O and (c, d) WO 3 •H 2 O/rGO [78].

Fig. I- 21 .

 21 Fig. I-21. TEM images of WO 3 hollow nanospheres/ (A) low-magnification and (B) high-magnification [20]. D Muñoz-Rojas reported on the effect of crystallite/particle size on the electrochemical lithiation of RuO2 films prepared by a hydrothermal route. A panel of samples with different

Fig. I- 22 .

 22 Fig. I-22. Characterization of the panel of materials prepared through a 'chimie douce' process (a) Evolution of the XRD patterns as a function of annealing temperature (Cu Kα) (b)-(f) TEM pictures and Fourier transforms for (b) R200 (c) R300, (d) R400, (e) R500 and (f) R800 [102].

Fig. I- 23 .

 23 Fig. I-23. HR-TEM image of the as-prepared RuO 2 •xH 2 O sample. The inset shows the SEAD Pattern [74].

(

  iii) XRD analysis B-O Park et al. [96,97] have used X-ray Diffraction (XRD) to characterize ruthenium oxide (RuO2) films of different thicknesses synthetized by cathodic electrodeposition on titanium substrates and prepared in aqueous acidic Ru(III)Cl3 solution.

Fig. I- 24 .

 24 Fig. I-24.X-ray diffraction patterns of RuO 2 films deposited on titanium substrate for different time at a current density of 5.0 mAcm -2 : (a) 30 min, 0.0014 g cm -2 ; (b) 60 min, 0.0023 g cm -2 ; (c) 120 min, 0.0040 g cm -2 and (d) 180 min, 0.0059 g cm -2 . The marks (#), (x) and (O) correspond to Ru, RuO 2 and Ti materials, respectively[START_REF] Park | Performance of supercapacitor with electrodeposited ruthenium oxide film electrodes-effect of film thickness[END_REF][START_REF] Park | Cathodic electrodeposition of RuO2 thin films from Ru(III)Cl3 solution[END_REF].

Fig. I- 25 .

 25 Fig. I-25.FT-IR spectra of RuO 2 deposited by CBD method[START_REF] Patil | Chemically synthesized hydrous RuO2 thin films for supercapacitor application[END_REF].The FT-IR absorption spectrum of RuO2 in the range 4000-400 cm -1 is shown in Fig.I-25. The strong band (υ1) around at 600 cm -1 is associated with the characteristic vibrational mode of rutile RuO2. The absorption peak (υ2) at around 1095 cm -1 is assigned to characteristic stretching vibration of peroxo groups. The absorption peak around 1604 cm -1 is due to the bending vibration of hydroxyl groups of molecular water (υ3). The sharp absorption band (υ4) at 3406 cm -1 is attributed to the stretching vibrations of OH -. Shoulder of the υ4 bond attributed to the hydrous nature of the RuO2 material. These results revealed that, deposited film contained hydroxide bonds indicates the formation of hydrous RuO2.

Fig I- 26 .

 26 Fig I-26. (a) CVs of WO 3 nanoparticles at three scan rates, 25, 100, and 500 mV/s. Inset shows corresponding CVs of carbon aerogels calcined at 400 °C were also included for comparison. (b) CVs of WO 3 /Carbon aerogels composites at 100 mV/s recorded at cycle numbers of 100, 300, 500, 700, and 1000. Also included was CV for plain CA recorded at the 50th cycle [79].

Fig. I- 27 .

 27 Fig. I-27. (a) Cyclic voltammograms of (1) RuO 2 •xH 2 O and (2) WO 3 measured at 25mVs -1 in 0.5M H 2 SO 4 ; (b) Cyclic voltammograms of a supercapacitor based on an asymmetric type consisting of a WO 3 anode and a RuO 2 •xH 2 O cathode measured at (1) 10mVs -1 , (2) 25mVs -1 , (3) 50mVs -1 , and (4) 100mVs -1 in 0.5M H 2 SO 4 ; (c) The plots of specific energy vs. specific power for (1) symmetric (RuO 2 -RuO 2 ) and (2) asymmetric (RuO 2 -WO 3 ) capacitors. The total weight of all active materials (including cathode and anode) for both symmetric and asymmetric capacitors is equal to ca. 4mg cm -2[START_REF] Chang | Microwave-assisted hydrothermal synthesis of crystalline WO3-WO3•0.5H2O mixtures for pseudocapacitors of the asymmetric type[END_REF].

Fig I- 28 .

 28 Fig I-28. Electrochemical Impedance measurements of nanoporous hydrous RuO 2 samples, for a frequency range from 100 kHz to 0.01 Hz at a potential of 1.0 V vs Ag/AgCl. The inset shows the magnification [74]. Both the RuO2•3.38H2O and RuO2•2.56H2O electrodes showed similar Nyquist plot curves with typical linear shape of electrochemical capacitors, where slope gradually changes from 45 to 90 • , the imaginary part of impedance sharp increased and showed the vertical line of capacitive behavior. From these results it was concluded that both the RuO2•3.38H2O and RuO2•2.56H2O electrodes exhibited nearly pure electrochemical capacitive behavior. In another work [80] EIS was conducted to elucidate the electrochemical capacitive behavior of hybrid SWCNT/WO3/PANI electrodes. Fig. I-29 shows the Nyquist plots of the electrodes measured within the range from 50 kHz to 50 mHz at 0 V vs Ag/AgCl.

Fig. I- 29 .

 29 Fig. I-29. Impedance spectra of thin RuO 2 films measured within the range from 50 kHz to 50 mHz at a 0 V DC potential. Inset is magnified for the high frequency region of the impedance spectra [80].Supercapacitor electrodes EIS responses look like a resistance at high frequency values and like a capacitance at low frequency values. In a theoretical Nyquist plot, there is a small semicircle in the high frequency region and a straight line in the low frequency region. The high frequency semicircle is attributed to the electrode-electrolyte interface, which is related to the double-layer capacitance in parallel with the charge-transfer

Fig. I- 30 .

 30 Fig. I-30. Electrode mass change vs charge during the polarization of CDC-1 nm in neat EMI-TFSI: Blue solid lines are measured mass change (EQCM), red dashed lines are the theoretical mass change of neat ions calculated from Faraday's law. The black dashed line shows the linear fitting of measured mass change [104]. Santos et al. [105] studied the Li + ion intercalation/adsorption behavior of dense WO3 films in acetonitrile solution containing LiClO4 by QCM measurements during cyclic voltammetry(EQCM). The mass-to-charge ratios were calculated from the EQCM data in LiClO4/ acetonitrile electrolytes, which can be used to estimate the molar mass of the species inserted in the material. However, none of the values obtained from the MCR was in the order of the equivalent weight of either ion (Li + , or ClO4 -) or solvent molecules (acetonitrile) of the study.

  de la formation électrochimique des films, ces agrégats sont piégés et de par leurs dimensions, ils remplissent des cavités. Après cette étape, ces agents tensioactifs peuvent être facilement éliminés par lavage avec un alcool approprié ce qui permet d'obtenir des pores de tailles contrôlées (~3-5 nm de diamètre). Ces nanostructures, avec des pores de petites dimensions et avec du coup un ratio surface sur volume très grand, sont censés faciliter le processus de transfert des ions. Ici, une importance particulière a été portée sur les matériaux amorphes plutôt que sur les matériaux cristallins pour évaluer les performances électrochimiques de ces premiers. La structure, la morphologie et la composition des films mésoporeux synthétisés par voie électrochimique ont été caractérisés (XPS, MEB et MET à haute résolution) et comparés avec leurs homologues denses. en présence de tensioactifs. Ici, le CTAB (cetyltrimethylammonium bromide) a été utilisé comme agent tensio-actif ionique lors de la préparation électrochimique de films RuO2.xH2O. Cela conduit à la création de mésopores de ~ 7-10 nm de diamètre après le départ des micelles correspondants. Les films analogues denses ont été également synthétisés par voie électrochimique dans des conditions similaires mais en l'absence des molécules de CTAB. La structure, la morphologie et la composition des films electrosynthétisés mésoporeux ont été caractérisés un ensemble de techniques (DRX, XPS, MEB, MET et SAED) et comparés avec leurs homologues compacts. Schéma de principe de la microscopie électronique à balayage (à gauche) et image d'un film compact d'oxyde de ruthénium hydraté (à droite). Enfin, des films composites à base de Nanotubes de Carbones (CNTs) et d'oxydes de ruthénium hydraté ont été réalisés. Tout d'abord, des films de nanotubes de carbone ont été déposés par la méthode de « drop casting » sur l'électrode d'or de la microbalance à partir d'une suspension de CNTs. Par la suite, une couche très fine d'oxyde de ruthénium hydraté a été électrodéposée sur ces films de CNTs. L'idée est de combiner les performances en termes de capacité du RuO2.xH2O avec celles des films de nanotubes de carbone. La structure et la morphologie de ces films ont été caractérisées avec MEB et MET à haute résolution. Image en coupe d'un film mince de l'oxyde de ruthénium hydraté électrodéposé sur des films de nanotubes de carbone. Dans une deuxième partie, la méthode d'ac-électrogravimétrie est présentée sous une approche théorique en donnant les bases de calcul des différentes fonctions de transfert. En effet, l'acélectrogravimétrie porte sur le couplage entre la spectroscopie d'impédance électrochimique et une microbalance à quartz rapide (QCM), utilisée en mode courant alternatif. La réponse en courant et en masse suite à une perturbation en potentiel de faible niveau, permet d'estimer simultanément la fonction de transfert électrochimique, de ces deux fonctions de transfert offre la possibilité d'une séparation des différents processus électrochimiques, au niveau des variations de masse et de charges. Fonctions de transfert principales théoriques utilisées pour la partie ajustement des résultats expérimentaux d'ac-electrogravimétrie.

Figure II- 1

 1 Figure II-1 illustrates a quartz disk with its gold electrodes, front view (a) and sectional view (b). The arrow indicates the active area of the electrodes. The second arrow, circular cap shows the electrode legs used for making connections. When a sinusoidal voltage is applied between the two electrodes, the upper and lower sides of the active zone of the crystal vibrate parallel to each other in a thickness shear mode. An acoustic wave is thus generated in this volume and under resonant conditions, has a characteristic frequency called quartz resonant frequency or microbalance frequency. This electrical excitation frequency corresponds to a conversion between electrical energy and maximal mechanical energy (acoustic) upon application of an alternative voltage. The quartz provided and equipped with these electrodes is called piezoelectric resonator.

Fig. II- 1 .

 1 Fig. II-1. Quartz face's covered with two gold electrodes on each side. In a front view (a) and in a cross-sectional view (b).

  LISE laboratory. The quartz crystal with 9 MHz resonant frequency (RAKON, France or AWS, Spain) with its up layer gold electrode, is fixed on a printed circuit chip. A silver paste is used to ensure the electrical contacts and a silicone glue is then applied to isolate them from the solution contact. This device is connected to an oscillator associated with a 9 MHz electronic circuit developed in the laboratory (Fig.II-2). It is possible to receive the microbalance frequency changes, fm, in real time via the FRQM software developed at LISE.

Fig. II- 2 .

 2 Fig. II-2. Quartz assembly coupled with its 9 MHz oscillator.

Fig. II- 3 .

 3 Fig. II-3. Experimental device for the cyclic electrogravimetry measurements.

Fig. II- 4 .

 4 Fig. II-4. Linear current response to a sinusoidal potential perturbation of small amplitude around a stationary V s value.

Fig. II- 5 .

 5 Fig. II-5. Equivalent electrical circuit (a) and plots of impedance of an electrochemical cell in the Nyquist plane (b) and in the Bode plane (c). Two types of plots are used to describe these relationships. They are illustrated in figure II-5 regarding the equivalent circuit of an electrochemical cell which has the impedance

  in the Nyquist plan (-Im Z, Re Z) (Fig. II-5b) or in the Bode illustration (Fig. II-5c). This allows to observe changes in | Z | and φ with frequency; Re Z and Im Z can be traced similarly. The electrochemical admittance,

Fig. II- 6 .

 6 Fig. II-6. Experimental setup for measurements of the electrochemical impedance.

Figure

Fig. II- 7 .

 7 Fig. II-7. Principle of the electrogravimetric measurement.

Figure II- 8 )

 8 is composed of different elements:  A three electrodes electrochemical cell: The reference electrode is usually a saturated calomel electrode (SCE) or Ag/AgCl, the counter electrode is made of platinum grid and the working electrode is the gold electrode deposited on the faces of the quartz resonator,  A potentiostat SOTELEM PG-STAT100,  An FRA-Solartron 1254 comprising a voltage generator, V', and analyzer of the transfer functions,  A reference frequency synthesizer, Marconi 2023,  A frequency/voltage converter developed by LISE.As shown in figure II-8, the 1254 generator delivers a sinusoidal perturbation of small amplitude, V' at a given modulation frequency, f. This signal is superimposed on the bias potential supplied by the potentiostat, Vs.The signal of the microbalance fm is sent to a frequency-voltage converter which subtracts a reference signal fr, near the frequency of the microbalance, issued by the frequency synthesizer Marconi-2023. The fm-fr signal is then converted into a continuous voltage Vf. If fm varies from fm then, the converter delivers a voltage variation VfThis result is finally sent to the FRA 1254 analyzer. Since Solartron 1254 analyzer has four measurement channels, it is possible to recover the I and V values parallel to Vf in order to measure the electrochemical impedance, II-8. This is the reason for which this measurement is called "electrochemical impedance coupled with electrogravimetry" or ac-electrogravimetry.

Fig. II- 8 .

 8 Fig. II-8. Ac-electrogravimetric and electrochemical impedance set-up.

Fig. II- 9 .

 9 Fig. II-9. Calibration and determination of the frequency / voltage converter TF,

  Figure II-10 shows schematically the input and output signals of synthesizer for determining the module of the e f s   transfer function. The signals e  and s f  are measured using respectively a Keithley-2000 voltmeter and a Fluke-PM6690 frequency meter. A plot in the Origin® software allows to determine e and s f  in a precise manner for adjusting the modulation depth of the given synthesizer.

Fig. II- 10 .F

 10 Fig. II-10. Calibration of Agilent 33250A synthesizer and determination of the frequency / voltage converter transfer function.For three settings of modulation depth, the following values for the synthesizer function

Fig. II- 12 .

 12 Fig. II-12. General illustration of the sputtering deposition system with diagnostic tools (Langmuir probe and OES).

(

  Figure II-13. The total deposited mass is higher for the films synthesized in the presence of SDS surfactant (Fig.II-13b), indicating the incorporation of the SDS surfactant molecules. These films are considered to be inorganic/organic hybrids composed of a WO3 inorganic matrix surrounding the SDS surfactant micelles, and they are extracted from the inorganic matrix in a subsequent step following the electrodeposition.

Fig. II- 13 .

 13 Fig. II-13. Synthesis of WO 3 thin films: typical electropotentiostatic deposition data and simultaneous QCM characterization (mass variation of the quartz crystal during electrodeposition) of (A) dense and (B) mesoporous WO 3 thin films (deposited at -0.5 V vs Ag/AgCl during 15 min).

  •nH2Ointo Ru(OH)y3Cl3-y•cH2O structure. Since the pH of the precursor solution RuCl3 varies with storage time; in the present study, attempt was made to maintain the pH of RuCl3 solution at about 2.0 (±0.1) with addition of diluted HCl solution and making fresh solution of RuCl3 before deposition. I. Zhitomirsky et al.[20] was the first to synthesis of RuO2 by a cathodic electrodeposition process on Ni, Ti, Pt foils and Si wafers. Following the same concept B.O. Park et al.[21, 22] reported the synthesis of Ruthenium oxide (RuO2) films of different thicknesses by cathodic electrodeposition on titanium substrates from aqueous acidic Ru(III)Cl3 solution. The author indicates that electrodeposition is an advantageous preparation route, mainly because: (i) it is a low temperature method of preparation and (ii) the resulted thin film presents high porosity.Inspired from these primary reports on RuO2 electrodeposition, we have chosen the same pathway for synthesizing hydrated RuO2 or more correctly RuOx.nH2O. The typical experimental set-up is illustrated in figure II-14. More precisely, the electrodeposition solutions were prepared from a freshly 10 mM electrolyte containing 0.1037 g of RuCl3.xH2O as precursor (ReagentPlus, Sigma-Aldrich, USA) dissolved in 50:50 v/v mixture of two solutions:10 -1 M KCl and 10 -1 M HCl solutions. The pH of the solution was adjusted to ~2.15-2.5 by few drops of 10 -1 M KOH. For the mesoporous thin film synthesis, the CTAB/precursor[25] ratio was 0.32 and the solution contained 0.116 g of cetyltrimethylammonium bromide (BioXtra, 99.0% Sigma-Aldrich, China).

Fig. II- 14 .

 14 Fig. II-14. Typical set-up used for the electrodeposition.

Fig. II- 15 .

 15 Fig. II-15. Principle and components of a Scanning Electron Microscope.

Fig. II- 16 .

 16 Fig. II-16. Layout of optical components in a basic TEM [27].

Fig. II- 17 .

 17 Fig. II-17. The schema of X-ray chamber, and the inside view of the X-ray tube (LISE Lab).

Fig. II- 18 .

 18 Fig. II-18. Basic components of a monochromatic XPS system.

Fig. II- 19 .

 19 Fig. II-19. General view of the XPS montage used in for our studies (LRS laboratory, UPMC). The composition of the studied MOx films were determined by X-ray photoelectron spectroscopy (XPS) with the same montage shown in figure II-19 (on a VG ESCALAB 250i-XL spectrometer using monochromatic Al Kα radiation as the X-ray source).

) 1 .

 1 Résumé du Chapitre IIITiO2 est un matériau polyvalent utilisé dans de nombreux domaines technologiques importants et divers[1][2][3]. En tant que matériau particulièrement stable, peu coûteux, non toxique, et abondant, TiO2 a attiré beaucoup d'attention dans les applications de stockage d'énergie, en particulier dans le domaine des batteries lithium-ion et des supercondensateurs[4][5][6][7][8][9]. Avec le succès de TiO2 comme matériaux d'anode pour les batteriesLi-ion, il est aussi intéressant d'étudier son utilisation pour les batteries Na-ion. Des films minces d'oxydes de métaux sont des matériaux idéaux pour le stockage électrochimique de l'énergie. En effet, les distances de diffusion requises pour le stockage des ions sont beaucoup plus courtes et ainsi, il est possible de travailler avec des coefficients de diffusion assez faibles. Le transfert lent d'ions dans les matériaux MOx restreint considérablement la cinétique électrochimique [10]. Par conséquent, il est primordial de créer les structures dans lesquelles une meilleure accessibilité est prévue pour le transfert des espèces chargées. L'ac-électrogravimétrie a la capacité de détecter la contribution des espèces chargées ou non chargées, au cours des différentes processus faradiques ou (pseudo)capacitif. Dans ce chapitre, et pour la première fois, cette méthodologie originale a été utilisée afin d'étudier le transfert des ions entre un film de TiO2 et l'électrolyte. Différentes morphologies de TiO2 amorphe ont été évaluées : forme compacte, forme poreuse et très poreuse. Elles ont été déposées par pulvérisation réactive magnétron RF. Cette technique de préparation permet de synthétiser à basse température différents matériaux avec différentes morphologies à l'échelle nanométrique. Les conditions de dépôt de haute pureté sont fournies sous une atmosphère d'Ar. Les couches minces de TiO2 amorphes ont été étudiées dans deux milieux différents, LiClO4 et NaClO4, afin d'identifier les espèces qui participent au processus de compensation de charge. En effet, ac-électrogravimétrie peut servir comme sonde gravimétrique afin d'étudier les mécanismes complexes de stockage de charge et extraire des subtilités inaccessibles avec des outils classiques d'investigation. Les courbes d'électrogravimétrie montrent une réponse quasiment capacitive dans la région anodique. La densité de courant cathodique et anodique des films de TiO2 avec la morphologie très poreuse est beaucoup plus élevée que celle observée pour les films poreux et denses. Cela indique une cinétique plus rapide de transfert des ions. Les valeurs de densité de courant mesurées sont presque cent fois supérieures à celle obtenue pour le film moins poreux. Les variations de masse sont également influencées par la présence des pores, la réponse de la microbalance est amplifiée dans le cas du film très poreux. Cette meilleure réponse est attribuée à une meilleure surface spécifique grâce à la présence de pores. Image de la surface d'un film très poreux de TiO 2 (a) et image en coupe avec estimation de l'épaisseur (b). Les résultats présentés dans ce chapitre pour les films minces de TiO2 amorphes poreux et très poreux établissent que les mécanismes de stockage de charge pseudo-capacitif peuvent être examinés par ac-électrogravimétrie. La technique fournit l'identification exacte des espèces chargées et non-chargées et des informations cinétiques à ce propos, ce qui est impossible avec des mesures d'EQCM classique. Le comportement électrochimique des films minces de TiO2 poreux et très poreux dans les solutions aqueuses de LiClO4 et NaClO4 implique les ions Li + , les ions Na + ainsi que les formes hydratées de ces ions. Il est à noter que des anions ont aussi été détectés par notre étude d'ac-electrogravimétrie. Variations de courant et de masse obtenues simultanément lors du cyclage électrochimique de films de TiO 2 (a) dense, (b) poreux, et (c) très poreux, déposés sur l'électrode d'or d'un résonateur à quartz. Les mesures sont en solution aqueuse de LiClO 4 0,5M avec une vitesse de balayage de 10 mV s -Les résultats de nos études dans une solution aqueuse de LiClO4 ont révélé que la contribution des espèces chargées a été amplifiée dans les films de TiO2 très poreux par rapport aux films moins poreux. Cette étude qualitative et quantitative de la contribution des espèces ioniques et non ioniques dans le processus de compensation de charge, ainsi que des informations dynamiques sur le transfert interfacial a encore prouvé la nature avantageuse des structures poreuses des films de TiO2. Celle-ci est probablement liée à une meilleure accessibilité fournie aux deux espèces cationiques Li + et Li + .H2O . En particulier, l'espèce lithium hydraté, Li + .H2O a été transférée rapidement et facilement à l'interface électrode/électrolyte, dans le cas des films TiO2 très poreux. De plus, les variations relatives de la concentration des ions dans l'électrode de TiO2 très poreuse sont significativement plus élevées par rapport à celles de leurs homologues moins poreuses. Pour NaClO4 en milieu aqueux et pour le film de TiO2 poreux, en raison d'une porosité intergranulaire réduite, la seule contribution majeure appartient au sodium hydraté. Dans ce cas, le transfert des espèces anioniques se révèle difficile. D'autre part, la surface active optimisée dans le cas du TiO2 très poreux conduit à un transfert ionique du sodium hydraté encore plus facile. La dernière section est dédiée à la comparaison entre deux électrolytes l'un aqueux et l'autre organique. Il s'agit d'étudier l'impact du solvant organique sur la dynamique du transfert des différentes espèces à la fois d'un point de vue cinétique et thermodynamique, et cela pour la première fois. Globalement, les résultats obtenus sont plus satisfaisants lorsque l'électrolyte à base de LiClO4 est aqueux. Par exemple, la capacité instantanée des espèces ioniques transférées à l'interface électrode très poreuse de TiO2/électrolyte, est beaucoup plus élevée lorsque l'électrolyte est aqueux. Cela peut être lié à la viscosité dynamique plus élevée du solvant organique par rapport au milieu aqueux. Il en est de même pour les résistances de transfert ioniques plus importantes en milieu organique. Dans le cas des mesures en solvant organique, l'eau libre n'apparaît pas mais le solvant organique oui. Celui-ci accompagne le transfert des ions Li + . Ceci influence indirectement la dynamique de transfert ionique qui est du coup ralentie. Fonctions de transfert de masse/potentiel, pour un film de TiO 2 très poreux dans (a) électrolyte aqueux de LiClO 4 0.5 M (comprenant trois espèces, en particulier Li + , Li + .H 2 O et ClO 4 -) et (b) électrolyte organique de LiClO 4 /PC 0,5M (comprenant trois espèces, en particulier Li + , PC et ClO 4 -). Les mesures sont effectuées à -0,9 V vs SCE (les courbes expérimentales et théoriques sont indiquées). Enfin, à notre connaissance, c'est la première fois que les mécanismes d'échanges ont été examinés de manière in-situ et détaillés entre différentes morphologies de TiO2 amorphe et deux types d'électrolyte, aqueux et organiques. Ces résultats sont très intéressants et originaux, grâce à la combinaison entre une QCM rapide et la spectroscopie d'impédance électrochimique. Cela permet une meilleure compréhension des mécanismes de transfert d'ions et de mieux comprendre l'impact des molécules de solvant sur ceux-ci dans le cas de matériaux à porosité variable. Ces avancées sont impossibles à déterminer en utilisant des EQCM simples. Par conséquent, la mise en place de caractérisations par ac-électrogravimétrie dans le domaine des matériaux liés à l'énergie est importante. Cela devra permettre de les optimiser pour créer une nouvelle génération de supercondensateurs à haute densité d'énergie.

  investigated the pseudocapacitance of TiO2 thin films anchored to CNTs. According to their investigation it was observed that amorphous TiO2 films exhibited superior charge storage capability than crystalline TiO2 films. The morphology dependent performance and ion intercalation behaviour of TiO2 thin films have been investigated by several in situ or ex situ characterization techniques, including electrochemical methods[6, 8,9, 14], X-ray diffraction spectroscopy[6, 8,9, 14], X-ray photoelectron spectroscopy[6, 8,9, 14]. However, none of these methods alone provide the information on the exact identification of the transferred ionic species, their dynamics of transfer at the interfaces, as well as the role of electrolyte composition and the effect of ions solvation on the intercalation/capacitive phenomena. The status of transferred ions is not a quite solved problem and the characterization of their transfer dynamics is not straightforward using conventional characterization tools. The main challenge is to find a powerful technique offering mechanistic solutions in a unique set-up that can be used to study ion transfer in-situ and in contact with an electrolyte. There have been studies using quartz crystal microbalance (QCM) as an in situ gravimetric probe to study the intercalation/electroadsorption of ions in metal oxide or carbon based electrodes. Conducting electrodes coated on the QCM resonator surface are used as working electrodes in an electrochemical cell, and thus, the electrodeposition process can be monitored. Materials of interest deposited are studied in terms of mass changes during the electrochemical processes[15][16][17][18]. Nevertheless, EQCM gives a global response corresponding in fact to several possible pathways such that ions, ions with solvation shells and even, indirectly free solvent molecules can contribute indirectly to the electrochemical process[19]. Additionally, ions may lose a part of their solvation shell to access to the sites which could be corresponded to confined nanopores. These possible pathways, and kinetic or dynamic aspects of the ion intercalation/electroadsorption processes have never been characterized in the previous EQCM studies due to the limitations of the technique. In spite of its great relevance, fast electrogravimetric methods, i.e., coupling fast quartz crystal microbalance (QCM) and electrochemical impedance spectroscopy (EIS) (ac-electrogravimetry), have not yet been used for studying transfer and transport phenomena in materials for charge storage (except for the use of QCM along with cyclic voltammetry experiments (EQCM).

  morphology of the synthesized TiO2 thin films was characterized by FEG-SEM and HR-TEM. Based on their preparation details when the operating pressure monitored by the Ar flow rate in the reactor was low i.e. 3 mtorr for 30 sccm of Ar, a fairly dense film with some distinct cracks observed on some parts of the sample is obtained (fig.III-1a). The average film thickness is ~ 300 nm and could be tailored by varying the deposition time or the pressure used for their fabrication[20][21]. An advantageous aspect of deposition based on reactive RF sputtering is the possibility to obtain different morphologies simply by varying the argon pressure in the reactor (already discussed in the experimental section). In order to procure more porous structures, an intermediate Ar pressure (60 sccm) was used. The morphological impact, is presented in fig III-1cwhere the image shows a crack-free film which is composed of spherelike shape nanoparticles of TiO2. The cross-section image (fig III-1d) gives a 600 nm average film thickness. This coating is chosen to be called porous TiO2 for the following discussions.Furtherly, when the maximum Ar pressure (140 sccm) was applied, a completely different morphology was procured as shown in figure III-1e. The corresponding TiO2 film which consists of nanosize TiO2 particles, curiously grown with a columnar structure, with a rough surface. The estimated film thickness is now ~700 nm (fig. III-1f). For further discussions, this deposition is referred to highly porous TiO2.

Fig. III- 1 .Fig. III- 2 .

 12 Fig. III-1. FEG-SEM images showing the top view and the cross-section of deposited dense (a, b), porous (c, d) and highly porous (e, f) TiO 2 thin film deposited on the Au coated electrode of quartz resonators by RF reactive sputtering (reactor conditions: RF power 200 W, 0.2 mtorr O 2 pressure, pressure: 3 mtorr for compact TiO 2 , 6 mtorr for less porous TiO 2 , 14 mtorr for highly porous TiO 2 ).

  -3). Coherent to what was previously shown by SEM-FEG, the image corresponding to porous TiO2 reveals a film with interconnected narrow cracks between TiO2 isolated grain islands of ~8-10 nm. This provides slight intergrain porosity which is dispersed all over the film as illustrated in figures III-3a and III-3c with two different magnifications. By looking the images of 'highly porous' TiO2 (fig.

Fig. III- 3 .

 3 Fig. III-3. HR-TEM images of porous (a, c) and highly porous (b, d) TiO 2 thin films with 30000X and 150000X magnifications.

  EQCM is a simultaneous measurement of the resonant frequency variations of a quartz resonator determined by QCM during CV measurements. A typical EQCM curve gives the current profile vs potential as well as the simultaneous QCM frequency variation. The quartz resonant frequency variations are converted into mass changes of the electrodes by Sauerbrey relation, i.e. the mass variations of the prepared TiO2 electrodes during reduction bias and oxidation bias can be monitored.

in 0 .

 0 5M LiClO4 aqueous electrolyte are presented in Fig.III-4. The CV curves show a capacitive response in the anodic region whereas the intercalation reaction is observed in the potential range from -0.1 V to -1.1 V vs ECS. An asymmetric voltammogram is obtained with a broad anodic response corresponding to the cation extraction slower than their cathodic insertion at this scan rate value and for the two porous films (Fig.III-4). The capacitive behaviour grows gradually and becomes very well pronounced in the CV response of the highly porous TiO2 film when compared with the current values of dense and porous films (Fig.III-4). This suggests that the high contribution of surface electroadsorption process which is also accompanied with the faradaic response (shown by red arrows in Fig. III-4) corresponds to highly porous TiO2 thin films. Both cathodic and anodic current density of the highly porous film (Fig. III-4c) are higher than those observed for the dense and porous films (Fig. III-4a and III-4b), this may indicate faster cation transfer kinetics. The current values measured are obviously amplified for the very porous films as compared to those obtained for dense and less porous films. The mass variations are also influenced by the presence of the pores (Fig. III-4), and the QCM response is amplified (~ 4 times) in the case of highly porous films. This enhanced behaviour can probably be attributed to the increased specific surface provided by the porous structure, as a result, the pores network provides a better accommodation of the electroactive sites and have an advantageous effect on the species exchange process. The mass responses shown in the reduction branches (Fig. III-4) correspond to the resonant frequency drops of the modified quartz resonators due to the mass increases of the films during reduction bias. In a reverse process, during oxidation bias, the inserted species are expelled out from the film, resulting in a decrease of the electrode mass.

Fig. III- 4 .

 4 Fig. III-4. Cyclic voltammograms and mass responses obtained simultaneously during the electrochemical cycling for (a) dense, (b) porous and (c) highly porous TiO 2 films deposited on the gold coated electrode of the quartz resonator. Measurements are in 0.5M LiClO 4 aqueous solution with a scan rate of 10 mV s -1 .

Fig. III- 5 .

 5 Fig. III-5. values corresponding to the average molecular weight of the species involved in the charge compensation process as a function of the potential for (a) dense, (b) porous and (c) highly porous TiO 2 films cycled in 0.5 M aqueous LiClO 4 solutions (obtained from the reduction branch of the EQCM results at a scan rate of 10 mV s -1 ).

1 .

 1 The charge/potential transfer functions (TFs), (Fig. III-6a and III-b) permit to separate the ionic contribution without any possibility to identify the ionic species involved. Here, it should be mentioned that the contribution of the parasitic reaction, occurring at low frequencies, was removed for keeping only the ionic transfer response. A large and somehow suppressed loop was obtained for both porous and highly porous TiO2 thin films without a fair separation. The theoretical functions in Fig. III-6 indicates that there are more than one charged species involved in both analyzed cases (Fig. III-6a and III-b). Actually, the time constants corresponding to each ionic transfer seem to be very close to each other. It is to be noted that the response of the highly porous film is clearly magnified (2 times) (Fig. III-6b), compared to the response of a porous TiO2 film (Fig. III-6a

Fig. III- 6 .

 6 Fig. III-6. Charge/potential transfer functions, for (a) porous TiO 2 and (b) highly porous TiO 2films measured in 0.5 M LiClO 4 aqueous electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).

Fig. III- 7 .

 7 Fig. III-7. Mass/potential transfer functions, for (a) porous TiO 2 (involving three species, specifically Li + , Li + .H 2 O and ClO 4 -) and (b) highly porous TiO 2 films (involving the same three species). The measurements are performed in 0.5 M LiClO 4 aqueous electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).

Li+

  are the slowest species transferred in both porous films since they are detected at lower frequency region in Fig. III-7a or III-b. It is important to note that the corresponding theoretical equation involves the molecular weight of the ionic and/or nonionic species, providing their identification by their molecular weight. Therefore, cations or their hydrated forms can be detected with an estimation of the hydration level (e.g. cation 1 (c1 = Li + .H2O n =1), cation 2

  /potential TFs were analyzed to validate our previous hypothesis involving three different species for porous and highly porous films. Partial mass/potential TFs are estimated for these films as shown in figure III-8, by removing the c2 contribution, calculating ∆𝑚 ∆𝐸 | 𝑐1𝑎 𝑡ℎ (fig. III-8a and III-d) or by removing the c1 contribution, calculating and III-e) or by removing the anion contribution, calculating ∆𝑚 ∆𝐸 | 𝑐1𝑐2 𝑡ℎ (fig. III-8c and III-f).All these partial mass/potential TFs exhibited a good agreement between the theoretical and experimental data. These TFs provide a crosscheck for validating the hypothesis involving multiple species and for obtaining a better separation of the various contributions.

Fig. III- 8 .

 8 Fig.III-8. Three partial mass/potential transfer functions, for porous (a, b and c) and highly porous (d, e and f) TiO 2 films, measured in 0.5 M LiClO 4 aqueous electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).The Ki and the Gi constants are determined by fitting the experimental data using the theoretical

  species shown in Fig. III-10b and III-10f. This parameter could indeed be defined as the capacity of the film to accommodate each of the previously involved species as a consequence of a potential perturbation given at each applied potential. Based on these values porous TiO2 film have the highest capacitance for transferring the cationic species (Li + and Li + .H2O) specially Li + .H2O and only a small capacitance corresponds to the anions (fig. III-10b).

Fig. III- 10 .

 10 Fig. III-10.Evolution of different parameters as a function of potential including: the characteristic frequency of species, f i , the instantaneous capacitance of species, Cap i , the transfer resistance of species, R ti , and the relative concentration of species (C i -C 0 ) for porous (a-d) and highly porous (e-h) TiO 2 films in aqueous 0.5M LiClO 4 .

Figure

  Figure III-10d and III-10h present the relative concentration change, Ci-C0, as a function of E for Li + , Li + .H2O and species for porous and highly porous TiO2 films. A significant difference is observed in the relative concentration change of the species when TiO2 films are highly porous. Both the (Ci-C0) values for Li + and Li + .H2O cations are magnified for highly porous TiO2 films. The (Ci-C0) values for Li + present quite a difference between the two films,

Fig. III- 11 .

 11 Fig. III-11. Electrogravimetric responses obtained simultaneously during the electrochemical cycling of (a) porous and (b) highly porous TiO 2 films deposited on the gold electrode of a quartz resonator. Measurements are in 0.5M NaClO 4 aqueous solution with a scan rate of 10 mV s -1 .

  pores (blue curves in Fig. III-11), and the QCM response is amplified (~ 2 times)

2 .

 2 The charge/potential transfer functions (TFs), , (Fig. III-12a and III-12b) permit to separate the ionic contribution without any possibility to identify the ionic species involved.Here, the contribution of the parasitic reaction, occurring at low frequencies, was removed for keeping only the ionic transfer response. Similar to what was previously observed in aqueous 0.5 M LiClO4, a large and quite suppressed loop was observed specially in the case of highly porous TiO2 thin films without an easy separation. The theoretical functions in Fig. III-12 indicated that there are more than one charged species involved in both cases (Fig. III-12a and III-12b). Indeed, the time constants corresponding to each ionic transfer seem to be very close to each other. It is to be noted that the response of the highly porous film is magnified almost 3 times (Fig. III-12b), compared to of a porous film. At this level, it is

Fig. III- 12 .

 12 Fig. III-12. Charge/potential transfer functions, for (a) porous TiO 2 and (b) highly porous TiO 2 films measured in 0.5 M NaClO 4 aqueous electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).

Fig. III- 13 .

 13 Fig. III-13. The mass/potential transfer functions, for (a) less porous TiO 2 (involving two species, specifically Na + .H 2 O and ClO 4 -

  TFs exhibited a good agreement between the theoretical and experimental data.

3 )Fig. III- 14 .

 314 Fig. III-14.Evolution of different key parameters as a function of potential including: the characteristic frequency of species, f i , the instantaneous capacitance of species, Cap i , the transfer resistance, R ti and the relative concentration of species, Ci-C0 , for porous (a-d) and highly porous (e-h) TiO 2 films in 0.5M NaClO 4 aqueous electrolyte.

  previously discussed for highly porous TiO2 in 0.5 M LiClO4 aqueous solution are compared when the same electrode is studied in 0.5 M LiClO4/propylene carbonate from -0.7 V to -1 V vs SCE. Before the ac-electrogravimetric discussions, the classical EQCM results of highly porous TiO2 film tested at room temperature for both types of electrolytes and are presented in Fig. III-15.

Fig. III- 15 .

 15 Fig. III-15. Electrogravimetric responses obtained simultaneously during the electrochemical cycling of highly porous TiO 2 films deposited on the gold coated electrode of the quartz resonator. Measurements are in 0.5M LiClO 4 aqueous solution (black curves) and 0.5 M LiClO 4 organic electrolyte (red curves, with a scan rate of 10 mV s -1 ).

Fig. III- 16 .

 16 Fig. III-16. Charge/potential transfer functions, , for highly porous TiO 2 films measured in (a) 0.5 M LiClO 4 aqueous electrolyte and (b) 0.5 M LiClO 4 organic electrolyte at -0.9 V vs SCE (both experimental and theoretical curves are given).

Fig. III- 17 .

 17 Fig. III-17. Mass/potential transfer functions, , for highly porous TiO 2 in (a) 0.5 M LiClO 4 aqueous electrolyte (involving three species, specifically Li + , Li + .H 2 O and ClO 4 -) and (b) 0.5 M LiClO 4 organic electrolyte (involving three species, specifically Li + , PC and ClO 4 -). The measurements were performed at -0.9 V vs SCE (both experimental and theoretical curves are given).

2 -Fig. III- 18 .

 218 Fig. III-18. Partial electrogravimetric transfer functions, for highly porous TiO 2 in 0.5 M LiClO 4 aqueous electrolyte (a, b and c) and in 0.5 M LiClO 4 organic electrolyte (d and e) films measured at -0.9 V vs SCE (both experimental and theoretical curves are given). The partial mass/potential TFs were analyzed to validate the hypothesis involving three different species in both electrolyte types. Partial mass/potential TFs are estimated for porous TiO2 electrode in aqueous LiClO4 solution (figure III-18a-c), by removing the c1 contribution, calculating ∆𝑚 ∆𝐸 | 𝑐2𝑎 𝑡ℎ (fig. III-18a), by removing the anion contribution, calculating ∆𝑚 ∆𝐸 | 𝑐1𝑐2 𝑡ℎ

  figure III-18a and III-18e) that for highly porous TiO2 thin film in both electrolytes: (i) species contribute at high frequencies (the fastest species), even if the presence of the anion is shown only at two potentials in aqueous solution (ii) hydrated lithium ion (Li + .H2O ) appears only in aqueous electrolyte at the intermediate frequencies, and (iii) Li + appears at low frequencies (the slowest species).The instantaneous capacitance of each species, Capi, both in aqueous and organic electrolyte are illustrated in Fig.III-18band III-18f. This shows that the capacity of the highly porous TiO2

3 Fig. III- 18 .

 318 Fig. III-18.Evolution of key parameters as a function of potential including: the characteristic frequency of species (f i ), the instantaneous capacitance of species (Cap i ), the transfer resistance of species (R ti ) and the relative concentration of species (C i -C 0 ) for highly porous TiO 2 film in 0.5M LiClO 4 (a-d) aqueous and 0.5 M LiClO 4 organic electrolyte (e-h).

4

 4 ClO 

des ions 4 ClO

 4 Chapitre IV L'utilisation de films minces d'oxyde métallique avec une porosité à l'échelle nanométrique est devenue un sujet d'intérêt croissant pour diverses applications électrochimiques, par exemple, dans le domaine du stockage d'énergie, pour les dispositifs électrochromes, etc. Parmi ces matériaux, le trioxyde de tungstène, WO3, est un oxyde métallique qui peut offrir une large gamme d'applications technologiques comme décrit dans le chapitre I. Par conséquence, les nouveaux développements et les approches pour améliorer les performances de ces systèmes peuvent avoir un impact technologique direct. L'insertion électrochimique réversible ou l'intercalation d'ions de l'électrolyte dans un matériau présente le principe fondamental de fonctionnement de dispositifs électrochimiques à base de WO3. Par conséquent, il est essentiel d'optimiser les interactions entre les ions de l'électrolyte et ces matériaux d'électrodes. Afin d'optimiser les performances d'une électrode à base de WO3, l'attention principale a été portée sur la nanostructuration de celle-ci. Les propriétés uniques qui en sont issues ainsi que les fonctionnalités peuvent être exploitées pour mettre au point des dispositifs électrochimiques originaux. Comme il a été discuté précédemment dans le chapitre expérimental, la synthèse électrochimique reste une technique simple, peu coûteuse et rapide à basse température qui peut également conduire à la formation de films nanométriques homogènes avec les qualités souhaitées. Cette approche utilise des molécules tensio-actives spécifiques qui adsorbées aux interfaces et sous génération électrochimique du film engendre la formation de films nanostructurés. Après dépôt, les agents tensioactifs utilisés peuvent être facilement éliminés par lavage avec un alcool approprié. Cela conduit à la formation de pores ou de cavités dues aux phases tensio-actives insérées dans le film électrogénéré. Ces nanostructures, avec des pores de petite taille et des grands rapports surface sur volume, sont censés faciliter les processus de transfert/transport d'ions à l'interface films/électrolyte. Pour suivre cette idée, le présent chapitre fournit une étude approfondie des processus d'intercalation/d'électroadsoption des ions au sein de films de WO3 mésoporeux. Ici, nous nous concentrons particulièrement sur les matériaux amorphes plutôt que cristallisés dans le but de souligner le rôle de cette structuration sur les performances électrochimiques des films de WO3. Ces films minces mésoporeux de WO3 ont été préparés par voie électrochimique en utilisant un tensioactif ionique, le SDS, lors de l'électrosynthèse. Représentation de la topographique de la molécule tensio-active utilisée en tant que porogène dans la présente étude. La structure, la morphologie et la composition des films mésoporeux de WO3 synthétisés ont été étudiées et comparées à leurs analogues denses. Les propriétés électrochimiques de ces films sont ensuite examinées. Les mécanismes d'électroadsorption/intercalation ont été regardés dans une solution aqueuse de LiClO4 par des méthodes électrogravimétriques (EQCM et acélectrogravimétrie). Les courbes d'électrogravimétrie montrent une réponse quasiment capacitive dans la région anodique. En accord avec les données de la littérature dans des conditions similaires, un voltamogramme asymétrique est obtenu avec le film dense. La densité de courant cathodique et anodique des films mésoporeux est plus élevée que celle observée pour les films denses, ce qui peut indiquer une cinétique plus rapide de transfert des ions. Les valeurs de densité de courant mesurées sont presque quatre fois supérieures à celle obtenue pour un film dense. Les variations de masse sont également influencées par la présence des mésopores, la réponse de la microbalance est amplifiée environ 4 fois dans le cas de film mésoporeux. Ce meilleur comportement est attribué à une meilleure surface spécifique. En effet, un meilleur accès aux sites électroactifs est fourni et c'est un effet avantageux pour la réponse électrochimique d'électrodes poreuses à base de WO3. Electrogravimétrie cyclique lors de la réaction électrochimique (A) de couches minces de WO 3 dense et (B) de couches minces de WO 3 mésoporeux déposés sur l'électrode d'or d'un résonateur à quartz 9MHz. Les mesures sont en solution aqueuse 0,5 M LiClO 4 avec une vitesse de balayage de 50 mV s -1 . Des analyses d'ac-electrogravimetrie permettent de détecter la contribution des espèces chargées ou non-chargé pendant les différents processus électrochimiques. Plus précisément, notre étude identifie clairement et de manière indiscutable l'implication de plusieurs espèces chargées (Li + , Li + .H2O) lors de la compensation de la charge, ainsi que les molécules libres de solvant qui contribuent indirectement au processus. D'une manière surprenante, une légère contribution  a été détectée dans le cas des films mésoporeux de WO3. Les résultats de l'étude indiquent aussi que les résistances de transfert de Li + et Li + .H2O diminuent lorsque les films de WO3 sont mésoporeux. Une différence significative est surtout observée pour les ions les plus grands comme Li + .H2O partiellement déshydratés. Cela suggère une augmentation de la surface en raison du volume des pores créé par la morphologie mésoporeuse ce qui facilite le transfert d'espèces chargées d'une manière tout à fait remarquable. Les changements des concentrations relatives des ions sont également amplifiés dans ces films amorphes et structurés. Schéma illustratif de l'étude effectué par ac-électrogravimétrie. Les variations de la concentration finale des cations sont beaucoup plus élevées dans les films mésoporeux que celles des films denses; environ 4 fois plus élevé pour Li + et environ 10 fois plus élevé pour Li + .H2O . Dans la littérature, il n'est pas fait mention de cette identification sans ambiguïté des différentes espèces. En effet, il est en général indiqué que seuls les cations déshydratés comme par exemple les ions Li + sont impliqués. De plus, notre stratégie permet d'obtenir des informations sur la dynamique de transfert et la quantification des espèces impliquées, point qui n'a jamais été trop abordé dans la littérature pour décrire le processus de compensation de charge du WO3. Introduction

  temperature and rapid alternative to the mesoporous thin film synthesis. The structure, morphology and the composition of the mesoporous electrochemically synthesized films were characterized, and compared with their dense counterparts. The electrochemical performance and ion intercalation/extraction mechanisms were studied in aqueous LiClO4 electrolytes by electrogravimetric methods (EQCM, and ac-electrogravimetry). Special attention was given to the poorly understood aspects, such as the nature of the ions involved in the charge compensation, solvation and the role of the electrolytes and the dynamic information of ions transfer at the electrode/electrolyte interfaces. It has been demonstrated herein that the ac-electrogravimetry responses of the electrodeposited WO3 thin films can serve as a gravimetric probe to study the complex Li + intercalation/extraction mechanisms and to extract subtleties unreachable with classical tools.

  previous reports (Fig.IV-1)[21, 45]. Similar morphologies are obtained for the mesoporous counterparts on the scale of FEG-SEM observations. The average film thickness is ~300 nm under these experimental conditions (Fig.IV-1B), and it can be tailored by changing the electrodeposition time.

Fig. IV- 1 .

 1 Fig. IV-1. FEG-SEM images showing the top view (A) and the cross-section (B) of an as deposited dense WO 3 thin film (electrodeposited on the Au electrode of a quartz resonator at -0.5 V vs Ag/AgCl during 20 min).

Fig. IV- 2 .

 2 Fig. IV-2. Compositional analysis by energy dispersive X-ray (EDX) spectroscopy of a dense WO 3 thin film (obtained by FEG-SEM equipped with an EDX detector) (substrate: gold electrode of the quartz resonator). The EDX analysis coupled with FEG-SEM observations indicates the presence of W and O in as-deposited dense thin films (Fig. IV-2). A small contribution of Au also appears which is due to the gold electrode of the quartz crystal substrate. The EDX spectrum of films synthesized in the presence of SDS templates (not given here) showed additional peaks corresponding to Na element, indicating the successful incorporation of the SDS templates in the inorganic/organic hybrids. The contribution of Na peak is substantially decreased after the extraction of the SDS templates, signifying the facile removal of the SDS templates (discussed in experimental section).

Fig. IV- 3 .D

 3 Fig. IV-3. HR-TEM images (A, B, C) and the EDX pattern (D) of mesoporous WO 3 thin films deposited by surfactant assisted electrodeposition (using SDS) at -0.5 V vs Ag/AgCl for 30 min, sample is thermally treated at 450°C for 2h.

Fig. IV- 4 .

 4 Fig.IV-4. X-ray Photoelectron Spectroscopy (XPS) survey spectrum (A) and the corresponding W 4f core level spectrum (B) of as-prepared dense WO 3 film electrosynthesized at -0.5 V vs Ag/AgCl for 20 min.

B

  To determine the exact composition and the oxidation state of the W species, as-deposited thin films were characterized by X-ray photoelectron spectroscopy (XPS) and the results are shown in Fig.IV-4. All peaks can be indexed to W and O elements (except the presence of Au peaks due to the substrate) indicating the high purity of as-synthesized sample. A fitting curve of the W 4f level is presented in Fig.IV-4B. The peaks at binding energies of 35.6 and 37.7 eV match

Fig. IV- 5 .

 5 Fig. IV-5. Cyclic voltammograms and mass responses obtained simultaneously during the electrochromic response of (A) dense and (B) mesoporous WO 3 thin films deposited on the gold electrode of the quartz resonator. Measurements are in 0.5M aqueous solution of LiClO 4 with a scan rate of 50 mV s -1 .The EQCM results of a dense and mesoporous WO3 film tested at room temperature in aqueous 0.5M LiClO4 electrolytes are presented in Fig.IV-5. The CV curves show a quasi-capacitive response in the anodic region whereas the coloration reaction is observed in the potential range of -0.15 V to -0.5 V vs Ag/AgCl. In agreement with the literature data under similar dynamic

Fig

  Fig. IV-6. m F q    values corresponding to the average molecular weight of the species involved in the charge compensation as a function of the potential for a dense (A) and a mesoporous (B) WO 3 film cycled in 0.5 M aqueous LiClO 4 solutions (obtained from the reduction branch of the EQCM results at a scan rate of 50 mV s -1 ).

  performed on mesoporous WO3 films and compared with their dense analogues.

Fig. IV- 7 .

 7 Fig. IV-7. The electrochemical impedances,

Fig. IV- 7 

 7 Fig. IV-7 exhibits the electrochemical impedance spectroscopy,   E () I  , of a dense and

Fig. IV- 8 .

 8 Fig. IV-8. Charge/potential transfer functions,

Fig. IV- 9 .,

 9 Fig. IV-9. The mass/potential transfer functions,

4 ClO  Fig. IV- 10 .,

 410 Fig. IV-10. Three partial transfer functions, for a mesoporous WO 3 thin film, (A)

  Li + ions and remarkably ~13 times for hydrated lithium ions (Li + .H2O) in the case of mesoporous films compared to dense films.

Figure IV- 11

 11 Figure IV-11 shows the evolution of the kinetic parameters, Ki, and the transfer resistance, Rti, of the species as a function of the potential applied. This potential range corresponds to the conditions where the electrochemical process of the WO3 thin films is observed. Based on the Ki values presented in Fig. IV-11 A and IV-11 B, Li + ions are persistently the fastest species transferred both in dense and mesoporous WO3 thin films.

Fig. IV- 11 .

 11 Fig. IV-11. Evolution of kinetic parameters, K i , for a dense (A) and mesoporous (B) WO 3 thin films, and the comparative curve of the transfer resistance values, Rt i , for cationic species in dense and mesoporous WO 3 thin films, Li + ions (C), and Li + .H 2 O ions (D), presented as a function of applied potential.

  values shown in Fig. IV-11. The transfer kinetics of the larger, partially dehydrated Li + .H2O is in the same order of magnitude in both mesoporous and dense films (Fig. IV-11 A and B). The transfer kinetics of free water molecules are somehow close to the values of the Li + ions in Fig. IV-11A and IV-11B. Additionally, these water molecules have the same flux directions with the cations, suggesting that they might be the water molecules accompanying the transfer of Li + species most likely due to an electrodragging

  the insertion isotherm. Fig. IV-12 presents the calculated relative concentration changes, (Ci-C0) for Li + , Li + .H2O, H2O and species for dense (Fig. IV-12 A) and mesoporous WO3 (Fig. IV-12B) thin films. A significant difference is observed when WO3 thin films are mesoporous. Both the (Ci-C0) values for Li + and Li + .H2O cations are magnified for mesoporous films. It is important

4 ClO  Fig. IV- 12 .

 412 Fig. IV-12.Evolution of the relative concentration, C i -C 0 , of each species over the potential applied, for a dense (A) and a mesoporous (B) WO 3 thin film, measured in 0.5 M LiClO 4 aqueous electrolyte.

  is more likely related to the better accommodation of both Li + and

Fig. V- 1 .

 1 Fig. V-1. The X-ray diffraction patterns of as-prepared RuO x .nH 2 O and RuO 2 films electrodeposited on Au substrate at -0.6V vs Ag/AgCl for 1h (a) as-prepared sample (b) annealed sample at 450°C for 2h.

Fig. V- 2 .

 2 Fig. V-2. SEM-FEG characterization of as-prepared compact (a, b) and mesoporous (c, d) RuO x .nH 2 O. (The samples are electrodeposited at -0,5 V for 30 min).

Fig. V- 3 .

 3 Fig. V-3. Mean changes electrodeposited RuO x .nH 2 O film thickness at different deposition times determined through SEM-FEG measurements (left) cross-section image of the as-prepared RuO x .nH 2 O (right) (prepared potentiostatically at -0,5 V during 1h).

Fig. V- 4

 4 Fig. V-4 shows the morphological state of the surface of SWCNTs covered by a thin layer of RuOx.nH2O electrodeposited with three different magnifications. The surface of virgin fine chains of carbon nanotubes is protected with a grey like coverage of hydrated ruthenium oxide film.

Fig. V- 4 .

 4 Fig. V-4. SEM-FEG images of SWCNTs electrode covered by thin layer of hydrated ruthenium oxide.

Figure V-5a

  Figure V-5a illustrates the morphology of the compact as-prepared RuOx.nH2O film consisting of dense dark branches. The SAED (fig. V-5c) reveals a certain crystallinity with the presence of faint rings. The as-prepared film is indexed as metallic Ru (hcp). In Figure V-5b different morphologies are observed after annealing at 450°C during 2h. In this image small grains, bigger grains and also compact branches co-exist together, but with exactly the same diffraction pattern. At 450°C, the SAED pattern is modified. It exhibits the polycrystalline nature of tetragonal RuO2: the RuO2 rutile structure.

Fig. V- 5 .

 5 Fig. V-5. TEM images and corresponding SAED for compact as-prepared RuO x .nH 2 O (a, c) and (b, d) RuO 2 heated at 450°C.

Fig. V- 6 .

 6 Fig. V-6. TEM images with corresponding SAEDs for as-prepared mesoporous RuO x .nH 2 O heated at 150°C (a, c) and (b, d) mesoporous RuO 2 calcinated at 450°C.

Fig. V-

  Fig. V-6a reveals nanoparticles of ~ 2-3 nm but the porosity is not evident and difficult to measure for the 150°C sample. Furtherly when the film is thermally treated up to 450°C the most distinguishable change is the appearance of grown aligned grains of around 6-7 nm and also the clear existence of intergrain porosity (fig. V-6b). The observations are accompanied by

Fig. V- 7 .

 7 Fig. V-7. TEM images with corresponding SAEDs for as-prepared compact (a, c) and mesoporous RuO x . nH 2 O.

  nH2O (Fig. V-8a, V-8b) along with an image of annealed RuO2 at 450°C are presented here (Fig. V-8c). The term non-porous and/or compact RuOx.nH2O is used to differentiate the films prepared by classical electrodeposition from mesoporous films prepared by surfactant-assisted electrodeposition using CTAB.

Fig. V- 8 .

 8 Fig. V-8. HR-TEM images for (a) as-prepared compact (b) as-prepared mesoporous and (c) 450°C annealed RuO x . nH 2 O.

Fig. V- 9 .

 9 Fig. V-9. HR-TEM images of SWCNT/RuO x .nH 2 O; the inset shows a sole SWCNT.

Fig. V- 11 .

 11 Fig. V-11. XPS results for as-prepared compact (a, b) and mesoporous (c, d) RuO x .nH 2 O: O 1s (a, c), Ru 3d (b, d) core level spectra.Foelske et al. [27] determined that a peak centered at 282.6 eV and developed at temperatures above 150 °C was indicative of an amorphous crystalline transition. The development of this peak with increasing temperature (compare Fig V-12 and V-13) suggests that this feature is an indication of ruthenium oxide hydration level and crystallinity, its onset in accordance with kinetic and thermal data indicating the loss of structural water. Assignment of this peak to RuO3 is discounted because of the Ru/O stoichiometry already discussed in respect to the 3d orbitals.

Fig. V- 12 .

 12 Fig. V-12. XPS results for as-prepared compact (a, b) and mesoporous (c, d) RuO x .nH 2 O annealed at 150°C for 2h: O 1s (a, b), Ru 3d (b, d) core level spectra. For O (1s) peak assignment, we first consider the anhydrous oxide and assign lattice oxygen to the signal at 529-529.1 eV. Since the sample is annealed at high temperature, it is equally difficult to assign this signal to water. The fitting of the Ru(3d)/C(1s) level indicates the presence of oxygen containing carbon bonds and so assigns this O (1s) energy to organic C-O bonds. This is confirmed by the absence of significant concentration of such species in the hydrated ruthenium oxide Ru (3d)/C (1s) spectrum. The remaining peak at 530.8 eV is at first readily assigned to surface hydroxide and supported by the extra intensity in the hydrated RuO2 sample (Fig. V-11); however, it is clear from the thermal studies that the overall density of any

Fig. V- 13 .

 13 Fig. V-13. XPS results for compact and mesoporous RuO 2 annealed at 450°C for 2h: O 1s (a, b), Ru 3d (b, d) core level spectra.

III- 1 .

 1 Cyclic electrogravimetryAs previously introduced in the experimental chapter, EQCM is a simultaneous measurement of the resonant frequency variation of a quartz resonator determined by QCM and of the current during CV measurements. A typical EQCM curve gives the potential vs current profile, simultaneous to the microbalance frequency variation vs applied potential as shown in fig. V-14. The quartz resonant frequency variations are converted into mass changes through the Sauerbrey relation (chapter II eq. 1)

Fig. V- 14 .

 14 Fig. V-14. CVs for both compact (a) and mesoporous (b) RuO x .nH 2 O in H 2 SO 4 0.5 M (black) and Na 2 SO 4 0.5 M (blue).

Fig. V- 15 .

 15 Fig. V-15. Mass changes for both compact (a) and mesoporous (b) RuO x .nH 2 O in H 2 SO 4 0.5 M (black) and Na 2 SO 4 0.5 M (blue). The EQCM results of compact and mesoporous RuOx.nH2O film tested at room temperature in aqueous 0.5M H2SO4 and 0.5M Na2SO4 electrolytes are presented in Fig. V-14 (I vs. V) and Fig. V-15 (mass vs. V). The CV curves show a typical rectangular type capacitive response in the potential range of 0.2 V to 0.9 V vs Ag/AgCl. In agreement with the literature data under similar dynamic conditions, a symmetric capacitive voltammogram is obtained suggesting the same rate of ions exchange at this scan rate (Fig. V-14).

Fig. V- 16 .

 16 Fig. V-16. Specific Capacitance for both compact (a) and mesoporous (b) RuO x .nH 2 O in H 2 SO 4 0.5 M (black) and Na 2 SO 4 0.5 M (blue).

  V-18c and V-18d), one big loop appears in the third quadrant. This loop can be attributed to either two species or three species where their time constants are not sufficiently different from each other. The loops in the third quadrant are characteristic for cation contributions or free solvent molecules in the same flux direction.Another contribution also appears in Fig.V-18d(for the mesoporous RuOx. nH2O thin film) at very low frequencies in the fourth quadrant (either anions or water molecules with opposite flux direction compared to cations) highlighting the challenge in obtaining an exact identification of these loops. Therefore, several configurations were tested using theoretical functions to determine the exact contribution of each species. The mass/potential TF response of a compact RuOx.nH2O thin film was fitted by considering three species cation 1 (c1= H + ), free solvent molecules (s= H2O) and cation 2 (c2=H3O + ) (Fig.V-18c). In the case of a mesoporous RuOx.nH2O film, a similar response is obtained, but with an additional contribution from another charged species, the anion (a= SO42-), which appears at very low frequencies (Fig.V-

1 Fig. V- 18 .

 118 Fig. V-18. ac-electrogravimetric results for both compact (left side images) and mesoporous (right side) RuO x .nH 2 O at 500 mV in H 2 SO 4 0,5M. (a,b) Charge/Potentiel Transfer Function: , (c,d)

1 Fig. V- 19 .

 119 Fig. V-19. Partial Mass/Potentiel transfer function for both compact (a and c) and mesoporous (b and d) RuO x .nH 2 O at 500 mV in H 2 SO 4 0,5M: partial when c2 contribution is eliminated (a and b)

Fig. V- 20 .

 20 Fig. V-20. Evolution of characteristic frequencies of each species, f i , as a function of applied potential for compact (left) and mesoporous (right) RuO x .nH 2 O in H 2 SO 4 0,5M.Coherent to what was already explained in the previous paragraph, from the evolution of characteristic frequencies, fi, of species (fig. V-20) in both cases, the rate of transfer is higher in the case of mesoporous films, and this allows a possible fast charge or discharge to be performed.

Fig. V- 21 .

 21 Fig. V-21. Evolution of Instantaneous Capacitance for each species, Cap i , as a function of applied potential for compact (left) and mesoporous (right) RuO x .nH 2 O in H 2 SO 4 0,5M.

Fig. V- 22 .

 22 Fig. V-22. Evolution of transfer resistance, Rt i , for each Species as a function of applied potentials; comparison between each involved species in both compact and mesoporous RuO x .nH 2 O in H 2 SO 4 0,5M.

Fig. V- 23 .

 23 Fig. V-23. Evolution of the concentration changes, 0 i CC  , of each species over the potential applied for compact (a) and mesoporous (b) RuO x .nH 2 O in H 2 SO 4 0,5M.

Fig. 24 .

 24 Fig. 24. ac-electrogravimetric results for both compact (a,c) and mesoporous (b,d) RuO x .nH 2 O at 500 mV in Na 2 SO 4 0,5M. (a,b) Charge/Potentiel Transfer Function: , (c,d) Mass/Potentiel Transfer

(c 1 (

 1 example at 500 mV presented at fig. V-24c and V-24d) is the apparition of anions at HF for compact films while in mesoporous counterpart the anion is only detected at very LF. Also in the contrary to what was expected from previously discussed results for mesoporous in H2SO4, here, only two charge species contribute. Therefore, at this stage it could be speculated that mesoporous film could provide accommodation for only two charged species, a cation and cation 1): Na +

4 Fig. V- 25 .

 425 Fig. V-25. Characteristic frequencies, f i , evolution as a function of applied potential for compact (left) and mesoporous (right) RuO x .nH 2 O in Na 2 SO 4 0,5M. The instantaneous capacitances, Capi, are presented in fig. V-26. Both in compact and mesoporous RuOx.nH2O, except the irregularities observed at 500 mV and 800 mV for H3O + ,

4 Fig. V- 26 .

 426 Fig. V-26. Evolution of the Instantaneous Capacitance, Cap i , as a function of applied potential for compact (left) and mesoporous (right) RuO x .nH 2 O in Na 2 SO 4 0,5M.

Fig. V- 27 .

 27 Fig. V-27. Evolution of the concentration, 0 i CC  , of each species over the potential applied for compact (a) and mesoporous (b) RuO x .nH 2 O in Na 2 SO 4 0,5M.

206Fig. V- 29 .

 29 Fig. V-29. ac-electrogravimetric results: Charge/Potentiel Transfer Function, , and

  4 and were used in the following fittings. Then, to identify and clarify the contribution of the charged and also the uncharged species (i.e. free electrolyte molecules), the mass/potential transfer functions, cation 1): H +

4 Fig. V- 30 .

 430 Fig. V-30. Evolution of Characteristic frequency (f i ), Instantaneous Capacitance of Species (Cap i ), transfer Resistances of each Species (Rt i ) and the relative concentration of species ( 0 i CC  ) as a function of potential for RuO x .nH 2 O, SWCNTs and SWCNTs/RuO x .nH 2 O at 500 mV in H 2 SO 4 0,5M.

Table I - 1 .

 I1 Comparison of the Performances of Supercapacitors Based on Tungsten Oxides and Other Popular Active Materials [57].

Table II -

 II

		7 16 3 10 1 . 	0.58	19.93

1. Values of various parameters used for the measurements correction.

Table III -2. Estimated

 III

values for K i (kinetics of transfer), G i (inverse of the transfer resistance), R ti (transfer resistance) and -G i /K i (the quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in 0.5M NaClO 4 aqueous electrolyte at -0.9 V vs. SCE for porous and highly porous TiO 2 films.

  Li + species contribute at high frequencies (the fastest species), (ii) free water molecules appear at the intermediate frequencies, and (iii) Li + .H2O appears at low frequencies (the slowest species). In the case of mesoporous WO3 thin films, an additional contribution is

		V -1
		-2
	Li + 0.1 Hz Experimental Li + .H 1 Hz 2 O Theoretical and : freq. decade of species at the electrode/electrolyte interfaces. Both for dense and mesoporous WO3 thin H 2 O 10 Hz -Im(m/E) C1C2S /g cm Re(m/E) C1C2S /g cm -2 V -1 films: (i) observed at the lowest frequency range corresponding to the anions transfer ( ) and their
	transfer kinetics is slower than cationic species and free water molecules (see values in Table
	IV-1). The Gi values determined from the ac-electrogravimetric study are related to the transfer
	resistance, (	i Rt		1 FG i

  -1).

	Specifically, for dense films, it pursues the order: Rti (Li + .H2O)> Rti (H2O)> Rti (Li + ), and for
	mesoporous films the same order persists: Rti (	4 ClO  )> Rti (Li + .H2O)> Rti (H2O)> Rti (Li + ),
	except the presence of additional	4

un film mésoporeux de RuO 2 ; effet de CTAB sur la porosité et la taille des grains du matériau électrogénéré.

  Chapitre VL'importance des condensateurs électrochimiques à base de RuO2 a déjà été discutée dans le chapitre bibliographique. En bref, RuO2 présente une capacité spécifique beaucoup plus élevée que tous les autres oxydes de métaux ou de différents types de carbone. Ce matériau présente également une conductivité métallique élevée et une faible résistance interne, ce qui peut provoquer un processus de charge-décharge rapide[1][2][3][4]. Cependant, de façon similaire aux films WO3 et TiO2 précédemment étudiés, la majorité des travaux récents ne proposent que de nouveaux modes de synthèse pour atteindre une capacité spécifique plus élevée. Il est notable qu'il y a un manque de techniques de diagnostic puissantes capable d'apporter des informations essentielles sur l'apport positif de cette nanostructuration de ces oxydes métalliques[5][6][7].La perméabilité de ces films d'oxydes de ruthénium hydratés compacts et mésoporeux vis-àvis des ions (intercalation / electroadsorption) a été étudié par ac-électrogravimétrie. La nature chimique et le rôle de chaque espèce (ions, ions solvatés et molécules de solvant libre), + et H3O + ) impliquées dans le processus de compensation de charge ; molécules d'eau contribuent indirectement au processus dans les deux films de RuOx.nH2O compacts et mésoporeux. Même une légère contribution des ions SO4 2-a été détectée dans le cas des films mésoporeux. La contribution de l'espèce chargée a été amplifiée dans les films de RuOx.nH2O mésoporeux par rapport aux homologues compacts. Cette étude qualitative et quantitative de la contribution des espèces ioniques dans le processus de compensation de charge, ainsi que des informations dynamiques du transfert interfacial prouve encore le caractère avantageux des films RuOx.nH2O structurés pour des applications énergétiques. Il a été prouvé que le film mésoporeux RuOx.nH2O accueille mieux les espèces

	Chapter V : RuO x .H 2 O
	directement ou indirectement impliquées dans les processus électrochimiques a été estimée
	pour la première fois. L'influence de la nanostructuration sur la dynamique du transfert des ions
	et l'impact de la taille des cations de l'électrolyte ont été examinés dans deux électrolytes
	aqueux, H2SO4 et Na2SO4.
	Les résultats de nos études en solution aqueuse de H2SO4 ont conduit à l'identification de
	Dans la première partie de ce chapitre, les deux techniques classiques (EQCM) et non-classiques (ac-électrogravimétrie) ont été exploitées pour étudier les mécanismes de transfert d'ions à l'interface film RuOx.nH2O mésoporeux/électrolyte. Pour leur fabrication, similairement aux résultats discutés précédemment pour WO3, l'électrogénération en présence de tensioactifs a été choisie. L'utilisation de CTAB comme agent tensio-actif ionique pendant la préparation électrochimique de films RuOx.nH2O a conduit à la création de mésopores de ~ plusieurs espèces chargées (H cationiques. Les ions H + en particulier, sont transférés rapidement à l'interface électrode
	mésoporeux / électrolyte, et leur profil de concentration relative en fonction du potentiel est
	significativement plus élevé par rapport aux valeurs obtenues pour leurs analogues compacts.
	L'étude a aussi été développée en solution aqueuse de Na2SO4, pour étudier à la fois l'impact de
	la taille du cation et du pH. A partir des profils cinétiques et thermodynamiques obtenus (fi vs
	E, Rst vs E, Cap vs E et Ci-C0 vs E), il a été conclu que les films mésoporeux ne présentent aucun
	avantage. En effet, nos études ont confirmé que les résultats les plus notables de RuOx.nH2O
	sont obtenus dans une solution de H2SO4.

7-10 nm qui sont organisés autour des micelles correspondantes. Les analogues denses ont été également synthétisés par la voie électrochimique dans les conditions similaires mais en l'absence des molécules de CTAB. La structure, la morphologie et la composition des films electrosynthétisés mésoporeux ont été caractérisés et comparés avec leurs homologues compacts. Image HR-TEM d'

  in rutile structure is 4. The mechanism of formation of pure RuO2 from RuCl3•nH2O precursor is rather complex. Nevertheless, when it comes to the potential application of this metal oxide the fitted photoelectron peaks gives a Ru/O ratio of ~0.3 and is attributed to Ru(OH)3, an assignment in line with hydrolysis products. The small deviation in the ratio probably due to C-O containing species presents as evident from the C(1 s)/Ru(3d) region. The Ru-Cl bond were identified and assigned to the signal at 199 eV. The changes at the surface of RuCl3, XPS the rutile structure, this was very well supported by our XPS results. Also the presence of structural water in the as-prepared and 150°C heated RuOx.nH2O samples is the reason of their differences with RuO2 in rutile structure. However, their XPS spectra remain quite similar, proving the co-existence of Ru metallic and hydrous RuOx.nH2O in the asprepared and 150°C annealed sample, the pure rutile RuO2 for the 450°C heated sample.

	(i)	RuO x .nH 2 O and RuO 2
	Figures V-11 to V-13 show the Ru (3d) and O (1s) regions for hydrated RuO2 (fig V-11 and V-
	12
	reveals two co-existing Ru(III) species, RuCl3 and Ru(OH)3, where Ru (3d5/2) signal at 282.5
	eV and Cl (2p3/2) at 199eV are due to RuCl3.
	Based on previously discussed conventional XRD and SAED results of samples, RuO2 annealed
	at 450°C has Compound	Peak	Binding	Std. Dev.
				Energy (eV)
		Ru (0)	Ru 3d 5/2	279.8	0.1
			Ru 3d 3/2	284.0
			Ru 3d 5/2	280.8
		RuO 2	Ru 3d 3/2	284.8	0.6
			Ru 3d 5/2sat.	282.5
			Ru 3d 3/2sat.	286.7
			Ru 3d 5/2	280.8
		RuO 2 . nH 2 O	Ru 3d 3/2	285.0	0.6
			Ru 3d 5/2sat.	282.7
			Ru 3d 3/2sat.	286.9
		RuCl 3	Ru 3d 5/2 (chloride)	282.8
		and	Ru 3d 3/2 (chloride)	287
			Ru 3d 5/2 (hydroxide)	282.3
		Ru(OH) 3	Ru 3d 3/2 (hydroxide)	286.4

Table V-1. Reference binding energies of Ru 3d core level for different Ru compositions [15].

Table V - 2 .

 V2 Estimated values for K i (kinetics of transfer), G i (the inverse of the transfer resistance), R ti (transfer resistance) and -G i /K i (the quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in aqueous 0.5M H 2 SO 4 at 500 mV vs. Ag/AgCl for dense and mesoporous RuO x .nH 2 O films.

							1 )
	Compact RuOx.nH2O
	c 2 (cation 2): H 3 O +	f=0.15 Hz	2.9	0.47×10 -4	0.028×10 -6	366	-6×10 -4
	19 g mol -1
	s (solvent): H 2 O	f=5.5 Hz		17.3×10 -4	0.86×10 -6	12	-5×10 -4
	18 g mol -1
	c 1 (cation 1): H +	f=6 Hz	17	18.9×10 -4	6.6×10 -6	1.57	-35×10 -4
	1 g mol -1
	Mesoporous RuOx.nH2O
	c 2 (cation 2): H 3 O +	f=3 Hz	1.93	1,885×10 -4	0.377×10 -6	27.5	-20×10 -4
	19 g mol -1
	s (solvent): H 2 O	f=11 Hz		6.9×10 -4	0.345×10 -6	30	-5×10 -4
	18 g mol -1
	c 1 (cation 1): H +	f=40 Hz	15	25×10 -4	39×10 -6	0.26	-155×10 -4
	1 g mol -1
	a (anion): SO4 2-	f=0.04 Hz	0.08	0.025×10 -4	-0.00024×10 -6	-48510	0.85×10 -4
	98 g mol -1

  2-) and their transfer kinetics is slower than cationic species and free water molecules (see values in TableV-2). When the two types of films are compared some difference in the level of its rapidity are observed between these two structures: H + is over ten time faster in mesoporous film while both H + and H2O are observed very close in the middle frequencies (around 12 Hz) in dense counterparts. The second main difference is the absence of anion in

compact RuOx.nH2O films while even very slight presence of anion at very low frequencies is identified in mesoporous film. Also, the H3O + ions which appear at low frequencies below ~ 1Hz in the compact film are fastened almost ten times in mesoporous analogues. About the

Table V - 3 .

 V3 Estimated values for K i (kinetics of transfer), G i (inverse of the transfer resistance), Rt i (transfer resistance) and -G i /K i (the quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in aqueous 0.5M Na 2 SO 4 at 500mV vs. Ag/AgCl for dense and mesoporous RuO x .nH 2 O films.

  2-) with their transfer kinetics slower than cationic species (see values in TableV-3). It is difficult to compare the two types of films, with the exception of Na + which appear at MF in both cases. The anion apparition is quite different in these two films as in compact RuOx.nH2O, sulfate ions appear at HF but at LF in mesoporous films.

Table V - 4 .

 V4 Estimated values for K i (kinetics of transfer), G i (the inverse of the transfer resistance), Rt i (transfer resistance) and -G i /K i (the quantity transferred per potential unit) parameters extracted from the fitting results of ac-electrogravimetric measurements in H 2 SO 4 0.5M at 500 mV vs. Ag/AgCl for SWCNTs and SWCNTs/RuO x .nH 2 O films. contrary to RuOx.nH2O and similar to SWCNTs the anions are the slowest species detected at LF.The evolution of instantaneous capacitance, Capi, is shown in Fig V-30 (d, e and f) for RuOx.nH2O, SWCNTs and SWCNTs/RuOx.nH2O, respectively. Compared to SWCNTs which does not exhibit high capacitance values for H + (average value around 2 mF cm -2 ), the capacitances measured for SWCNTs/RuOx.nH2O are over 4 times magnified and this film specifically favors H + ions which is comparable to what was observed for pure RuOx.nH2O.

x .nH 2 O H 2 SO 4 0.5 M

  2-anions which remains to be the most difficult ions to transfer. The resistance of anions in case of SWCNTs and SWCNTs/RuOx.nH2O composite films is much more important than what was observed for RuOx.nH2O.

							 SWCNTs	 RuO x .nH 2 O/
							in H 2 SO 4 0.5 M	SWCNTs in H 2 SO 4
							0.5 M
	100	a)					H H	+ 3 O	+
	10						H	2 O
							SO
	1 f i /Hz
	0,1
	0,01
		0,3	0,4	0,5	0,6	0,7	0,8
			E vs Ag/AgCl /V

 RuO

Schéma de principe de la microscopie électronique à transmission (à gauche) et image à haute résolution d'un film mésoporeux de trioxyde de tungstène (à droite).La fabrication de films mésoporeux d'oxydes de ruthénium hydraté (résultats présentés dans le chapitre V), comme pour l'élaboration des films de WO3, est basée sur une électro génération

Chapter IV: WO 3 I.

des paramètres cinétiques précédemment introduits sont également présentés pour des films de CNTs et des films de RuOx•nH2O pour permettre une comparaison complète afin d'obtenir une meilleure compréhension des différentes réponses en fonction de la nature des trois films.

Schéma comparatif de la variation de la concentration des espèces pour un film CNTs pur (image à gauche) et un film composite CNTs/ RuO x .nH 2 O (à droite).

Le comportement des films composites montre, comparativement aux autres films, une amélioration notable en termes de capacité instantanée ainsi qu'un nombre amplifié de cations transférés au sein de ces films. Cette nouvelle structure composite combine plusieurs avantages comme la haute conductivité et la grande surface spécifique des CNTs ainsi que le caractère pseudo-capacitif des couches minces de RuOx.nH2O composées de grains nanométriques.

as supercapacitor there are several reports accentuating on the preferable functionality of hydrated ruthenium oxide, RuOx.nH2O [22][23][24]. Therefore, it is curious to follow the evolution of oxidation states when both compact and mesoporous films lose their hydration content by progressive thermal treatment and to compare their binding energy values with what is reported in the literature. To follow this investigation, first RuCl3.xH2O as the main precursor is analyzed. This provides a reference for both O1s and Ru3d binding energies as shown in fig.

V-10.

(i) XPS results of RuCl 3 .xH 2 O Precursor:

The acquisition reveals a Ru (3d5/2) signal at 282. compounds in our analysis and also in ref [15], it is expected that this would be attributable to trivalent ruthenium. The O (1 s) signal at 530.5 eV is assigned to OH groups, and the ratio of Moreover, for a complex electrochemical process, these values correspond to an average molecular weight related to the various species, and it is actually an average in terms of mass and kinetics [32]. Therefore, at this point, one can arguably discuss that at this scan rate (20 mV s -1 ), H + ions are exclusively involved in the charge compensation process (Fig. V-17c).

III-3. Relative Molecular Mass Estimation,

However, it cannot guarantee the absence of any other species which may have different time pH of this electrolyte: in H2SO4 solution H + ions could most efficiently interact with hydrated RuOx.nH2O electrodes as the concentration of these species is high. The second hypothesis could be related to the cation size effect and the fact that bigger Na + ions might not be preferable compared to H + ions. This later hypothesis, however is debatable since both ionic radius of H + and Na + are small enough to be able to find their way through the nanometric pore volumes in mesoporous films. Another speculation could come from the inaccessibility of the pores or the fact that the transfer of ions in a confined pore volume impose Na + ions to lose their hydration shell and this indirectly influences on their rapidity and also the number of these ions willing to be transferred at the interface.

V. Nanocomposite films of CNTs / RuO 2 .xH 2 O Investigated by ac-Electrogravimetric Methods

V-1. EQCM study of SWCNTs/RuO 2 .xH 2 O film in aqueous solution

The and V-29f). Indeed, the H + contribution is located in the fourth quadrant but is note really visible due to the small H + mass. In a global point of view, the evolution for species over the total applied potential window could be summarized as following.

For SWCNTs, over the whole potential window, a constant appearance of species is observed:

The H + cation appears at HF (~90 Hz), free solvent molecules are then detected at MF ~ 30 Hz and finally at very LF ~ 0.1Hz anions appear. From 100 mV to 400 mV the instantaneous capacitance of H + cation rises from 2 mF cm -2 and reaches a maximum value of 2.7 mF cm +2 at 400 mV and then, gradually drops to 2 mF cm -2 at 800 mV. For anions the instantaneous capacitance increases slowly from 0.1 mF cm -2 at 100 mV to 0.46 mF cm -2 at 800 mV. For SWCNTs/RuOx.nH2O composite films, H + cations do not appear as fast as in SWCNTs, these species appear at MF with a slight rise from ~8Hz at 100 mV to ~18 Hz at 800 mV. This is followed by the free solvent contribution very close to cations ~10-12 Hz and anions appear again at LF ~0. HO molecules indirectly contribute to the process in both compact and mesoporous RuO2.xH2O films following the same flux direction as the cations which indicates an electrodragging process. Even a slight contribution of SO4 2- ions was detected in the case of mesoporous films. The contribution of the charged species is magnified in mesoporous RuOx.nH2O films compared to the compact counterparts. This qualitative and quantitative study of ionic species contribution in the charge compensation process, together with dynamic information of their interfacial transfer further proves the advantageous nature of RuOx.nH2O structured films for energy applications. The mesoporous RuOx.nH2O film better accommodates both cationic species, H + and H3O + . The H + ions in particular, are transferred quite fast at the mesoporous electrode/electrolyte interfaces, and their concentration profile is significantly higher with respect to the values obtained in their compact analogues. The results of the transfer resistances of the cations are much lower when the RuOx.nH2O films are mesoporous.

In 0.5 M aqueous Na2SO4 solution, the major contribution of the charged species in both compact and mesoporous RuOx.nH2O films corresponds to Na + . However, neither from kinetic parameters (fi vs E, Rst vs E, Capi vs E) nor thermodynamic parameters (Ci-C0 vs E), mesoporous films do not show any advantage. This could be related to the neutral pH of this electrolyte, the most appreciable results of RuOx.nH2O are reported in H2SO4 solution since H + ions could most efficiently interact with available bonds of hydrated RuOx.nH2O electrode. The second hypothesis could be related to a cation size effect and the fact that bigger Na + ions might not be preferable compared to smaller H + ions. Another reason might be related to the inaccessibility of the pores or the fact that the transfer of ions in a confined pore volume impose Na + ions to lose their solvation shell and this indirectly influences on their rapidity.

The second part of this chapter was attributed to an enlarged comparative study between three main different structures. First, three-dimensional composite film of SWCNTs/RuOx.nH2O was elaborated via a simple two-step procedure route and then, bare SWCNTs, bare RuOx.nH2O films were compared. The results of our studies in 0.5 M aqueous H2SO4 electrolyte showed a promoted behaviour for SWCNTs/RuOx.nH2O composite films. This advanced behavior includes: (i) an ameliorated instantaneous capacitance, Capi (ii) Low transfer resistance, Rti and (iii) an amplified number of cations willing to be transferred into the film. This composite

General Conclusion & Perspectives

During this thesis project different types of MOx thin films were studied by means of multiscale time-resolved electrogravimetric methods for the very first time. An attempt was made to improve their electrochemical performance by using a nanostructuration approach in order to procure new morphologies of materials with favorable functionalities.

First, the results of our classical EQCM studies for various morphologies of TiO2 prepared by reactive magnetron RF sputtering showed the advantageous role of the porous structure when compared with less porous and compact analogues. A fine study was then conducted by acelectrogravimetry which proved a better performance of highly porous structures from both kinetic and thermodynamic points of view. While the exact identification of ions and their separation from free solvent molecules could not be achieved by our classical EQCM results, the involvement of different charged and non-charged species participating in the charge compensation process was detected and fairly separated from ac-electrogravimetric results.

Moreover, in a comparison to understand the impact of accompanying solvent (either organic or aqueous) on the targeted parameters, the favorable nature of the aqueous electrolyte was revealed.

The advantageous impact of nanostructuration was also achieved by synthesizing mesoporous WO3 thin films with surfactant assisted electrodeposition method using SDS molecules as porogen. ac-electrogravimetry was used to compare the mesoporous electrode with the compact counterparts. Due to an increased surface area provided by the presence of pores with a diameter of ~ 2-5 nm, it was underlined:

 The participation of anion even slightly as absent in results of dense WO3

 A facilitated transfer of species especially larger charged cationic species,  A larger quantity of charged species which can be stored in the film but also free solvent molecules transferred through the electrode/electrolyte interface.

The same electrochemical route was chosen to produce mesoporous hydrous RuOx.nH2O by using CTAB molecules as an ionic surfactant (~7-10 nm of pore diameter). Again, our acelectrogravimetric results demonstrated the attractive aspect of the mesoporous structure in particular when studied in acidic medium due to the better interaction of small H + ions with the hydrous RuOx.nH2O structure.

 This porous structure showed a high specific capacitance which stands well enough among other values reported in the literature.

 An ameliorated instantaneous capacitance was observed for the involved species.

 Lower transfer resistance of species was observed at the interface of mesoporous electrode/electrolyte.

 An amplified number of cations were willing to be transferred at the interface of this porous film.

In a final step of this project, it was aimed to pursue a similar concept for improving the performance of RuOx.nH2O electrodes by preparing a three-dimensional composite film based on SWCNTs/RuOx structure. A promoted behavior for this new structure was observed from our ac-electrogravimetric results. We observed that this structure benefited both from the high conductivity and large surface area of CNTs but also from the pseudocapacitive character of the thin RuOx.nH2O layers composed of nanometric grains. More precisely,  An ameliorated instantaneous capacitance also lower Rti compared to pure SWCNTs.

 An amplified number of cations willing to be transferred into the film compared to both bare SWCNTs and RuOx.nH2O.

Indeed, the major originality of this work was brought by ac-electrogravimetry as a combined single body technique which allows the study of ions intercalation/electroadsorption phenomena to be performed in situ. This unique methodology permits the exact nature of the transferred ionic species, their dynamics of transfer at the interface as well as effects of ions solvation to be clearly investigated. The use of this combined technique for the characterization of our elaborated metal oxides and particularly its eligibility to underscore the real impact of their nanostructuration was reported for the first time. Therefore,  The establishment of the ac-electrogravimetry characterization in the energy materials domain is significant for designing structurally optimized materials by any other up-todate routes for the next-generation of high energy density supercapacitors.The latter subject of study discussed regarding composite materials could indeed be vastly developed in order to study and to compare the combination of pseudocapacitive metal oxides with CNTs.

 Another interesting category of insertion materials, namely ''Layered Double Hydroxides (LDHs)'' were developed in a first step by our EQCM studies on the thin films of Ni2Al-NO3 and Co2Al-NO3 showed very promising results, the combination of LDHs with CNTs or even their sole study by ac-electrogravimetry remains as another original perspective to achieve.The comparison brought to discussion in the third chapter regarding the impact accompanying solvent (whether it is aqueous or organic) could be effectively expanded to a larger window for study by including ionic liquids to this comparison.